Upload
others
View
1
Download
0
Embed Size (px)
Citation preview
A111D2 14bD5b
NAT'L INST OF
A111021 46056
NBS
PUBLICATIONS
I v : : :* :•
!
J, ; >.
i
;
v
t i r t » * f.
i
?w &? * f 4 ?i ? >t»twm 5 i W «il >2 > * i
.
r. • ; f rrx: :• •:sn>ri r in; ? •• t
$
f 5n ? * f\ p ? •/? s ujuirxs) •«»': ts xrnm'ivtj:
UNITED STATES DEPARTMENT OF COMMERCE
C. R. Smith, Secretary
UNATIONAL BUREAU OF STANDARDS • A. V. Astin, Director
Molten Salts: Volume 1, Electrical Conductance,
Density, and Viscosity Data
G. J. Janz,* F. W. Dampier,* G. R. Lakshminarayanan,*
P. K. Lorenz,* and R. P. T. Tomkins*
*This report was prepared under contract at the Molten Salts Data Center
Rensselaer Polytechnic Institute, Troy, N.Y. 12180
NSRDSNBS 15
National Standard Reference Data Series
National Bureau of Standards 15
Issued October 1968
For sale by the Superintendent of Documents, U.S. Government Printing Office
Washington, D.C. 20402  Price S3.00
National
NOV 2 9 1968
142552Q1IOO\)^i
No  /i>
/6
Library of Congress Catalog Card Number: 6860051
Foreword
The National Standard Reference Data System is a Governmentwide effort to provide for
the technical community of the United States effective access to the quantitative data of physical
science, critically evaluated and compiled for convenience, and readily accessible through a
variety of distribution channels. The System was established in 1963 by action of the President’s
Office of Science and Technology and the Federal Council for Science and Technology.
The responsibility to administer the System was assigned to the National Bureau of Standards
and an Office of Standard Reference Data was set up at the Bureau for this purpose. Since 1963,
this Office has developed systematic plans for meeting highpriority needs for reliable reference
data. It has undertaken to coordinate and integrate existing data evaluation and compilation
activities (primarily those under sponsorship of Federal agencies) into a comprehensive program,
supplementing and expanding technical coverage when necessary, establishing and maintaining
standards for the output of the participating groups, and providing mechanisms for the dissemina
tion of the output as required.
The System now comprises a complex of data centers and other activities, carried on in Gov
ernment agencies, academic institutions, and nongovernmental laboratories. The independent
operational status of existing critical data projects is maintained and encouraged. Data centers
that are components of the NSRDS produce compilations of critically evaluated data, critical re
views of the state of quantitative knowledge in specialized areas, and computations of useful
functions derived from standard reference data. In addition, the centers and projects establish
criteria for evaluation and compilation of data and make recommendations on needed modifications
or extensions of experimental techniques.
Data publications of the NSRDS take a variety of physical forms, including books, pamphlets,
looseleaf sheets and computer tapes. While most of the compilations have been issued by the
Government Printing Office, several have appeared in scientific journals. Under some circum
stances, private publishing houses are regarded as appropriate primary dissemination mechanisms.
The technical scope of the NSRDS is indicated by the principal categories of data compilation
projects now active or being planned: nuclear properties, atomic and molecular properties, solid
state properties, thermodynamic and transport properties, chemical kinetics, colloid and surface
properties, and mechanical properties.
An important aspect of the NSRDS is the advice and planning assistance which the National
Research Council of the National Academy of SciencesNational Academy of Engineering provides.
These services are organized under an overall Review Committee which considers the program as a
whole and makes recommendations on policy, longterm planning, and international collaboration.
Advisory Panels, each concerned with a single technical area, meet regularly to examine major
portions of the program, assign relative priorities, and identify specific key problems in need of
further attention. For selected specific topics, the Advisory Panels sponsor subpanels which
make detailed studies of users’ needs, the present state of knowledge, and existing data resources
as a basis for recommending one or more data compilation activities. This assembly of advisory
services contributed greatly to the guidance of NSRDS activities.
The NSRDSNBS series of publications is intended primarily to include evaluated reference
data and critical reviews of longterm interest to the scientific and technical community.
A. V. Astin, Director
hi
Preface
This work was undertaken to meet the need for a critical assessment of the existing data for
electrical conductance, density and viscosity of inorganic compounds in the molten state. The
scope embraces the publications in the scientific literature to the current date (December, 1966):
while care was taken to be comprehensive, it is clear that there will be omissions and that the task
is therefore one to be continued and extended.
The results for some 174 compounds as singlesalt melts are reported: no attempt was madein the present effort to embrace the results for molten salt mixtures. With the exception of quater
nary ammonium salts, an anion classification has been used for the presentation of the data: i.e..
Fluorides, Chlorides, Bromides, Iodides, Carbonates, Nitrites, Nitrates, Oxides, Sulfides, Sulfates,
and Miscellaneous.
The authors will be pleased to have additional studies directed to their attention.
Acknowledgments
This work was made possible in large part by financial support received from the Office of
Standard Reference Data, National Bureau of Standards, Washington, D.C., for the compilation
and critical evaluation of published literature in the general field of molten salts. The participation
of A. T. Ward and R. D. Reeves in the first stages of this work, and the assistance of A. G. Timidei,
and C. G. M. Dijkhuis in the preparation of the final copy are acknowledged with pleasure.
IV
Contents
Page
Foreword iii
Preface iv
Acknowledgments iv
1. Introduction
2. Symbols and units
.3. Preparation of tables 1
4. Estimation of uncertainty 2
5. Discussion 2
Lithium fluoride 2
Sodium fluoride 3
Potassium fluoride 3
Cesium fluoride 3
Beryllium fluoride 3
Magnesium fluoride, calcium fluoride, strontium
fluoride, barium fluoride, lanthanum (II) fluoride,
and cerium (III) fluoride 4
Thorium (IV) fluoride and uranium (IV) fluoride 4
Manganese fluoride, copper (II) fluoride, silver
fluoride, zinc fluoride, and lead fluoride 4
Lithium chloride 4
Sodium chloride 4
Potassium chloride 5
Rubidium chloride 6
Cesium chloride 6
Beryllium chloride 6
Magnesium chloride 6
Calcium chloride 7
Strontium chloride 7
Barium chloride 7
Scandium (III) chloride 8
Yttrium (III) chloride 8
Lanthanum (III) chloride 8
Cerium (III) chloride 8
Praseodymium (III) chloride 8
Neodymium (III) chloride 9
Gadolinium (III) chloride 9
Dysprosium (II) chloride, holmium (III) chloride,
and erbium (III) chloride 9
Thorium (IV) chloride 9
Uranium (IV) chloride 9
Manganese (II) chloride 9
Titanium (IV) chloride 9
Copper (I) chloride 9
Silver chloride 10
Zinc chloride 10
Cadmium chloride 11
Mercury (I) chloride 11
Mercury (II) chloride 11
Alumium (III) chloride 11
Gallium (III) chloride 12
Indium chloride 12
Indium (II) chloride 12
Indium (III) chloride 12
Thallium (I) chloride 12
Tin (II) chloride 12
Tin (IV) chloride 13
Lead (II) chloride 13
Bismuth (III) chloride 13
Tellurium (II) chloride 13
Tellurium (IV) chloride 13
Lithium bromide 14
Sodium bromide 14
Potassium bromide 14
Rubidium bromide 15
Page
Cesium bromide 15
Magnesium bromide 15
Calcium bromide 15
Strontium bromide 15
Barium bromide 16Lanthanum (III) bromide 16Praseodymium (III) bromide 16Neodymium (III) bromide 16Gadolinium (III) bromide 16
Copper (I) bromide 16Silver bromide 16Zinc bromide 17
Cadmium bromide 17
Mercury (II) bromide 17
Aluminum bromide 18
Indium (III) bromide 18
Thallium (I) bromide 18
Lead (II) bromide 18
Bismuth (III) bromide 18
Lithium iodide 19
Sodium iodide 19
Potassium iodide 19
Rubidium iodide 20
Cesium iodide 20Magnesium iodide 20
Calcium iodide 20
Strontium' iodide 20
Barium iodide 21
Aluminum (III) iodide 21
Lanthanum (III) iodide, cerium (III) iodide, prase
odymium (III) iodide, and neodymium (111)
iodide 21
Silver iodide 21
Zinc iodide 21
Cadmium iodide 22Mercury (II) iodide 22Gallium (II) iodide 22
Indium (III) iodide 22
Thallium (I) iodide 23
Lead (II) iodide 23
Bismuth (III) iodide 23
Lithium carbonate 23
Sodium carbonate 23
Potassium carbonate 23
Lithium nitrite 24
Sodium nitrite 24
Potassium nitrite 24
Rubidium nitrite 25
Cesium nitrite 25
Barium nitrite 25Lithium nitrate 25
Sodium nitrate 25
Potassium nitrate 26
Rubidium nitrate 27
Cesium nitrate 28Silver nitrate 28
Thallium (I) nitrate . 28
Vanadium pentoxide and chromium trioxide.. 29
Molybdenum trioxide 29
Wiistite (Feo. 9sO) 29
Boron oxide 29
Silicon dioxide 29
Germanium dioxide 30
Lead oxide 30
V
PagePage
Arsenic trioxide 30
Antimony sesquioxide, bismuth sesquioxide, andtellurium dioxide 30
Iron (II) sulfide 30
Cobalt (II) sulfide 30
Nickel (II) sulfide 31
Copper (I) sulfide 31
Silver sulfide 31
Germanium (II) sulfide 31
Tin (II) sulfide 31
Lead sulfide 31
Antimony (III) sulfide 31
Bismuth (III) sulfide 31
Lithium sulfate 32
Sodium sulfate 32
Potassium sulfate 32
Rubidium sulfate 32
Cesium sulfate 32
Silver sulfate 33
Tetrapropylammonium tetrafluoroborate 33
Tetrapropylammonium hexafluorophosphate 33
Tetrapropylammonium tetraphenylborate 33
Tetrabutylammonium bromide 33
Tetrabutylammonium iodide 33
Tetrabutylammonium tetrafiuoroborate 34
Tetrabutylammonium hexafluorophosphate 34
Tetrabutylammonium tetraphenylborate 34
Tetrahexylammonium tetrafluoroborate 34
Tetranamylammonium thiocyanate 34
Lithium molybdate 35
Sodium molybdate 35
Potassium molybdate 35Sodium tungstate 35Potassium tungstate 35Sodium thiocyanate' 35Potassium thiocyanate 35Sodium hydroxide 36Potassium hydroxide 36Potassium dichromate 36Sodium metaphosphate 36Uranyl chloride 36Lithium hydride 36Lithium chlorate 37Lithium perchlorate 37
List of tables 1 to 174 39
6. Numerical values of electrical conductance, density,
and viscosity 427. Cumulative tables of temperature dependent equa
tions 108
Table 175. Specific conductancebest equations... 109Table 176. Densitybest equations 114Table 177. Equivalent conductance 117Table 178. Viscositybest equations 120Table 179. Specific conductanceexponential equa
tions 122Table 180. Specific conductancepower series equa
tions 126Table 181. Viscosityexponential equations 131Table 182. Viscositypower series equations 133
8. References 1359. Additional data sources 137
10.
Compound index 138
VI
Molten Salts: Volume 1, Electrical Conductance, Density, and Viscosity Data
G. J. Janz, F. W. Dampier, G. R. Lakshminarayanan, P. K. Lorenz, and R. P. T. Tomkins
Data on the electrical conductance, density and viscosity of singlesalt melts were compiled froma comprehensive search of the literature up to December 1966 and a critical assessment made of
the compiled data. Recommended values were determined and are presented as functions of temperature in the form of equations and tables.
The results for some 174 compounds as singlesalt melts are reported; no attempt was made in
the present effort to embrace the results for molten salt mixtures. Data are presented for fluorides,
chlorides, bromides, iodides, carbonates, nitrites, nitrates, oxides, sulfides, sulfates, and a miscel
laneous group.
Key Words: Data compilation, density, electrical conductance, molten salts, standard referencedata, viscosity.
1.
Introduction
The critical assessment of the electrical con
ductance, viscosity, and density data of inorganic
compounds in the molten state (i.e., “singlesalt
melts”) was undertaken to meet the need for
consistent sets of values for these properties.
With the exception of quaternary ammoniumslats, an anion classification has been used in this
compilation: i.e.. Fluorides, Chlorides, Bromides,Iodides, Carbonates, Nitrites, Nitrates, Oxides,
Sulfides, Sulfates, and additional salts given as
Miscellaneous. The order within each anionic
group is in the list of tables preceding section 6.
Results are reported for some 174 compounds.
2.
Symbols and Units
The equations used to express the temperaturedependence of density, conductance, and viscosity
are as follows:
Density: Equivalent conductance:
p — a — bT A= A Ae~EA/RT
Specific conductance:
k= a + bT
k= a + bT+ cT1
k = a + bT+ cT2 + dTs
Viscosity:
r1=A v
EJHT
rj = a + bT+ cT2
p = a + bT+ cT2 + dT*
The symbols and units are:
J = joule
cal = thermochemical calorie = 4. 1840JT(°K)= temperature in degrees Kelvin, defined in
the thermodynamic scale by assigning273.16 °K to the triple point of water (freez
ing point, 273.15 °K = 0 °C).
R = gas constant = 1.98717 calmol 1 deg 1
= 8.3143 J mol 1 deg 1
A = equivalent conductance (ohm"'cm equiv 1)
A\= 'm ohm 1 cm 2 equiv 1
Ea = in cal mol 1
k= specific conductance (ohm 1 cm 1)
p = density (g cm 3)
7] = viscosity (cp)
Av = in cpEv = in cal mol 1
.
3.
Preparation of Tables
The selection of the best values of the data for
the calculations was based on consideration of
different factors, such as: experimental techniques,
the number of measurements, the temperaturerange, the deviations of the data from a fitted curve,
and the reliability of previous work from any onecenter. In general the data of each investigation
were evaluated by fitting linear, quadratic andexponential equations by the method of least
squares; usually the equation with the smallest
standard deviation was selected as the best equation. In some cases, however, the data from several
laboratories have been combined for the precedinganalysis (see: discussions of the individual salts
(sec. 5)).
The literature references are given as footnotes
in these tables. Where only one reference is under
scored the data from that investigation has beenused to gain the best values. Where more than onereference is underlined, the data from these sourceswere combined as reported in section 5, to gain
the best values. The tabulated bestvalues of
specific conductance, density, and viscosity, werecalculated using the equations listed with eachtable (sec. 6).
Equivalent Conductance— The equivalent con
ductance of a singlesalt melt is defined by the
, .. A(Equivalent Weight) ^ x ^ j
relation: A —
k
. 1 he tabulatedP
1
values of specific conductance and density wereused to gain the values of A (sec. 6), and the latter,
to develop the exponential equations for equivalentconductance.
Melting Points — The melting point reference is
listed at the bottom of each table together with the
references for density, conductance and viscosity
(sec. 6). In some cases (e.g., Mgl2 , Gal2 ) the melting
point could only be indicated as less than a certain
temperature since the actual melting point was not
stated in the investigation (the lowest temperatureat which measurements were made on the liquid
melt).
Extrapolation Beyond the Experimental Temperature Limits — To calculate equivalent conductanceover the corresponding temperature range for whichspecific conductance data were reported, extrapo
lation of the density data was necessary in somecases. When this extrapolation exceeded a temperature range greater than 20°, the values are enclosedin brackets (sec. 6).
Estimation of Precision —(i) Definitions: The standard deviation was com
puted by the expression:
S(A C A C )2
n—p
where Xe and Xc are the experimental and calculated
values (from least squares equations), respectively,
for each temperature, n the number of data points,
and p the number of coefficients. The standarddeviation, s, is used as the index of precision (sec. 7).
The percent precision (P.P.) is defined by:
P.P. =x 100
where Z is the value of the physical property at the
“midpoint temperature” (i.e., the midpoint of the
temperature range over which the physical propertyhas been investigated). Thus, for LiCl the percentprecision would be simply
[0.00074 X 102/6.215] = 0.012 percent.
Here 6.215 is the value of k at 980 °K (temperaturelimits, 910 to 1050 °K; refer. Table 19, sec. 6).
The percent precision values, stated in brackets,normally follow immediately the precision valuese.g., 5 = 0.00074 (0.012%) for LiCl. The units for
precision are those of the physical property beingconsidered.
(ii) Computations: All computations were ef
fected with the digital computer facilities at Rensselaer Polytechnic Institute and Fortran IV programs.The calculations with the quadratic equations, in
the majority of the cases, were taken to eight signifi
cant figures; the calculations with the exponentialand cubic equations, similarly to 14 significant fig
ures. The coefficients of these equations are statedto more significant figures than is justified by theaccuracy in order that the equations may be used to
gain values within the limits of the precision of
the measurements.
4. Estimation of Uncertainty
Estimates of uncertainty were based primarily oncomparisons of the departures of the experimentalresults from the best values. Where this was im
possible, the estimate of uncertainty was guided bymore qualitative factors. In all cases, considerationwas also given to experimental techniques andprevious results from the respective laboratories.
The precision (i.e., the standard deviation was animportant consideration throughout this part of
the work.The Percent Departure (P.D.) is defined by:
P.D.Experimental Value — Tabulated Value
Tabulated Value100
and has been used to compare the results of different
investigators with the best values (sec. 6). ThePercent Departure analysis for three salts, KC1,NaNCG, and KNO3 is illustrated in figures 1 to 3
respectively (sec. 5).
Where an uncertainty statement is bracketed,the brackets indicate that the estimate has beenbased on minimal information.
5. Discussion
In this section the following information is givenfor each compound: precision, estimated uncertain
ty, source of the temperature dependent equation,and the departure values. For the data used to gain
the best equation, the details given are as follows:
literature reference, temperature range, number of
data points, and (for viscosity only) the experimentaltechnique. The maximum percent departure hasalso been given, where possible (e.g., KC1 (fig. 1):
the maximum percent departure between the values
of van Artsdalen [79]1 and Winterhager [85] is
1.24(1112The uncertainty statements in brackets, being
based on minimal information, are more qualitative
than the unbracketed values.
Lithium Fluoride
[Refer: Table 1, p. 42, for numerical values]
Four investigations of the specific conductancefor molten LiF have been reported [42. 83, 86, 88],
Compared to the data of Winterhager and Werner[86] the results of van Artsdalen and Yaffe [83],and Yim and Feinleib [88] show maximum depart
ures of 14.7 percent (1140 °K) and —4.1 percent
(1173 °K) respectively; the results of Ryschkewitsch
[42] show larger departures. It has been suggested
[198] that some experimental factors (e.g., possibly
1 Figures in brackets indicate the literature references on page 135.
2
a distortion of the potential probe arrangement) led
to systematically high values in the van Artsdalenmeasurements. The work of Winterhager andWerner [86] appears the most thorough; their
data (1148.2 to 1310 °K, 9 points) were selected.
Using the quadratic equation for specific conductance the precision is 5 = 0.0237 (0.264%). The un
certainty of the specific conductance values is
estimated to be about 12 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.303 (0.23%).
Three density studies have been reported [25,
81, 83]. The estimated uncertainty of the density
values, based on the van Artsdalen studies [83], is
0.5 percent. The maximum departure between the
densities of van Artsdalen and Jaeger [25] is 0.5
percent (1141.7 °K). The studies of Schinke ~ndSauerwald [81] were to establish the volume changeon fusion.
Sodium Fluoride
[Refer: Table 2, p. 42, for numerical values]
Five investigations of the specific conductance for
molten NaF have been reported [31, 46, 67, 86, 88].
The tabulated values were calculated from the data
of Winterhager and Werner [86] (1276.2 to 1411.2 °K,
8 points). Using the linear equation for specific
conductance the precision is 5 = 0.0089 (0.17%). Themaximum departure between the data of Winter
hager [86] and Yim and Feinleib [88] is 3.1 percent
(1270 °K). The uncertainty of the specific conduc
tance values is estimated to be about 3.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.119 (0.10%).
Of the two density investigations [25, 31], the
results of Jaeger [25] were selected to generate
the tabulated values; the information was insufficient
for an estimate of accuracy.
Potassium Fluoride
[Refer: Table 3, p. 43, for numerical values]
Eight investigations of the specific conductancefor molten KF have been reported [26, 31, 42, 73,
83, 86, 88, 198]. The tabulated values were calcu
lated from the data of Winterhager and Werner[86] (1132.2 to 1285.2 °K, 12 points). Using thelinear equation for specific conductance the pre
cision is 5 = 0.0201 (0.526%). The study of specific
conductance for KF by Bredig and Bronstein [198]was limited to one temperature (1178.2 °K). Comparison of this value (3.77 11
_1 cm 1) with that of
Winterhager and Werner shows the departure to
be 1.85 percent. The results of the other investi
gators show larger departures. The uncertainty of
the specific conductance values is estimated to beabout 12 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.188 (0.16%).
Of the three density studies [26, 81,83], the in
vestigation of van Artsdalen [83] appears mostthorough. The maximum departure between the
density data of van Artsdalen and Jaeger andKapma [26] is 0.9 percent (1140 °K). The study of
Schinke and Sauerwald [81] were to establish the
volume change on fusion. The uncertainty of the
density values is judged to be about 0.6 percent.
Cesium Fluoride
[Refer: Table 4, p. 43, for numerical values]
Two investigations of the specific conductancefor molten CsF have been reported [182, 83]. Thetabulated values were calculated from the data of
Bronstein, Dworkin, and Bredig [182] (1010.2 to
1125.2 °K, 6 points). Using the linear equation for
specific conductance the precision is 5 = 0.0456
(1.73%). The maximum departure between the
results of Bredig [182] and Yaffe and van Arts
dalen [83] is 34 percent (1050 °K). The uncertainty
of the specific conductance values is estimated to
be about 5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.118(0.097%).Of the two density studies [25, 83], the data of
van Artsdalen [83] were selected to calculate the
tabulated values. The maximum departure betweenthe densities reported by Jaeger [25] and van Arts
dalen [83] is 1.1 percent (1041.9 °K). The uncer
tainty of the density values is judged to be about
0.8 percent.
Beryllium Fluoride
[Refer: Table 5, p. 44, for numerical values]
The tabulated values of specific conductance for
molten BeF2 were obtained from the data of Mackenzie [143] (973 to 1173 °K, 6 points). Since the
least squaring to quadratic, cubic and exponential
equations was unsatisfactory, the values weregained graphically. No attempt to estimate the
accuracy of the specific conductance values wasmade.Two investigations of the viscosity have been
reported [143, 225]. The tabulated values werecalculated from the data of Moynihan and Cantor
[225] (846.9 to 1252.2 °K, 25 points, rotating cylinder
viscometer). The exponential equation expresses
the data of Moynihan and Cantor with a precision
5 = 3.08X 10 6 (2.77%). The uncertainty of the
viscosity values is judged to be about 3.0 percent.
The viscosities of the second study (Mackenzie
[143], restricted falling ball technique), show de
partures of about 8.0 percent from those of Moynihanand Cantor.
3
Magnesium Fluoride, Caleium Fluoride,Strontium Fluoride, Barium Fluoride,Lanthanum (III) Fluoride, and Cerium(III) Fluoride
[Refer: Tables 6 to 11, pp. 44 to 45, for numericalvalues]
The tabulated values of density for molten MgF2 ,
CaF2 , SrF2 ,BaF2 , LaF3 ,
and CeF3 were calculated
from the data of Kirshenbaum, Cahill, and Stokes
[95]. The maximum departure between the den
sity values of Mashovetz [197] and Kirshenbaum[95] is 0.4 percent for CaF2 . The uncertainty of
density values is estimated to be about 0.5 percentfor CaF2 and (1.0%) for the other five fluorides.
Thorium (IY) Fluoride and Uranium (IV)
Fluoride
[Refer: Tables 12 and 13, p. 46, for numerical values]
The tabulated values of density for molten ThF4
and UF4 were calculated from the data of Kirshen
baum and Cahill [167]. The uncertainty of the
density values is estimated to be about (1%).
Manganese Fluoride, Copper (II) Fluoride,Silver Fluoride, Zinc Fluoride, and LeadFluoride
[Refer: Tables 14 to 18, pp. 46 to 47]
The tabulated values of the specific conductancesfor molten MnF2 ,
CuF2 , AgF, ZnF2 ,and PbF2 were
calculated from the graphical data of Winterhagerand Werner [86], The number of data points inter
polated from the Winterhager graphs, the cor
responding temperature ranges and the best equa
tion are as follows:
MnF2 4 points, 1223—1273 °K, linear equationCuF2 6 points, 12331370 °K, linear equationAgF 6 points, 773—923 °K, linear equationZnF2 4 points, 11731223 °K, linear equationPbF2 7 points, 11231273 °K, linear equation.
The uncertainty of the specific conductancevalues is estimated to be about (20%).
Lithium Chloride
[Refer: Table 19, p. 47, for numerical values]
Nine investigations of the specific conductancefor molten LiCl have been reported [33, 42, 44,
45, 55, 62, 66, 79, 85]. The specific conductancevalues of van Artsdalen and Yaffe [79] (917.1 to
1056.5 °K; 7 of the 9 reported temperatures omitting
896.0 and 907.6 °K) and two values from Edwards[62] (920.2 and 940.2 °K) were used to develop the
quadratic equation. Using the quadratic equation
for specific conductance the precision is 5 = 0.00074(0.012%). The maximum percent departures of the
specific conductance values of various investi
gators from the combined data of van Artsdalen
[79] and Edwards et al. [62] , are as follows: Bloomet al. [66], 3.2 (910 °K); Biltz and Klemm [33], 0.8
(954.2 °K); Grothe [55], 0.3 (973.2 °K): Winterhager and Werner [85], —0.7 (961.2 °K) and Kar
pachev et al. [44], —3.0 (910 °K). The results of
Ryschkewitsch [42] show larger departures. Theuncertainty of the specific conductance values is
estimated to be about 0.7 percent. Considerablecorrosion of the cell (above 1056 °K) was noted byvan Artsdalen.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0847 (0.048%).
Of the seven sets of density data [3, 25, 55, 62,
66, 79, 81] the most thorough studies appear to bethose of van Artsdalen [79] and Bloom [66]. Theuncertainty of the tabulated densities, calculated
from the van Artsdalen data [79] is estimated to
be about 0.2 percent. Compared to the density data
of van Artsdalen, the results of Bloom et al. [66]
,
Brunner [3], Edwards et al. [62], Jaeger [25] andGrothe [55] show maximum departures of 0.2 per
cent (900 °K), —0.2 percent (1050 °K). —0.3 percent
(1050 °K), —0.4 percent (913 °K) and —0.4 percent
(1050 °K) respectively.
Four sets of viscosity data have been reported
[12, 45, 47, 121]. The tabulated values of vis
cosity were calculated from the data of Murgulescuand Zuca [121] (902.9 to 1082.9 °K, 11 points, oscil
lating ball technique). The cubic equation expresses
the data of Murgulescu and Zuca with a precision
5 = 0.0092 (0.81%). The uncertainty of the vis
cosity values is estimated to be about 1.0 percent.
The investigator, reference, experimental method,and the maximum percent deviation from the values
of Murgulescu and Zuca are as follows: Fawsitt
[12], oscillating disk, +21.7 percent: Karpachev
[45], oscillating ball. 200 percent; and Karpachev
[47], oscillating ball, 7.4 percent. No explanation
for the two vastly different results was offered by
Karpachev.
Sodium Chloride
[Refer: Table 20, p. 48, for numerical values]
Seventeen investigations of the specific conduct
ance for molten NaCl have been reported [2, 4,
10, 27, 33, 42, 49, 52, 55, 62, 63, 71, 79, 82, 85,
199], The specific conductance data of van Arts
dalen and Yaffe [79] (1079.6 to 1294.6 °K, 24 of the
26 reported temperatures, omitting 1075.5 and1077.8 °K) were used to develop the tabulated val
ues. Using the quadratic equation for specific con
ductance the precision is 5 = 0.00164 (0.043%).
Compared to the data of van Artsdalen the results
of Ryschkewitsch [42], and Edwards et al. [62],
show maximum departures of —0.6 percent (1093
°K) and 0.8 percent (1273 °K) respectively; the
4
results of the other investigators show larger
departures. The estimated uncertainty of the spe
cific conductance values is about 0.8 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0870 (0.057%).
Of the eleven density studies [3, 11, 25, 55,
62, 66, 79, 80, 81, 96, 126] the most thorough ap
pears to be that of van Artsdalen [79]. Comparedto the density data of van Artsdalen [79] the results
of Brunner [3], Edwards et al. [62] and Kirshen
baum [126] show departures of —0.2 percent
(1080 °K), —0.4 percent (1111 °K) and 0.6 percent
(1290 °K) respectively; the results of Bloom et al.
[66] and Jaeger [25] show larger departures. Thestudies of Sauerwald et al. [80, 81] and Bockris
et al. [96] were to establish the volume change onfusion. The uncertainty of the tabulated densities,
calculated from van Artsdalen data is estimated to
be about 0.4 percent.
Four investigations of the viscosity have beenreported [12, 38, 57, 121]. The tabulated values of
viscosity were calculated from the data of Murgulescu and Zuca [121] (1085.9 to 1243.2 °K, 11 points,
oscillating ball technique). The cubic equation ex
presses the data of Murgulescu and Zuca with a
precision 5 = 0.0057 (0.55%). The uncertainty of
the viscosity values is estimated to be about 1.0
percent.
The investigator, reference, experimental method,and the maximum percent departure from the valuesof Murgulescu and Zuca are as follows: Fawsitt
[12], oscillating disk, 4.30 percent; Dantuma [38],oscillating ball, 8.4 percent; Ogawa [57], restricted
falling sphere, 7.2 percent.
Potassium Chloride
[Refer: Table 21, p. 48, for numerical values]
Nineteen investigations of the specific conductance for molten KC1 have been reported [2, 4, 10,
26, 27, 42, 44, 49, 50, 55, 62, 63, 66, 79, 85, 123,
124, 125, 129], The departures of recent deter
minations from the values of van Artsdalen [79] are
illustrated in figure 1. The tabulated values werecalculated from the data of van Artsdalen and Yaffe
[79] (1063.2 to 1198.3 °K, 15 points). Using thequadratic equation for specific conductance theprecision is 5 = 0.003 (0.14%). The departure be
tween the data of van Artsdalen and Crook andBockris [123] is about 0.4 percent over the range1053.2 to 1198.2 °K. Van Artsdalen [79] andCrook [123] both used well established ac conductance techniques (0.5 to 20 kc/sec); the results
of Duke [124] were gained with a dc technique. Theresults of Buckle and Tsaoussoglou [125a], gainedwith a new ac technique (10 to 100 kc/sec) arelower than the van Artsdalen data by about 0.8
percent. The results of the other investigators showlarger departures. The uncertainty of the specific
FIGURE 1. Comparison of percent departure of the data ofvarious investigators with the van Artsdalen specific conduct
ance data for KC1.
o Base line— van Artsdalen and Yaffe [79]
V Huber and Potter [63]
o Edwards and Taylor [62]
A Crook [123]a Duke and Bissell [124]
^ Winterhager and Werner [85]
0 Bloom and Knaggs [66]
<=> Murgulescu and Zuca [129]
Q Buckle and Tsaoussoglou [125]
conductance values is estimated to be about 0.6
percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.109 (0.092%).
The density of molten KC1 has been the subject
of more than ten investigations [3, 11, 26, 62, 66, 70,
79, 80, 81, 126, 178]. The uncertainty of the tabulated
density values, calculated from the van Artsdalen
data [79] is estimated to be about 0.5 percent. Thedensity data of Kirshenbaum [126], p = 2.0625.350 10 4 T °K (1101 to 1607 °K), extends to
higher temperatures than any of the other investiga
tions; at 1100 °K, the Kirshenbaum data are about
1.45 percent lower than the van Artsdalen values.
The maximum percent departure between the den
sities of van Artsdalen [79] and the other investi
gators are as follows: Brunner [3], —0.2 (1080 °K);
Arndt and Gessler [11], — 1.1 (1123 °K); Jaeger andKapma [26], —0.14 (1130 °K); Edwards et al. [62],
0.4' (1060 °K); Bloom et al. [66], 0.5 (1063 °K); Peakeand Bothwell [70], —0.7 (1170 °K); Neithamer andPeak [178], —0.6 (1178 °K). The studies of Vogel,
Schinke, and Sauerwald [80] and Schinke and Sauer
wald [81] were to establish the volume change onfusion.
Three investigations of the viscosity for moltenKC1 have been reported [12, 102, 111]. The tabulated
values of viscosity were calculated from the data of
Murgulescu and Zuca [102] (1056.5 to 1202.0 °K, 11
points, oscillating ball techinque). The cubic equa
tion expresses the data of Murgulescu and Zucawith a precision 5 = 0.0132 (1.43%). The uncertainty
of the viscosity values is estimated to be about 1.5
percent.
5
The investigator, references, experimental method, and the maximum percent departure from the
values of Murgulescu and Zuca are as follows:
Fawsitt [12], oscillating disk, 25 percent; andKarpachev and Stromberg [111], oscillating ball,
5.2 percent.
Rubidium Chloride
[Refer: Table 22, p. 49, for numerical values]
Three investigations of specific conductance for
molten RbCl have been reported [33, 82, 129]. Thetabulated values were calculated from the data of
van Artsdalen and Yaffe [82] (1003.0 to 1197.3 °K,
11 points). Using the quadratic equation for specific
conductance the precision is 5 = 0.0026 (0.15%).
Compared to the data of van Artsdalen [82], the
results of Murgulescu and Zuca [129] and Klemm[33] show departures of 3.18 percent (1140 °K) and6.03 percent (1188.2 °K) respectively. The uncertainty of the specific conductance values is es
timated to be about 3.5 percent.
The tabulated values of equivalent conductanceare expressed by the exponential equation with a
precision 5 = 0.192 (0.19%).
Of the four density studies [25, 35, 36, 82] the
most thorough appears to be that of van Artsdalen
[82]. Compared to the data of van Artsdalen theresults of Klemm [36], and Biltz [35] show maximumdepartures of —0.8 percent (1055 °K), and 0.3 per
cent (1200 °K) respectively. The uncertainty of the
tabulated density values calculated from the vanArtsdalen data [82] is estimated to be about 0.4
percent.
Two investigations of viscosity have been reported
[109, 121]. The tabulated values were calculated
from the data of Murgulescu and Zuca [121] (1005.2
to 1148.2 °K, 11 points, oscillating ball technique).
The cubic equation expresses the data of Murgulescu and Zuca with a precision 5 = 0.0058 (0.50%).
The uncertainty of the viscosity values is estimatedto be about 1.0 percent.
The viscosities of the second study (Janz andReeves [109], oscillating hollow cylinder technique)are consistently higher than those of Murgulescuand Zuca (e.g., 53.5% at 1010 °K, 9.9% at 1140 °K).
Cesium Chloride
[Refer: Table 23, p. 49, for numerical values]
Four investigations of the specific conductancefor molten CsCl have been reported [33, 82, 129,
199], The tabulated values were calculated from the
data of van Artsdalen and Yaffe [82] (926.5 to 1170.0°K, 11 points). Using the quadratic equation for
specific conductance the precision is 5=0.00280(0.18%).
The maximum departure between the specific
conductance values of van Artsdalen [82] and Biltz
and Klemm [33] is 10.6 percent (1104.2 °K). The
uncertainty of the tabulated specific conductancevalues is estimated to be about 5.0 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
of 5 = 0.2520 (0.26%).
Five density studies have been reported [25, 59,
80, 81, 82]: of these the most thorough appears to
be that of van Artsdalen [82]. The uncertainty of thedensity values calculated from the van Artsdalendata [82] is estimated to be about 0.1 percent.The accuracy of the density measurements for
CsCl is greater than the accuracies for any of theother molten salts; these data appear highly suitable
for high temperature calibration reference stand
ards. The maximum departure between the densitydata of Jaeger [25] and van Artsdalen [82] is 0.12
percent (1154.2 °K).
Two investigations of viscosity have been reported
[109, 121]. The tabulated values were calculated
from the data of Murgulescu and Zuca [121] (928.0
to 1110.2 °K, 11 points, oscillating ball technique).
The cubic equation expresses the data of Murgulescu and Zuca with a precision 5 = 0.0067 (0.82%).
The uncertainty of the viscosity values is estimatedto be about 1.0 percent.
The viscosities of the second study (Janz andReeves [109], oscillating hollow cylinder techinque)
show a linear “crossover” departure from those of
Murgulescu and Zuca (e.g., 13.3% at 940 °K; 18.8%at 1110 °K).
Beryllium (II) Chloride
[Refer: Table 24, p. 50, for numerical values]
Two investigations of the specific conductance for
molten BeCh have been reported [32, 186]. Thetabulated values were calculated from the data of
Delimarskii, Sheiko, and Feshchenko [186] (718.2
to 761.2 °K, 5 points). Using the linear equation for
specific conductance the precision is 5 = 9.70 • 10 °
(3.3%). Comparison of the data of Delimarskii [186]
and Voigt and Biltz [32] shows that the values of
Delimarskii are considerably lower, the mazimumdeparture being 180 percent (718.2 °K). The uncer
tainty of the specific conductance values is esti
mated to be about (50%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0169 (21.6%).
The density data of Klemm [36] were used to
calculate the tabulated values; no estimate of accu
racy was attempted owing to the limited information.
Magnesium Chloride
[Refer: Table 25, p. 50, for numerical values]
Three investigations of the specific conductancefor molten MgCf> have been reported [35, 63, 94].
The tabulated values were calculated from the dataof Bockris et al. [94] (987.2 to 1252.1 °K. 27 points).
6
Using the quadratic equation for specific conduc
tance the precision is 5 = 0.00300 (0.24%). Compared to the data of Bockris et al., the results of
Biltz and Klemm [35] and Huber, Potter, and Clair
[56] show maximum departures of— 1.1 percent
(1214 °K) and — 1.6 percent (1111 °K) respectively.
The uncertainty of the tabulated specific conduc
tance values is estimated to be about 1 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
of 5 = 0.1053 (0.28%).
Of the three density studies [36, 63, 91, 113] the
data of Ellis and Smith [91] were selected to calcu
late the tabulated values. Compared to the data
of Ellis et al. [91, 113] the maximum percent depar
tures of the densities of Klemm [36] and Huber,Potter, and Clair [63] are 0.24 (1044.2 °K) and 0.6
(1000 °K) respectively. The uncertainty of the den
sity values is judged to be about 0.2 percent.
!
An exponential equation, rj = 0.355 exp (5250/R71
),
for the viscosity has been reported by Ukshe [223]
without any mention of the temperature limits.
'
Calcium Chloride
[Refer: Table 26, p. 50, for numerical values]
Ten investigations of the specific conductancefor molten CaCL have been reported [2, 4, 11, 35,
42, 50, 71, 83, 85, 94]. The tabulated values werecalculated from the data of Bockris et al. [94]
(1046.3 to 1291.8 °K, 21 points). Using the exponential equation for specific conductance the
precision is 5 = 0.00587 (0.25%). Compared to the
data of Bockris et al., the results of Biltz andKlemm [35], Yaffe and van Artsdalen [83], and Leeand Pearson [50] show maximum departures of— 6.4 percent (1061 °K), 4.4 percent (1223 °K), and0.02 percent (1073 °K) respectively; the results
of the other investigators show larger departures.
I
The uncertainty of the specific conductance valuesis judged to be about 2.5 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
of 5 = 0.03441 (0.05%).
Of the four density studies [11, 17, 63, 83] the
most thorough appears to be that of van Artsdalenand Yaffe [83]. Compared to the density data of
van Artsdalen the results of Arndt and Gessler
[11], and Huber, Potter, and Clair [63] show maximum departures of —1.0 percent (1223 °K) and— 0.9 percent (1060 °K) respectively. The uncertainty of the density values calculated from thevan Artsdalen data [83] is estimated to be about0.9 percent.
Two investigations of the viscosity have beenreported [47, 109]. The tabulated values werecalculated from the data of Janz and Reeves [109]
(1058.7 to 1242.6 °K, 12 points, oscillating hollowcylinder technique). The cubic equation expressesthe data of Janz and Reeves with a precision
5 = 0.0738 (3.64%) and the uncertainty of the data
is judged to be about 4.0 percent.
The viscosities of the second study (Karpachevand Stromberg [47]; oscillating ball technique)
are consistently higher than those of Janz andReeves (e.g., 3.8% at 1073 °K; 18.7% at 1173 °K).
Strontium Chloride
[Refer: Table 27, p. 51, for numerical values]
Three investigations of the specific conductancefor molten SrCL have been reported [4, 83, 94].
The tabulated values were calculated from the data
of Bockris et al. [94] (1145.7 to 1357.0 °K, 14 points).
Using the exponential equation for specific con
ductance the precision is s = 0.0012 (0.05%). Thedeparture between the values of van Artsdalen andYaffe [83] and Bockris [94] is about 3.1 percent for
the range, 1145.7 to 1289.9 °K. The uncertainty of
the tabulated values is judged to be about 4.0
percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
of5= 0.0247 (0.036%).
Four density studies have been reported [11, 81,
83, 91]; of these the van Artsdalen and Yaffe [83]
study appears the best. Compared to the data of
van Artsdalen [83] the results of Arndt and Gessler
[11] and Ellis et al. [91] show maximum departures
of— 1.2 percent (1170°K) and — 0.4 percent (1163 °K)
respectively. The uncertainty of the density values,
calculated from the van Artsdalen data [83], is
judged to be about 0.7 percent.
The tabulated values of viscosity were calculated
from the data of Janz and Reeves [109] (1150.5 to
1258.6 °K, 18 points, oscillating hollow cylinder tech
nique). The exponential equation expresses the data
of Janz and Reeves with a precision 5=0.0706(2.88%) and the uncertainty of the data is judged to
be about (4.0%).
Barium Chloride
[Refer: Table 28, p. 51, for numerical values]
Five investigations of the specific conductance
for molten BaCl> have been reported [4, 63, 83,
85, 94]. The tabulated values were calculated fromthe data of Bockris et al. [94] (1232.6 to 1358.8 °K,
14 points). Using the exponential equation for
specific conductance, the precision is 5 = 0.00254
(0.12%). Compared to the data of Bockris et al.,
the results of Winterhager and Werner [85], andArndt [4] show maximum departures of 2.8 percent
(1241 °K) and —4.4 percent (1273 °K) respectively.
The uncertainty of the specific conductance values
is judged to be about 9.0 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
of 5 = 0.01954 (0.025%).
7
Five density studies have been reported [11, 63,
70, 81, 83]; of these the work of van Artsdalen andYaffe [83] appears the most thorough. The maximumdeparture between the density data of Arndt andGessler [11] and van Artsdalen [83] is —1.0 percent
(1273 °K); the results of Peake and Bothwell [70]
and Huber et al. [63], show larger departures. Theuncertainty of the density values calculated fromthe van Artsdalen data [83] is estimated to be about
5.0 percent.
Two investigations of the viscosity for this salt
have been reported [109, 210]. The tabulated values
were calculated from the data of Janz and Reeves
[109] (1261.4 to 1313.9 °K, 5 points, oscillating
hollow cylinder technique). The cubic equation
expresses the data of Janz and Reeves with a
precision s = 0.0651 (1.60%) and the uncertainty
of the data is considered to be about 4.0 percent.
The results of the second study (Slavyanskii [210])
are presented in graphical form only. The inter
polated values are consistently higher than those
of Janz and Reeves (e.g., 9.3% at 1274 °K; 28% at
1307 °K).
Scandium (III) Chloride
[Refer; Table 29, p. 51, for numerical values]
The tabulated values of specific conductance for
molten ScCfi were calculated from the data of Biltz
and Klemm [30] (1213 to 1264 °K, 5 points). Thedensity data of Klemm [36] are limited to two temperatures (1213 and 1273 °K). The data for these
properties are insufficient to establish the precision
or to judge the accuracy.
Yttrium (III) Chloride
[Refer; Table 30, p. 52, for numerical values]
The tabulated values of specific conductance for
molten YCfi were calculated from the data of Biltz
and Klemm [35] (973.2 to 1148.2 °K, 6 points). Usingthe quadratic equation for specific conductance the
precision is s = 0.00428 (0.69%) and the uncertainty
of the data is judged to be about 10 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
of 5 = 0.276 (1.8%).
The density values were calculated from the data
of Klemm [36]; no estimate of accuracy was at
tempted owing to the limited information.
Lanthanum (III) Chloride
[Refer: Table 31, p. 52, for numerical values]
Three investigations of the specific conductancefor molten LaCf? have been reported [35, 83, 118].
The tabulated values were calculated from the dataof van Artsdalen and Yaffe [83] (1146.2 to 1260.2
°K). Using the quadratic equation for specific
conductance the precision is 5 = 0.009 (0.05%). Theresults of Dworkin, Bronstein and Bredig [118]
(k = 1.640A 2.564 • covering a limited
range, 1153.2 to 1193.2 °K, are consistently smaller
than those of van Artsdalen (e.g., 10.7%, 1200 °K).
The uncertainty of the specific conductance values
is judged to be about 10 percent.
The exponential equation expresses the tabu
lated values of equivalent conductance with a
precision of 5 = 0.277 (0.63%).
The maximum departure between the density
results of Klemm [36] and those of van Artsdalenand Yaffe [83] is 0.94 percent (1250 °K). The uncer
tainty of the tabulated density values, calculated
from the data of van Artsdalen and Yaffe [83]
is judged to be about 0.6 percent.
The tabulated values of viscosity were calculated
from the exponential equation of Smirnov. Khokhlov,and Stepanov [136] (1183 to 1276 °K. 18 points,
oscillating ball viscometer). The uncertainty of
the viscosity values is estimated to be about (1.0%).
Cerium (III) Chloride
[Refer: Table 32, p. 53, for numerical values]
Two investigations of the specific conductancefor molten CeCfi have been reported [99. 119].
The tabulated values were calculated from the data
of Bronstein, Dworkin, and Bredig [119] (1101.2 to
1204.2 °K, 8 points). Using the quadratic equation
for specific conductance the precision is 5 = 0.00580
(0.41%). The maximum departure between the data
of Bredig [119] and Mellors and Senderoff [99] is
19.1 percent (1131.2 °K). The uncertainty of the
specific conductance values is estimated to be about
15 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.188(0.58%).
The density data of Senderoff [99] were used to
calculate the tabulated values; no estimate of accu
racy was attempted owing to the limited information.
Praseodymium (III) Chloride
[Refer: Table 33, p. 53, for numerical values]
Two investigations of the specific conductance for
molten PrCl 3 have been reported [32, 120]. Thetabulated values were calculated from the data of
Voigt and Biltz [32] (1097 to 1238 °K. 6 points). Usingthe exponential equation for specific conductancethe precision is 5 = 0.0032 (0.32%). The maximumdeparture between the data of Voigt [32] and Dworkin, Bronstein, and Bredig [120] is 20 percent
(1150 °K). The uncertainty of the specific conductance values is estimated to be about 15 percent.
8
Neodymium (III) Chloride
[Refer: Table 34, p. 53, for numerical values]
Two investigations of the specific conductancefor molten NdCfi have been reported [32, 118]. Thetabulated values were calculated from the data of
Voigt and Biltz [32] (1048 to 1173 °K, 6 points). Usingthe linear equation for specific conductance the
precision is 5 = 0.0024 (0.30%). The uncertainty of
the specific conductance values is estimated to beabout (12%).
Gadolinium (III) Chloride
[Refer: Table 35, p. 54, for numerical values]
The tabulated values of specific conductance for
molten GdCl3 were calculated from the data of
Dworkin, Bronstein, and Bredig[171] (902.2 to 971.2
°K, 4 points). Using the exponential equation for
specific conductance the precision is 5 = 0.00525(1.17%). The uncertainty of the specific conductancevalues is estimated to be about (20%).
Dysprosium (III) Chloride, Holmium (III)
Chloride, and Erbium (III) Chloride
[Refer: Tables 36 to 38, p. 54, for numerical values]
The tabulated values of specific conductance for
molten DyCb, H0CI3 , and ErCb were calculated
from the data of Dworkin, Bronstein, and Bredig
[171]. The number of data points, the temperature
range, the precision, the estimated uncertainty andthe best equation are as follows:
DyCh 3 points, 9521003 °K,
5 = 0.00483 (1.13%), (20%), linear equation.
HoCh — 4 points, 1020—1092 °K,
5 = 0.00289 (0.57%), (20%), linear equation.
ErCh  3 points, 10741 1 12 °K,
5 = 0.000150 (0.03%), (20%), linear equation.
Thorium (IV) Chloride
[Refer: Table 39, p. 55, for numerical values]
The tabulated values of specific conductancefor molten ThCh were calculated from the data of
Voigt and Biltz [32] (1087.2 to 1195.2 °K, 5 points).
Using the quadratic equation for specific con
ductance the precision is 5 = 0.0140 (1.96%), andthe uncertainty of the specific conductance valuesis estimated to be about 15 percent.
The exponential equation expresses the tabulated values of equivalent conductance with a
precision 5 = 0.273 (1.2%).
The density results reported by Klemm [36]
show little change with temperature; no estimateof accuracy was attempted.
Uranium (IV) Chloride
[Refer: Table 40, p. 55, for numerical values]
The tabulated values of specific conductance for
molten UCI4 were calculated from the data of Voigt
and Biltz [32] (843 to 893 °K, 3 points). Using the
linear equation for specific conductance the pre
cision is 5 = 0.0013 (0.32%). The uncertainty of the
tabulated specific conductance values is estimated
to be about (9%). The melting point (840 °K) ob
served by Voigt [32] is lower than the established
melting point (863 °K) [130].
Manganese (II) Chloride
[Refer: Table 41, p. 55, for numerical values]
Two investigations of the specific conductancefor molten MnCU have been reported [85, 192]. Thetabulated values were calculated from the data of
Murgulescu and Zuca [192] (923.2 to 1123.2 °K, 5
points). Using the quadratic equation for specific
conductance the precision is 5 = 3.66 • 10~ 4 (0.022%).
Comparison of the data of Murgulescu [192] andWinterhager and Werner [85] shows the maximumdeparture to be about 27 percent (1128.2 °K). Theuncertainty of the specific conductance values is
estimated to be about 20 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.265 (0.59%).
The density data of Murgulescu [192] were used
to calculate the tabulated values; no estimate of
accuracy was attempted owing to the limited
information.
Titanium (IV) Chloride
[Refer: Table 42, p. 55, for numerical values]
The tabulated values of viscosity for molten TiCbhave been calculated from the data of Toropov [204]
(293 to 333 °K, 3 points, capillary viscometer). Theexponential equation expresses the data of Toropovwith a precision 5 = 0.0095 (1.39%). No estimate of
accuracy was attempted owing to the limited
information.
Copper (I) Chloride
[Refer: Table 43, p. 56, for numerical values]
Five investigations of the specific conductance for
molten CuCl have been reported [33, 35, 85, 189,
212]. The tabulated values were calculated from the
data of Grantham and Yosim [189] (746.2 to 1430.2
°K, 19 points). Using the cubic equation for specific
conductance the precision is 5 = 6.40 • 10~ 3 (0.16%).
This cubic equation can be used to gain values of
specific conductance (within 6%) in the range 700 to
9
740 °K. Grantham [189] has reported a specific con
ductance maximum at 1123 °K. Compared to the
data of Grantham the results of Klemm and Biltz
[33], and Winterhager and Werner [85] show maxi
mum departures of — 5.5 percent (740 °K), and 5.1
percent (950 °K) respectively. The uncertainty of the
specific conductance values is estimated to beabout 5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5= 0.968(0.84%).
The data of Klemm [36] were used to calculate the
densities; no estimate of accuracy was attemptedowing to the limited information.
The tabulated values of viscosity were calculated
from the data of Karpachev and Stromberg [47]
(773.2 to 973.2 °K, 5 points, oscillating ball tech
nique). The cubic equation expresses the data with
a precision 5 = 0.00069 (0.037%). The uncertainty
of the viscosity values is estimated to be about
(2.0%).
Silver Chloride
[Refer: Table 44, p. 56, for numerical values]
Eight investigations of the specific conductancefor molten AgCl have been reported [1, 10, 21, 23,
60, 72, 100, 166, 202, 212]. The tabulated values
were calculated from the quadratic specific con
ductance equation of Bell and Flengas [166] (753
to 1013 °K). The precision reported by Flengas is
5 = 0.0035 (0.082%). The maximum percent depar
tures between the specific conductance values of
Bell and Flengas [166] and the other investigators
are as follows: Spooner and Wetmore [60], 0.4
percent (773.2 °K); Doucet and Bizouard [100],
1.1 percent (873.2 °K); Arndt and Gessler [10],
4.4 percent (973 °K); Tubandt and Lorenz [21],
— 3.8 percent (873 °K); Lorenz and Hochberg [23],
2.6 percent (873 °K); and Harrap and Heymann[72], —2.7 percent (873 °K). The uncertainty of
the specific conductance values is estimated to beabout 0.7 percent.
The exponential equation expresses the tabu
lated values of equivalent conductance with a
precision 5 = 0.279 (0.21%).
Of the five density studies [22, 54, 60, 81, 166,
212] the data of Flengas [166] were selected to cal
culate the tabulated values. Compared to the den
sity data of Flengas [166] the results of Spoonerand Wetmore [60], Lorenz and Hochberg [22],
and Boardman, Dorman, and Heymann [54], showmaximum departures of 0.2 percent (743 °K), — 0.8
percent (901 °K), and —1.1 percent (900 °K) respec
tively. The studies of Schinke and Sauerwald [81]
were to establish the volume change on fusion.
The estimated uncertainty of the density values is
about 0.1 percent.
Two investigations of the viscosity have beenreported [24, 72]. The tabulated values werecalculated from the data of Harrap and Heymann
[72] (723.2 to 973.2 °K, 10 points, vertical capillary
viscometer). The cubic equation expresses the data
of Harrap and Heymann with a precision s = 0.0033
(0.19%). The uncertainty of the viscosity values
is estimated to be about 1.5 percent.
The results of the second study (Lorenz andHochberg [24], oscillating disk technique) are
consistently lower than those of Harrap and Heymann (e.g., 2.7%, 876.2 °K: 6.4%, 942.2 °K).
Zinc Chloride
[Refer: Table 45, p. 57, for numerical values]
Five investigations of the specific conductance for
molten ZnCf> have been reported [33, 87, 94, 98,
189]. The tabulated values were calculated from thedata of Bockris et al. [94] (593.3 to 969.7 °K). Tocover the entire range it was necessary to generatethree quadratic equations: the temperature range,the number of data points, and the precision appropriate to this subdivision are as follows:
593.3 to 672.5 °K, 7 points, s = 4.66 x 10~ 4 (6.6%);
672.5 to 824.7 °K, 10 points, 5 = 8.38 X 10 4 (1.25%);824.7 to 969.7 °K, 13 points, 5 = 1.60 X 10 3 (0.53%).
Comparison of the data of Bockris [94] and Grantham and Yosim [189] in the low temperature region
(593.3 to 672.5 °K) shows the maximum departureto be 42 percent (633 °K). The uncertainty of the
specific conductance values for this region is esti
mated to be about 30 percent. The maximum departure between the data of Bockris [94] and Duke andFleming [87] (in the range 672.5 to 824.7 °K) is — 5.6
percent (748 °K). In the high temperature range(824.7 to 969.7 °K) comparison of the results of
Bockris [94] and Grantham [189] shows the maximum departure to be 3.94 percent (937.2 °K). Theuncertainty of the specific conductance values in
the region 672.5 to 969.7 °K is estimated to be about
5 percent.
For temperatures above 960 °K values of specific
conductance may be gained from the following
quadratic equation (5=0.011 (1.8%)) based on the
data of Grantham [189] (937.2 to 1136.2 °K, 5 points):
k= 1.503444.54126 • 10~ 3r+ 3.55485 • lOT2.
The three exponential equations express the
tabulated values of equivalent conductance with
the precisions 5 = 0.040 (18%) (593.3 to 672.5 °K);
5 = 0.062 (3.3%) (672.5 to 824.7 °K); 5 = 0.080 (0.94%)
(824.7 to 969.7 °K) respectively.
Of the seven investigations of density [36, 40.
56, 87, 91, 98, 113] the results of Mackenzie andMurphy [98] were selected to calculate the tabu
lated values. The density values of Mackenzie [98]
are in agreement with those of Klemm [36] to within
(0.3%). Compared to the data of Mackenzie, theresults of Duke and Fleming [87], Wachter andHildebrand [40] and Ellis and Smith [91] showmaximum departures of —0.2 percent (866 °K),
10
— 0.5 percent (823.9 °K) and —1.6 percent (934 °K)
respectively.
The tabulated values of viscosity were obtainedfrom the data of Mackenzie and Murphy [98] (593.2
to 673.2 °K, 5 points, restricted falling ball tech
nique). Since the least squaring to exponential,quadratic and cubic were poor, it became necessaryto obtain the tabulated values from a smooth curveof the experimental data.
Cadmium Chloride
[Refer: Table 46, p. 57, for numerical values]
Six investigations of the specific conductance of
molten CdCL have been reported [19, 27, 33, 51,
66, 94]. The tabulated values were calculated from
the data of Bockris et al. [94] (844.7 to 1082.4 °K,
25 points). Using the quadratic equation for specific
conductance the precision is 5 = 0.000149 (0.007%).
Compared to the data of Bockris, the results of
Bloom and Heymann [51], Bloom and Knaggs [66]
and Aten [19] show departures of — 0.3 percent
(873 °K), 0.8 percent (1000 °K) and —0.8 percent
(853 °K) respectively; the results of the other investi
gators show larger departures. The uncertainty of
the specific conductance values is estimated to be
about 0.6 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.02004(0.035%).
Of the three investigations of density [15, 54, 66],
the data of Bloom et al. [66] and Boardman et al. [54]
were selected to generate the linear equation to
express the density values. The maximum percent
departure between the density values of Bloom [66]
and Boardman [54] is 0.3 percent (850 °K) while that
between the tabulated values and the values of
Lorenz, Frei, and Jabs [15] is 1.3 percent (870 °K).
The uncertainty of the density values is estimated
to be about 0.3 percent.
Two investigations of viscosity have been reported
[47, 53]. The tabulated values of viscosity werecalculated from the data of Bloom, Harrap, andHeymann [53] (863.2 to 963.2 °K, 10 points, vertical
capillary viscometer). The exponential equationexpresses the data of Bloom, Harrap, and Heymannwith a precision 5=0.0075 (0.36%). The uncertainty
of the viscosity values is estimated to be about 1.5
percent.
The viscosities of the second study (Karpachevand Stromberg [47], the oscillating ball technique)are consistently higher than those of Bloom, Harrap,and Heymann. The maximum departure from thetabulated values is 5.2 percent (873 °K).
Mercury (I) Chloride
[Refer: Table 47, p. 58, for numerical values]
The tabulated values of specific conductancefor molten HgCl were calculated from the data of
Biltz and Klemm [35] (802.2 to 819.2 °K, 4 points).
Using the exponential equation for specific conductance the precision is 5 = 0.00604 (0.60%).The uncertainty of specific conductance values is
estimated to be about (20%).The exponential equation expresses the tabu
lated values of equivalent conductance with aprecision s = 0.00732 (0.017%).The density data of Klemm [36] were used to
calculate the tabulated values; no estimate of accuracy was attempted owing to the limited information.
Mercury (II) Chloride
[Refer: Table 48, p. 58, for numerical values]
Four investigations of the specific conductancefor molten HgCU have been reported [35, 94, 103,
189]. The tabulated values were calculated from the
data of Grantham and Yosim [189] (559.2 to 705.2 °K,
17 points). Using the cubic equation for specific con
ductance the precision is 5 = 3.87 • 10~ 7 (0.50%).
Grantham’s [189] results in the temperature range559.2 to 802.2 °K exhibit a maximum value at 753 °K.
The maximum departure between the data of Bockris et al. [94] and Grantham and Yosim [189] is 2.6
percent (579 °K); the results of Biltz and Klemm[35] and Janz and McIntyre [103] show larger depar
tures. The uncertainty of the specific conductancevalues is estimated to be about 3 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 8.5 • 10 5 (4.2%).
Of the three density studies [18, 103, 127], the
data of Janz and McIntyre [103] were selected to
calculate the tabulated values. Compared to the
data of Janz, the results of Johnson, Silva, andCubicciotti [127] and Prideaux [18] show maximumdepartures of 0.4 percent (550 °K) and 2.5 percent
(630 °K) respectively. The uncertainty of the density
values is judged to be about 0.5 percent.
The tabulated values of viscosity were calculated
from the data of Janz and McIntyre [103] (554.0 to
579.3 °K, 5 points, oscillating hollow sphere tech
nique). The cubic equation expresses the data with
a precision 5 = 0.0080 (0.49%). The uncertainty of
the viscosity values is estimated to be about (3.0%).
Aluminum (III) Chloride
[Refer: Table 49, p. 58, for numerical values]
The density data of Nisel’son and Sokolova [149](480.1 to 623.2 °K, 18 points) for molten AlCR wereused to calculate the tabulated values. Using thequadratic equation for density the precision is
5 = 0.0422 (3.7%). No estimate of accuracy wasattempted owing to the poor precision and limitedinformation.
The tabulated values of viscosity were calculatedfrom the data of Nisel’son and Sokolova [149]
297268 068—2 11
(461.5 to 549.2 °K, 12 points, capillary viscometer).
The cubic equation expresses the data with a preci
sion 5 = 0.00159 (0.62%). The uncertainty of the
viscosity values is estimated to be about (1.0%).
Gallium (III) Chloride
[Refer: Table 50, p. 59, for numerical values]
Of the two density studies [148, 149] for molten
GaCb, the data of Greenwood and Wade [148]
were selected to calculate the tabulated values.
The maximum departure between the densities
reported by Nisel’son and Sokolova [149] andWade [148] is 0.77 percent (388.8 °K). The estimated
uncertainty of the density values is about 0.4
percent.
Two investigations of the viscosity have beenreported [148, 149]. The tabulated values werecalculated from the data of Nisel’son and Sokolova
[149] (355.9 to 519.7 °K, 12 points, capillary vis
cometer). The cubic equation expresses the data of
Nisel’son and Sokolova with a precision 5 = 0.0121
(1.78%). The uncertainty of the viscosity values is
estimated to be about 2.0 percent.
The results of the second study (Greenwood andWade [148]; capillary viscometer) are in excellent
agreement with those of Nisel’son and Sokolova(e.g., 0.63% at 360 °K).
Indium Chloride
[Refer: Table 51, p. 59, for numerical values]
The tabulated values of specific conductance for
molten InCl were calculated from the data of Klemm[34] (498.2 to 624.2 °K, 5 points). Using the quadratic
equation for specific conductance the precision is
5 = 0.0176 (1.5%). The estimated uncertainty of the
tabulated specific conductance values is about
(12%).The exponential equation expresses the tabu
lated values of equivalent conductance with a pre
cision 5 = 0.205 (0.39%).
The density values were calculated from the data
of Klemm [34]; no estimate of accuracy was at
tempted owing to the limited information.
Indium (II) Chloride
[Refer: Table 52, p. 60, for numerical values]
The tabulated values of specific conductance for
molten InCl2 were calculated from the data of
Klemm [34] (508.2 to 780.2 °K, 8 points). Using the
quadratic equation for specific conductance the
precision is 5 = 0.0074 (1.5%). The uncertainty of the
specific conductance values is estimated to be about
(12%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.389 (2.4%).
The density values were calculated from the data
of Klemm [34]; no estimate of accuracy was at
tempted owing to the limited information.
Indium (III) Chloride
[Refer: Table 53, p. 60, for numerical values]
The tabulated values of specific conductancefor molten InCfi were calculated from the data of
Klemm [34] (859.2 to 967.2 °K, 6 points). Using the
linear equation for specific conductance the
precision is 5 = 0.00235 (0.61%). The uncertainty
of the specific conductance values is estimatedto be about (10%).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.0580 (0.42%).
The density values were calculated from the data
of Klemm [34]: no estimate of accuracy was at
tempted owing to the limited information.
Thallium (I) Chloride
[Refer: Table 54, p. 61, for numerical values]
Two investigations of the specific conductancefor molten T1C1 have been reported [21. 189]. Thetabulated values were calculated from the data of
Grantham and Yosim [189] (720.2 to 1169.2 °K.
22 points). Using the cubic equation for specific
conductance the precision is 5 = 5.52 • 10 3 (0.30%).
The maximum departure between the data of
Tubandt and Lorenz [21] and Grantham [189] is
0.7% (880 °K). The uncertainty of the specific
conductance values is estimated to be about
0.7 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.363 (0.43%).
The data of Klemm [36] were used to calculate
the densities; no estimate of accuracy was attemptedowing to the limited information.
Tin (II) Chloride
[Refer: Table 55, p. 61, for numerical values]
Two investigations of the specific conductance for
molten SnCl2 have been reported [35, 189]. Thetabulated values were calculated from the data of
Grantham and Yosim [189] (529.2 to 1235.2 °K, 21
points). Although the cubic equation expresses the
data with a precision 5 = 4.41 • 10 3 (0.18%), it is not
entirely satisfactory in the low temperature region
(1.0% at 560.2 °K). Grantham’s results exhibit a
maximum value for specific conductance at 1148 °K.
The maximum departure between the data of Biltz
and Klemm [35] and Grantham [189] is 5.1 percent
(520 °K). The uncertainty of the specific conductancevalues is estimated to be about 4 percent.
The exponential equation expresses the tabulated
12
values of equivalent conductance with a precision
5 = 4.95 (7.4%).
Of the two density studies [25, 36], the data of
Jaeger [25] were selected to calculate the tabulated
values. The maximum departure between the re
sults of Jaeger [25] and Klemm [36] is 1.34 percent
(638.2 °K). The uncertainty of the density values is
judged to be about 1.3 percent.
Tin (IV) Chloride
[Refer: Table 56, p. 62, for numerical values]
The density data of Pugachevick, Nisel’son,
Sokolova, and Anurov [147] for molten SnCL wereused to calculate the tabulated values. The esti
mated uncertainty of the density values is about
(0.8%).
Two investigations of the viscosity have beenreported [147, 204]. The tabulated values were calcu
lated from the data of Pugachevick, Nisel’son,
Sokolova, and Anurov [147] (273 to 423 °K, 20 points,
capillary viscometer). The exponential equation
expresses the data of Pugachevick [147] with a pre
cision 5 = 0.0059 (1.15%). The uncertainty of the
viscosity values is judged to be about 1.5 percent.
The results of the second study (Toropov [204];
capillary viscometer) are in good agreement with
those of Pugachevick (e.g., —4.6%, 293 °K; 0.7%,333 °K).
Lead (II) Chloride
[Refer: Table 57, p. 62, for numerical values]
Six investigations of the specific conductance for
molten PbCfi have been reported [7, 51, 72, 85,
97, 151, 212]. The tabulated values were calculatedfrom the data of Lantratov and Moiseeva [97]
(773.2 to 923.2 °K, 7 points). Using the quadraticequation for specific conductance the precision is
5 = 0.00802 (0.44%). Compared to the data of Lantratov and Moiseeva the results of Lorenz andKalmus [7] and Bloom and Heymann [51] showmaximum departures of —1.0 percent (881 °K)and —0.5 percent (873 °K); the results of the otherinvestigators show larger departures. The uncertainty of the specific conductance values is esti
mated to be about 5 percent.
The exponential equation expresses the tabulated values of equivalent conductance with a
precision 5 = 0.301 (0.58%).
Of the four density studies [15, 40, 54, 150] thedata of Boardman, Dorman, and Heymann [54]
were selected to calculate the tabulated values.The maximum percent departures between theresults of Boardman et al. [54], and those of Wachterand Hildebrand [40], Bell and Flengas [150], andLorenz, Frei, and Jabs [15] are —0.3 percent(818.5 °K), 0.7 percent (920 °K) and —0.8 percent(800 °K) respectively. The uncertainty of the densityvalues is estimated to be about 0.3 percent.
Two investigations of the viscosity have beenreported [8, 72]. The tabulated values were cal
culated from the data of Harrap and Heymann1 72]
(773.2 to 973.2 °K, 6 points, vertical capillary
viscometer). The exponential equation expressesthe data of Harrap and Heymann with a precision
5 = 0.0091 (0.33%). The uncertainty of the viscosity
data is estimated to be about 1.5 percent.
The viscosities of the second study (Lorenz andKalmus [8]; horizontal capillary viscometer) are
consistently higher than those of Harrap andHeyman. The maximum departure from the tabu
lated values is 15 percent (781 °K).
Bismuth (III) Chloride
[Refer: Table 58, p. 63, for numerical values]
The specific conductance of molten BiCl3 hasbeen determined by Voigt and Biltz [32] and Grantham [114]. The tabulated values were calculatedfrom the data of Grantham [114] (502.2 to 898.2 °K,
11 points). Using the cubic equation for specific
conductance the precision is 5= 10.7 • 10 4 (0.18%).
The maximum departure between the specific con
ductance values of Grantham [114] and Voigt [32]
is 2.4 percent (519.2 °K). The uncertainty of the
specific conductance values is estimated to beabout 2.3 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=1.58 (9.6%).
Of the two density investigations [25, 32], the data
of Voigt and Biltz [32] were selected to generatethe tabulated values. The maximum departure be
tween the densities reported by Voigt [32] andJaeger [25] is 0.34 percent (655.2 °K). The uncer
tainty of the density values is estimated to be about
0.4 percent.
The tabulated values of viscosity were calculated
from the data of Aten [16] (553.2 to 613.2 °K, 9 points,
Ubbelohde viscometer). The cubic equation ex
presses the data of Aten with a precision 5 = 0.1592
(0.70%). The uncertainty of the viscosity values is
estimated to be about (1.5%).
Tellurium (II) Chloride
[Refer: Table 59, p. 63, for numerical values]
The tabulated values of specific conductance for
molten TeCl 2 have been calculated from the data
of Voigt and Biltz [32] (479 to 578 °K, 11 points).
Using the quadratic equation for specific conduct
ance the precision is 5 = 8.010 4(0.80%). The
uncertainty of the specific conductance values is
estimated to be about (10%).
Tellurium (IV) Chloride
[Refer: Table 60, p. 63, for numerical values]
The tabulated values of specific conductance
13
for molten TeCR were calculated from the data of
Voigt and Biltz [32] (509 to 589 °K, 5 points). Usingthe quadratic equation for specific conductancethe precision is 5 = 6.09 • 10 4
(0.38%). The uncertainty of the specific conductance values is esti
mated to be about (9%).
Lithium Bromide
[Refer: Table 61, p. 64, for numerical values]
The tabulated values of specific conductance for
molten LiBr were calculated from the data of
van Artsdalen and Yaffo [82] (831.2 to 1022.2 °K, 11
points). Using the quadratic equation for specific
conductance the precision is 5 = 0.00254 (0.47%).
The uncertainty of the specific conductance values
is estimated to be about (1.5%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.318 (0.17%).
Of the three density studies [3, 81, 82] the data
of van Artsdalen and Yaffe [82] were selected to
calculate the tabulated values. The maximum depar
ture between the density values of van Artsdalen
[82] and Brunner [3] is 3.3 percent (880 °K). Thestudies of Schinke and Sauerwald [81] were to estab
lish volume change on fusion. No estimate of accu
racy was attempted owing to the limited information.
Two investigations of the viscosity have beenreported [47, 102]. The tabulated values were calcu
lated from the data of Murgulescu and Zuca [102]
(862.2 to 1046.2 °K, 13 points, oscillating ball tech
nique). The exponential equation expresses the
data of Murgulescu and Zuca with a precision
5=0.0180 (1.56%). The uncertainty of the viscosity
values is estimated to be about 2.0 percent.
The viscosities of the second study (Karpachevand Stromberg [47], oscillating ball technique) are
consistently higher than those of Murgulescu andZuca. The maximum departure from the tabulated
values is 51.6 percent (873 °K).
Sodium Bromide
[Refer: Table 62, p. 64, for numerical values]
Five investigations of the specific conductance for
molten NaBr have been reported [10, 52, 82, 129,
199], The tabulated values were calculated fromthe data of van Artsdalen [82] (1017.2 to 1229.0 °K,
15 points). Using the exponential equation for specific conductance the precision is 5 = 0.00322(0.10%). The maximum percent departure betweenthe data of van Artsdalen [82] and Arndt and Gessler
[10] is —1.8 percent (1173 °K); the results of theother investigators show larger departures. Theuncertainty of the specific conductance values is
estimated to be about 7 percent.The exponential equation expresses the tabulated
values of equivalent conductance with a precision5 = 0.179 (0.12%).
Of the four density investigations [3, 25, 81, 82],
the data of van Artsdalen and Yaffe [82] were se
lected to calculate the tabulated values. The maximum departure between the density values of
van Artsdalen [82] and Brunner [3] is — 0.3 percent(1050 °K); the results of Jaeger [25] show larger
departures. The studies of Schinke and Sauerwald[86] were to establish the volume change on fusion.
The uncertainty of the density values is estimated to
be about 1 percent.
Two investigations of the viscosity have beenreported [12, 102]. The tabulated values were calcu
lated from the data of Murgulescu and Zuca [102]
(1053.7 to 1212.7 °K, 10 points, oscillating ball tech
nique). The cubic equation expresses the data of
Murgulescu and Zuca with a precision 5 = 0,0040
(0.38%). The uncertainty of the viscosity values is
estimated to be about 1.0 percent.
The viscosities of the second study (Fawsitt [12],
oscillating disk technique) show departures of— 2.29
percent (1053 °K) and +5.83 percent (1153 °K) fromthose of Murgulescu and Zuca.
Potassium Bromide
[Refer: Table 63, p. 65, for numerical values]
Nine investigations of the specific conductancefor molten KBr have been reported [10, 26, 33, 52,
66, 82, 100, 125, 129]. The tabulated values werecalculated from the data of van Artsdalen and Yaffe
[82] (1011.0 to 1229.5 °K, 23 points). Using the quadratic equation for specific conductance the precision
is 5 = 0.00465 (0.26%). The maximum departure
between the results of van Artsdalen and Murgulescu and Zuca [129] is —0.8 percent (1140 °K); the
results of the other investigators show larger depar
tures. The uncertainty of the specific conductancevalues is estimated to be about 1.3 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.578 (0.53%).
Of the six investigations of density [3, 15, 26, 66,
81, 82], the most thorough appears to be that of
van Artsdalen and Yaffe [82]. Compared to the dataof van Artsdalen [82] the results of various investi
gators show the following maximum departures:
Jaeger and Kapma [26], —0.4 percent (1018.4 °K);
Brunner [3], —0.1 percent (1050 °K); Bloom et aU[66], 0.9 percent (1120 °K); and Lorenz, Frei. andJabs [15], —4.6 percent (1073 °K). The studies of
Schinke and Sauerwald [81] were to establish thevolume change on fusion. The uncertainty of thedensity values is estimated to be about 0.4 percent.
Three investigations of the viscosity have beenreported [12, 47, 102]. The tabulated values werecalculated from the data of Murgulescu and Zuca[102] (1017.8 to 1181.2 °K, 11 points, oscillating ball
technique). The cubic equation expresses the data
of Murgulescu and Zuca with a precision 5 = 0.0056
(0.59%). The uncertainty of the viscosity values is
estimated to be about 1.0 percent.
14
The investigator, reference, experimental method,and the maximum departure from the values of
Murgulescu and Zuca are as follows: Fawsitt [12],
oscillating disk, +24.9 percent; and Karpachev andStromberg [47], oscillating ball, — 19.1 percent.
Rubidium Bromide
[Refer: Table 64, p. 65, for numerical values!
The tabulated values of specific conductance for
molten RbBr were calculated from the data of
van Artsdalen and Yaffe [82] (968.9 to 1178.6 °K, 11
points). Using the quadratic equation for specific
conductance the precision is 5 = 0.00248 (0.18%).
The uncertainty of the specific conductance values
is estimated to be about 3.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.798 (0.91%).
Of the two density investigations [25, 82], the
data of van Artsdalen [82] were selected to calculate
the tabulated values. The maximum departure be
tween the densities reported by Jaeger [25] andvan Artsdalen [82] is 0.53 percent (1104.2 °K). Theuncertainty of the density values is estimated to beabout 0.4 percent.
The tabulated values of viscosity were calculatedfrom the data of Murgulescu and Zuca [102] (959.7
to 1139.5 °K, 11 points, oscillating ball technique).The cubic equation expresses the data of Murgulescu and Zuca with a precision 5 = 0.0046 (0.38%).
The uncertainty of the viscosity values is estimatedto be about 1.0 percent.
Cesium Bromide
[Refer: Table 65, p. 66, for numerical values]
Two investigations of the specific conductance for
molten CsBr have been reported [82, 199]. Thetabulated values were calculated from the data of
van Artsdalen and Yaffe [82]. Using the quadratic
equation for specific conductance the precision is
5 = 0.0025 (0.22%). The specific conductance values
of Markov and Prisyazhunyii [199] are lower than
those of van Artsdalen (e.g., —9.1% 1123 °K). Theuncertainty of specific conductance values is esti
mated to be about (5%).
The exponential equation expresses the tabulated
I
values of equivalent conductance with a precision
5 = 0.317(0.42%).
Of the three density investigations [25, 74, 82],
the data of van Artsdalen [82] were selected to calcu
late the tabulated values. The maximum departurebetween the densities of Jaeger [25] and van Arts
dalen is 0.7 percent (941 °K); the results of Johnsonet al. [74] show larger departures. The uncertainty
of the density values is estimated to be about 0.5
percent.
Magnesium Bromide
[Refer: Table 66, p. 66, for numerical values!
The tabulated values of specific conductance for
molten MgBr2 were calculated from the data of
Bockris et al. [94] (987.5 to 1244.3 °K, 25 points).
Using the quadratic equation for specific conductance the precision is 5 = 0.000232 (0.021%). Theuncertainty of the specific conductance values is
estimated to be about (1.0%).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.101 (0.29%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the limited
information.
Calcium Bromide
[Refer: Table 67, p. 67, for numerical values]
The tabulated values of specific conductance for
molten CaBr2 were calculated from the data of
Bockris et al. [94] (1013 to 1290.8 °K, 36 points).
Using the exponential equation for specific con
ductance the precision is 5 = 0.00397 (0.22%). Theuncertainty of the specific conductance values is
estimated to be about (2.5%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0535 (0.087%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated vqlues; no esti
mate of accuracy was attempted owing to the limited
information.
Strontium Bromide
[Refer: Table 68, p. 67, for numerical values]
The tabulated values of specific conductance for
molten SrBr2 were calculated from the data of
Bockris et al. [94] (928.8 to 1185.9 °K, 30 points).
The quadratic equation expresses the data of
Bockris with a precision 5 = 0.00196 (0.14%). Theuncertainty of the specific conductance values is
estimated to be about (6%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.436 (1.0%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the
limited information.
15
Barium Bromide
[Refer: Table 69, p. 68, for numerical values]
The tabulated values of specific conductance for
molten BaBr2 were calculated from the data of
Bockris et al. [94] (1126.3 to 1338.5 °K, 13 points).
The quadratic equation expresses the data of
Bockris with a precision 5 = 0.00501 (0.34%). Theuncertainty of the specific conductance values is
estimated to be about (10%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0390 (0.07%).
Of the two density studies [66, 91], the data of
Bloom et al. [66] were selected to calculate the
tabulated values. The maximum departure betweenthe densities reported by Bloom [66] and Ellis andSmith [91] is 1.06 percent (1160 °K). The uncer
tainty of the density values is estimated to beabout 1 percent.
Lanthanum (III) Bromide
[Refer: Table 70, p. 68, for numerical values]
Two investigations of the specific conductancefor molten LaBr3 have been reported [83, 171]. Thetabulated values were calculated from the quadratic
equation of Yaffe and van Artsdalen [83] for the
temperature range of 1050.2 to 1185.2 °K. The pre
cision reported by Yaffe and van Artsdalen is
5 = 0.003 (0.3%). The maximum departures betweenthe results of Dworkin, Bronstein, and Bredig [171]
and van Artsdalen [83] is 23.3 percent (1100 °K).
Similar disagreement between investigators is also
observed for the conductance data of NdBr3 ,
LaCl3 , PrCl3 ,and CeCl3 ; hence van Artsdalen’s
results should be viewed with reservation. Theuncertainty of the specific conductance values is
estimated to be about 23 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0874 (0.32%).
The density data of van Artsdalen [83] were usedto calculate the tabulated values; no estimate of
accuracy was attempted owing to the limited
information.
Praseodymium (III) Bromide
[Refer: Table 71, p. 68, for numerical values]
The tabulated values of specific conductance for
molten PrBr3 were calculated from the data of
Dworkin, Bronstein, and Bredig [171] (1000 to
1043 °K, 3 points). The linear equation for specific
conductance expresses the data with a precision
5 = 0.00228 (0.40%). The uncertainty of the specific
conductance values is estimated to be about
20 percent.
Neodymium (III) Bromide
[Refer: Table 72, p. 69, for numerical values]
Two investigations of the specific conductancefor molten NdBr3 have been reported [83. 171]. Thetabulated values were calculated from the quadraticequation of Yaffe and van Artsdalen [83] for the
temperature range of 963.2 to 1143.2 °K. Theprecision reported by Yaffe and van Artsdalen is
5 = 0.0036 (0.80%). The maximum departure be
tween the results of Dworkin, Bronstein, andBredig [171] and van Artsdalen [83] is 58 percent
(1020 °K). Similar disagreement between these
investigators is also observed for the conductancedata of LaBr3 ,
LaCl3 ,PrCl3 , and CeCb: hence, van
Artsdalen’s results should be viewed with reserva
tion. The uncertainty of the specific conductancevalues is estimated to be about 50 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.101 (0.67%).
The density data of van Artsdalen [83] were usedto calculate the tabulated values; no estimate of
accuracy was attempted owing to the limited
information.
Gadolinium (III) Bromide
[Refer: Table 73, p. 69, for numerical values]
The tabulated values of specific conductance for
molten GdBr3 were calculated from the data of
Dworkin, Bronstein, and Bredig [171] (1073 to
1115 °K, 3 points). The linear equation for specific
conductance expresses the data with a precision5 = 0.00109 (0.23%). The uncertainty of the specific
conductance values is estimated to be about2.0 percent.
Copper (I) Bromide
[Refer: Table 74, p. 69, for numerical values]
The tabulated values of specific conductance for
molten CuBr were calculated from the data ofTubandt [41] (764 to 823 °K, 3 points). Using theexponential equation for specific conductance theprecision is 5 = 0.00533 (0.20%). The uncertainty ofthe specific conductance values is estimated to beabout (8%).
Silver Bromide
[Refer: Table 75, p. 70, for numerical values]
Six investigations of the specific conductance for
molten AgBr have been reported [1, 10, 21. 23. 72,
100]. The tabulated values were calculated from thedata of Doucet and Bizouard [100] (773.2 to 1073.2 °K,
7 points) and Harrap and Heymann [72] (one pointat 723.2 °K). Using the quadratic equation for
specific conductance the precision is 5 = 0.00348
16
(0.12%). The maximum departures between the
tabulated values based on the results of Doucet[100] and Harrap [72], and the data of other
investigators are as follows: Kohlrausch [1],
3.4 percent (723 °K); Arndt and Gessler [10],
1.0 percent (723 °K); Lorenz and Hochberg [23],— 4.1 percent (873 °K). The uncertainty of the
specific conductance values is estimated to beabout 0.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.108 (1.01%).
Of the four density studies [2, 22, 54, 81] the
data of Boardman et al. [54] and Lorenz andHochberg [22] were selected to calculate the
tabulated values. The maximum departure betweenthe densities reported by Boardman [54] andLorenz [22] is 0.08 percent (930 °K). The uncertainty
of the density values is judged to be about 0.08
percent.
The high accuracies and good reproducibilities
obtained for both the specific conductance anddensity by several investigators indicate the possible
use of AgBr as a calibration standard for specific
conductance.
Two investigations of the viscosity have beenreported [24, 72]. The tabulated values were cal
culated from the data of Harrap and Heymann [72]
(713.2 to 873.2 °K, 9 points, vertical capillary viscom
eter). The cubic equation expresses the data of
Harrap and Heymann with a precision s — 0.0067
(0.25%). The uncertainty of the viscosity data is
estimated to be about 1.5 percent.
The viscosity study by Lorenz and Kalmus [24]
(oscillating disk technique) was carried out at
temperatures higher (882.2 to 1076.2 °K) than those
of Harrap and Heymann. The extrapolated value at
860 °K is lower (16%) than the tabulated value.
Zinc Bromide
[Refer: Table 76, p. 70, for numerical values]
Two investigations of the specific conductancefor molten ZnBr2 have been reported [94, 98]. Thetabulated values were calculated from the data of
Bockris et al. [94] (671.2 to 912.8 °K, 23 points).
Using the quadratic equation for specific conductance the precision is 5 = 0.0012 (1.48%). Mackenzieand Murphy [98] have determined the specific
conductance at one temperature (673.2 °K) (k=0.014)which is 18 percent below the value found byBockris. The uncertainty of the specific conductancevalues is estimated to be about (18%).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5 = 0.3248 (21.0%).
Of the two density studies [43, 113] the data ofBockris, Pilla, and Barton [113] were selected tocalculate the tabulated values. The maximumdeparture between the results of Salstrom [43] andBockris [113] is 2.0 percent (712.1 °K). The un
certainty of the density values is judged to beabout 1.7 percent.The viscosity of ZnBr2 was determined by
Mackenzie and Murphy [98] at one temperature(673.2 °K) using the restricted falling ball technique.The uncertainty of the viscosity value is estimatedto be about (8.0%).
Cadmium Bromide
[Refer: Table 77, p. 71, for numerical values]
The tabulated values of specific conductance for
molten CdBr2 were calculated from the data of
Bockris et al. [94] (849.6 to 1055.6 °K, 23 points).
Using the quadratic equation for specific conduct
ance the precision is 5 = 0.00161 (0.13%). The un
certainty of the specific conductance values is
estimated to be about (1.5%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0263 (0.06%).
The tabulated values of density were calculated
from the data of Boardman et al. [54] ; no estimate
of accuracy was attempted owing to the limited
information.
The tabulated values of viscosity were calculated
from the data of Bloom, Harrap, and Heymann [53]
(853.2 to 949.2 °K, 7 points, vertical capillary viscom
eter). The cubic equation expresses the data with a
precision 5 = 0.0072 (0.30%). The uncertainty of the
viscosity values is judged to be about (1.5%).
Mercury (II) Bromide
[Refer: Table 78, p. 71, for numerical values]
Three investigations of the specific conductancefor molten HgBr2 have been reported [94, 103, 189].The tabulated values were calculated from the dataof Grantham and Yosim [189] (528.2 to 729.2 °K,9 points). Using the cubic equation for specificconductance the precision is 5 = 8.65 • 107 (0.21%).Grantham’s [189] results in the temperature range528.2 to 853.2 °K exhibit a maximum value at
723 °K. Compared to the data of Grantham [189]the results of Bockris et al. [94] and Janz andMcIntyre [103] show maximum departures of1.0 percent (560 °K) and 0.8 percent (563 °K)respectively. The uncertainty of the specificconductance values is estimated to be about1.5 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5 = 8.6 • 104 (7.0%).
Of the two density studies [18, 103], the data ofJanz and McIntyre [103] were selected to calculatethe tabulated values. The maximum departurebetween the results ofPrideaux [18] and Janz [103]is 0.1 percent. The uncertainty of the density valuesis judged to be about 0.1 percent.Two investigations of the viscosity have been
reported [6, 58]. The tabulated values were calcu
17
lated from the data of Jander and Broderson [58](528.2 to 548.2 °K, 3 points, vertical capillary
viscometer). The exponential equation expressesthe data of Jander [58] with a precision 5 = 0.0078(0.39%). The uncertainty of the viscosity values is
considered to be about 1.5 percent.
The viscosities of the second study (Beck [6]
vertical capillary method) show considerable de
parture from those of Jander [58] (e.g., 15.5%,528 °K: 47.0%, 548 °K).
Aluminum Bromide
[Refer: Table 79, p. 72, for numerical values]
Two investigations of the viscosity for molten
AlBr3 have been reported [138, 203]. The tabulated
values were calculated from the data of Grothe andKleinschmit [138] (373 to 523 °K, 4 points, oscillat
ing hollow cylinder technique (with modification)).
The exponential equation expresses the data of
Grothe and Kleinschmit with a precision 5 = 0.0152
(1.32%). The uncertainty of the viscosity values is
estimated to be about 1.5 percent.
The results of the second study (Gorenbein [203];
capillary viscometer technique) are in good agree
ment with those of Grothe and Kleinschmit (e.g.,
3.0% at 383 °K; 1.4% at 423 °K).
Indium (III) Bromide
[Refer: Table 80, p. 72, for numerical values]
The tabulated values of specific conductance for
molten InBr3 were calculated from the data of
Klemm [34] (709.2 to 813.2 °K, 6 points). Using the
quadratic equation for specific conductance the
precision is 5 = 0.00178 (1.07%). The uncertainty of
the specific conductance values is estimated to beabout (12%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0260 (0.38%).
The density data of Klemm [34] were used to
calculate the tabulated values: no estimate of
accuracy was attempted owing to the limited
information.
Thallium (I) Bromide
[Refer: Table 81, p. 73, for numerical values]
Two investigations of the specific conductance for
molten TIBr have been reported [21, 189], Thetabulated values were calculated from the data of
Grantham and Yosim [189] (745.2 to 1127.2 °K,
20 points). Using the quadratic equation for specific
conductance the precision is 5 = 4.87 • 103 (0.38%).The maximum departure between the data of
Tubandt and Lorenz [21] and Grantham [189] is
0.96 percent (740 °K). The uncertainty of the specific
conductance values is estimated to be about1 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.0982 (0.16%).
The data of Buckle, Tsaoussoglou, and Ubbelohde[196] were used to calculate the densities; no esti
mate of accuracy was attempted owing to thelimited information.
Lead (II) Bromide
[Refer: Table 82, p. 74, for numerical values]
The specific conductance of molten PbBr2 hasbeen determined by Lorenz and Kalmus [7] andHarrap and Heymann [72]. The tabulated values
were calculated from the data of Lorenz [7] (655 to
765 °K, 12 points). Using the quadratic equation for
specific conductance the precision is 5 = 0.00164
(0.19%). The maximum departure between the
specific conductance values of Harrap [72] andLorenz [7] is 2.6 percent (773.2 °K). The uncertainty
of the specific conductance values is estimated to
to be about 2.7 percent.
At high temperatures the following quadratic
equation for specific conductance based on the
data of Harrap [72] (698.2 to 823.2 °K, 6 points) is
recommended :
k =  1.90813 + 4.23738 • 10~3:T 5.70634 • 10 7T 2.
The precision is 5 = 0.0132 (1.7%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.265 (1.0%).
Of the two density studies [15, 54], the data of
Boardman, Dorman and Heymann [54] were selected
to calculate the tabulated values. The density re
ported by Boardman [54] is 0.80 percent (873.2 °K)
higher than the value of Lorenz, Frei, and Jabs [15]
.
The uncertainty of the density values is judged to
be about 0.8 percent for the temperature range of
778.2 to 873.2 °K.
Three investigations of the viscosity have beenreported [8, 72, 142]. The tabulated values werecalculated from the data of Murgulescu and Zuca[142] (698 to 1023 °K, 14 points, oscillating ball
technique). The cubic equation expresses the data
of Murgulescu and Zuca with a precision 5 = 0.0191
(0.71%). The uncertainty of the viscosity values is
estimated to be about 1.0 percent.
The investigator, reference, experimental method,and the maximum percent departure from the values
of Murgulescu and Zuca are as follows: Lorenz andKalmus [8], capillary viscometer, 11.5 percent at
705 °K; Harrap and Heymann [72], capillary viscom
eter, 3.9 percent at 823 °K.
Bismuth (III) Bromide
[Refer: Table 83, p. 75, for numerical values]
The tabulated values of specific conductance for
molten BiBr3 were calculated from the data ofGrantham [114] (496.2 to 998.2 °K, 17 points).
18
Using the quadratic equation for specific conduct
ance the precision is 5 = 0.00132 (0.38%). Thespecific conductance increases with temperature
until a maximum is reached near 710 °K and then
decreases with further increasing temperature.
The uncertainty of the tabulated specific conduct
ance values is estimated to be about (3.0%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 1.30 (10%).
The density data of Jaeger [25] were used to
calculate the tabulated values; no estimate of
accuracy was attempted owing to the limited
information.
Lithium Iodide
[Refer: Table 84, p. 75, for numerical values]
Three investigations of the specific conductanceof molten Lil have been reported [82, 108, 227],
The recent results of Johnson [227] (756.2 to
876.5 °K, 15 points) were selected to generatethe best equation. Using the quadratic equationfor specific conductance the precision is 5 = 0.0026(0.61%). The specific conductance values of Karland Klemm [108] extends to very high temperatures(767 to 1163 °K). Compared to the data of Johnson,the results of Karl and Klemm and Yaffe andvan Artsdalen [82] are lower by 5.6 to 5.0 percentand 7.2 to 10.6 percent respectively. The uncertainty is estimated to be about 5.0 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.0659 (0.04%).
The density data of van Artsdalen [82] were usedto calculate the tabulated values. The values shouldbe considered with reservation due to partial de
composition of Lil, as reported by the authors, at
higher temperatures.
The tabulated values of viscosity were calculatedfrom the data of Karpachev and Stromberg [47](723.2 to 923.2 °K, 5 points, oscillating ball technique). The cubic equation expresses the data witha precision 5 = 0.0095 (0.57%). The uncertainty is
judged to be about (5.0%).
Murgulescu and Zuca [122] attempted to determine the viscosity of molten Lil but could not obtainreproducible results due to decomposition of themelt; no experimental data were reported.
Sodium Iodide
[Refer: Table 85, p. 76, for numerical values]
Five investigations of the specific conductancefor molten Nal have been reported [2, 10, 66, 82,129]. The tabulated values were calculated fromthe data of van Artsdalen and Yaffe [82] (936.2 to
1187.3 °K, 15 points). Using the quadratic equationfor specific conductance the precision is 5 = 0.00263(0.10%). Compared to the specific conductance dataof Bloom et al. [66] the results of Murgulescu andZuca [129] show departures of +5.2 percent to
— 3.2 percent over a temperature range of 940 to
1140 °K while that of van Artsdalen [82] shows a
maximum departure of 3.5 percent at 940 °K. Theuncertainty of the specific conductance values is
estimated to be about 3.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0127 (0.0084%).
Of the three density studies [25, 66, 82], the data
of yan Artsdalen [82] were selected to calculate
the tabulated values. The maximum percent de
parture between the density data of van Artsdalen
[82] and Bloom et al. [66] is 0.4 percent (940 °K)
while that between van Artsdalen and Jaeger [25]is 1.0 percent (1133 °K). The uncertainty of the
density values is judged to be about (0.4%).
Two investigations of the viscosity have beenreported [47, 122]. The tabulated values werecalculated from the data of Murgulescu and Zuca[122] (946.4 to 1107.8 °K, 13 points, oscillating ball
technique). The exponential equation expresses the
data of Murgulescu and Zuca with a precision
5 = 0.00847 (0.72%) and the estimated uncertainty
is about 1.0 percent.
The viscosities of the second study (Karpachevand Stromberg [47], oscillating ball technique) are
consistently higher than those of Murgulescu andZuca (e.g., 16.0%, 946.4 °K; 4.7%, 1107.8 °K).
Potassium Iodidey
[Refer: Table 86, p. 76, for numerical values]
Seven investigations of the specific conductancefor molten KI have been reported [10, 26, 33, 66,
79, 125a, 129]. The tabulated values were calculated
from the data of van Artsdalen and Yaffe [79]
(958.6 to 1183.9 °K, 21 points). Using the quadratic
equation the precision is 5 = 0.0075 (0.48%). Compared to the data of van Artsdalen the results of
Murgulescu and Zuca [129], Buckle and Tsaousso
glou [125a] and Bloom et al. [66] show departures
of 0.5 percent (1000 °K), 0.9 percent (1000 °K),
and 1.3 percent (1000 °K); the results of the other
investigators show larger departures. The uncer
tainty of the specific conductance values is estimated
to be about 0.9 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.758 (0.68%).
Of the four density studies [26, 66, 79, 81], the
most thorough appears to be that of van Artsdalen
and Yaffe [79], The maximum departure betweenthe densities of van Artsdalen [79] and Bloom et al.
[66] is 0.3 percent (1080 °K) while that betweenvan Artsdalen and Jaeger and Kapma [26] is
— 0.8 percent (1070 °K). The studies of Schinke andSauerwald [81] were to establish the volume changeon fusion. The uncertainty of the density values is
judged to be about 0.25 percent.
Two investigations of the viscosity have beenreported [47, 122]. The tabulated values were
19
calculated from the data of Murgulescu and Zuca[122] (975.1 to 1165.2 °K, 13 points, oscillating ball
technique). The exponential equation expressesthe data of Murgulescu and Zuca with a precision
5 = 0.00851 (0.70%). The uncertainty of the viscosity
values is estimated to be about 1.0 percent.
The viscosities of the second study (Karpachevand Stromberg [47], oscillating ball technique) are
consistently higher than those of Murgulescu andZuca (e.g., 27.2%, 1034.4 °K: 3.9%, 1165.2 °K).
Rubidium Iodide
[Refer: Table 87, p. 77, for numerical values]
The tabulated values of specific conductance for
molten Rbl were calculated from the data of van
Artsdalen and Yaffe [82] (929.5 to 1158.2 °K,
17 points). Using the quadratic equations for
specific conductance the precision is 5 = 0.00169
(0.16%). The uncertainty of the specific conductancevalues is estimated to be about (3.5%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.378 (0.45%).
Of the two density studies [25, 82], the data of
van Artsdalen [82] were selected to calculate the
tabulated values. The maximum departure betweenthe densities reported by Jaeger [25] and vanArtsdalen [82] is 1.4 percent (950 °K). The esti
mated uncertainty of the density values is about
0.7 percent.
The tabulated values of viscosity were calculated
from the data of Murgulescu and Zuca [122]
(922.2 to 1126.4 °K, 16 points, oscillating ball
technique). The cubic equation expresses the data
of Murgulescu and Zuca with a precision 5 = 0.0037
(0.34%). The uncertainty of the viscosity values is
judged to be about (1.0%).
Cesium Iodide
[Refer: Table 88, p. 77, for numerical values]
The tabulated values of specific conductance for
molten Csl were calculated from the data of vanArtsdalen and Yaffe [82] (932.0 to 1137.2 °K,
14 points). Using the quadratic equation for specific
conductance the precision is 5= 1.40 • 104 (0.16%).
The uncertainty of the specific conductance values
is estimated to be about (5.0%).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.378 (0.48%).Of the three density studies [25, 74, 82], the data
of van Artsdalen [82] were selected to calculate
the tabulated values. The maximum departurebetween the densities reported by Jaeger [25] andvan Artsdalen [82] is 0.42 percent (950 °K). Thedata of Johnson et al. [74] are insufficient to cal
culate departure values. The estimated uncertaintyof the density values is about 0.4 percent.
The tabulated values of viscosity were calculated
from the data of Murgulescu and Zuca [122]
(910.2 to 1126.9 °K, 14 points, oscillating ball
technique). The cubic equation expresses the data
of Murgulescu and Zuca with a precision 5 = 0.0163
(1.24%). The estimated uncertainty of the viscosity
values is judged to be about (1.5%).
Magnesium Iodide
[Refer: Table 89, p: 78, for numerical values]
The tabulated values of specific conductance for
molten Mgl2 were calculated from the data of Bockris et al. [94] (910.2 to 1176.5 °K, 21 points). Usingthe quadratic equation for specific conductance the
precision is 5 = 0.00110 (0.18%). The uncertainty of
the specific conductance values is estimated to beabout (1.3%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0810 (0.29%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the
limited information.
Calcium Iodide
[Refer: Table 90, p. 78. for numerical values]
The tabulated values of specific conductance for
molten Cal 2 were calculated from the data of
Bockris et al. [94] (1058.7 to 1286.6 °K, 26 points).
Using the quadratic equation for specific conductance the precision is 5 = 0.00055 (0.041%). Theuncertainty of the specific conductance values is
estimated to be about (2.0%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.422 (0.69%).
The density equation of Bockris, Pilla, andBarton [113], based on the data of Ellis and Smith
[91], was used to calculate the tabulated values;
no estimate of accuracy was attempted owing to the
limited information.
Strontium Iodide
[Refer: Table 91, p. 79, for numerical values]
The tabulated values for specific conductance for
molten Srl 2 were calculated from the data of Bockriset al. [94] (821.6 to 1270.4 °K, 28 points). Using thequadratic equation for specific conductance, theprecision is 5 = 0.00139 (0.13%). The uncertainty ofthe specific conductance values is estimated to beabout (6.0%).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5 = 0.571 (1.28%).
The density equation of Bockris. Pilla, and Barton[113], based on the data of Ellis and Smith [91],
20
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the limited
information.
Barium Iodide
[Refer: Table 92, p. 79, for numerical values]
The tabulated values of specific conductance for
molten Bal2 were calculated from the data of Bockris
et al. [94] (991.7 to 1292.3 °K, 26 points). Using the
quadratic equation for specific conductance the
precision is 5 = 0.0035 (0.35%). The uncertainty of
the specific conductance values is estimated to beabout (10%). It should be noted that the specific
conductance values are reported at temperaturesbelow the established melting point (mp 1013 °K)
[130, 131],
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.250 (0.5%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the limited
information.
Aluminum (III) Iodide
[Refer: Table 93, p. 79, for numerical values]
The tabulated values of specific conductance for
molten A1I3 were calculated from the data of Biltz
and Klemm [35] (464.2 to 543.2 °K, 9 points). Usingthe quadratic equation for specific conductance the
precision is 5 = 1.2510~ 7 (3.2%). The uncertainty
of the specific conductance values is estimated to
be about (20%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.121 (7.2%).
The density data of Biltz and Klemm [35] wereused to calculate the tabulated values; no estimate
of accuracy was attempted owing to the limited
information.
Lanthanum (III) Iodide, Cerium (III) Iodide,
Praseodymium (III) Iodide, and Neodymium(III) Iodide
[Refer: Tables 94 to 97, p. 80, for numerical values]
The tabulated values of specific conductance for
molten Lal 3 , Cel 3 ,Prl 3 ,
and Ndl 3 were calculated
from the data of Dworkin, Sallach, and Bronstein
[106]. The number of data points, the temperaturerange, the precision ( 5 ) and the estimated uncer
tainty of the specific conductance values are as
follows:
Lal3— 4 points, 1069 to 1144 °K, 5=0.0003 (0.06%),(10%).
Cel3 — 4 points, 1069 to 1 133 °K, 5=0.0003 (0.06%),(18%).
Prl3 — 3 points, 1036 to 1082 °K, 5=0.0003 (0.07%),(15%).
Ndl3  3 points, 1072 to 1115 °K, 5=0.0003 (0.07%),(15%).
Silver Iodide
[Refer: Table 98, p. 81, for numerical values]
Six investigations of the specific conductance for
molten Agl have been reported [1, 10, 11, 21, 23,
35] . The tabulated values were calculated from the
data of Biltz and Klemm [35] (825.2 to 923.2 °K,
4 points), Gessler and Arndt [11] (823.2 to 1073.2
°K, 5 points) and Kohlrausch [1] (823.2 to 973.2
°K, 4 points). Using the exponential equation for
specific conductance the precision is 5 = 0.111
(4.3%). Compared to the data of Biltz the results
of Gessler [11] and Kohlrausch [1] show depar
tures of +5 percent and —6.5 percent respectively
for the temperature range 825 to 923 °K. Themaximum departure between the tabulated values
based on the results of Biltz [35], Gessler [11],Kohlrausch [1], and the values of Tubandt andLorenz [21] is —1.2 percent (923 °K); the results
of Lorenz and Hochberg [23], and Arndt andGessler [10], show larger departures. It shouldbe noted that specific conductance values are re
ported at temperatures below the established melt
ing point (mp 831 °K) [130]. The uncertainty of the
specific conductance values is estimated to beabout 12 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.122 (0.10%).
The density data of Lorenz and Hochberg [22]
were used to calculate the tabulated values; noestimate of accuracy was attempted owing to lim
ited information.
The tabulated values of viscosity were calculated
from the data of Lorenz and Hochberg [24] (878.2
to 1100.2 °K, 8 points, oscillating disk technique).
The cubic equation expresses the data of Lorenzwith a precision 5 = 0.058 (2.6%). The uncertainty
of the viscosity values is judged to be about (3.0%).
Zinc Iodide
[Refer: Table 99, p. 81, for numerical values]
Two investigations of the specific conductancefor molten Znl2 have been reported [94, 189]. Thetabulated values were calculated from the data ofBockris et al. [94] (717.7 to 870.6 °K, 28 points).
Using the quadratic equation for specific conductance the precision is 5=1.10*10~ 3 (0.78%).The maximum departure between the data ofBockris [94] and Grantham and Yosim [189] is
1.2 percent (753.2 °K). The uncertainty of the specific
21
conductance values is estimated to be about 1.5
percent.
For temperatures above 870 °K values of specific
conductance can be gained from the following cubicequation (5 = 0.00271 (0.54%)) based on the data of
Grantham [189] (724.2 to 1262.2 °K, 27 points):
k = 2.09556 9.20558 • 103r+ 1.2 18344 • 10" 5r 2
4.631264 • lOT3.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.222 (3.37%).
The density equation of Bockris, Pilla, and Barton
[113], based on the data of Ellis and Smith [91],
was used to calculate the tabulated values; no esti
mate of accuracy was attempted owing to the limited
information.
Cadmium Iodide
[Refer: Table 100, p. 82, for numerical values]
The specific conductance of molten Cdl2 has beeninvestigated by Bloom et al. [66] and Bockris et al.
[94]. The tabulated values were calculated from thedata of Bockris [94] (674.9 to 912.8 °K, 32 points).
Using the quadratic equation for specific conductance the precision is 5 = 0.0020 (0.47%). The maximum departure between the specific conductancevalues of Bockris [94] and Bloom [66] is 6 percent(730 °K). The uncertainty of the tabulated specificconductance values is estimated to be about 4.5
percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5 = 0.450 (2.27%).
The density data of Bloom et al. [66] were usedto calculate the tabulated values; no estimate ofaccuracy was attempted owing to the limitedinformation.
Mercury (II) Iodide
[Refer: Table 101, p. 82, for numerical values]
Four investigations of the specific conductancefor molten Hgl2 have been reported [29, 94, 103,
189]. The tabulated values were calculated fromthe data of Grantham and Yosim [189] (532.2 to
724.2 °K, 13 points). Using the cubic equation for
specific conductance the precision is 5=1.61 • 10~4
(0.89%). Grantham’s [189] investigation of specific
conductance extends up to 905.2 °K and the negative temperature coefficient persists at the highesttemperatures. The maximum departure betweenthe data of Grantham [189] and Bockris et al. [96]is 2.3 percent; the results of the other investigators
show larger departures. The uncertainty of thespecific conductance values is estimated to beabout 2.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0313(3.3%).Of the three density studies [18, 78, 103], the
data of Janz and McIntyre [103] were selected to
calculate the tabulated values. Compared to the
data of Janz and McIntyre [103] the results of
Prideaux [18] and Polyakov [78] show maximumdepartures of 0.4 percent (596 °K) and 1.0 percent(573 °K) respectively. The uncertainty of the density values is judged to be about 0.1 percent.
Three investigations of viscosity have been re
ported [6, 78, 103], The tabulated values werecalculated from the data of Janz and McIntyre[103] (541.6 to 631.3 °K, 5 points, oscillating hol
low sphere method). The exponential equation ex
presses the data of Janz with a precision 5 = 0.0195
(1.02%). The uncertainty of the viscosity values is
estimated to be about 3.0 percent.
Beck [6] and Polyakov [78] measured the vis
cosity of molten Hgl2 at 531.2 and 533.2 °K re
spectively. These two values differ markedly fromeach other.
Gallium (II) Iodide
[Refer: Table 102, p. 83, for numerical values]
The tabulated values of specific conductance for
molten GaI 2 were generated from the data of
Riebling and Erickson [105] (423.2 to 623.2 °K,
9 points). Riebling [105] has reported three ex
ponential equations for specific conductance for
the temperature ranges (423 to 484 °K), (484 to 552°K) and (552 to 623 °K) respectively. Using these
equations the specific conductance values weregained at 423.2, 453.2, 483.2, 493.2, 518.2, 543.2,
563.2, 593.2, and 623.2 °K. These data were least
squared to develop a linear equation and the pre
cision is 5 = 0.0050 (3.6%). The uncertainty of the
specific conductance values is estimated to beabout (15%).The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.453 (7.7%).
The density data of Riebling [105] were used to
calculate the tabulated values; no estimate of ac
curacy was attempted owing to the limited infor
mation.
Indium (III) Iodide
[Refer: Table 103, p. 83, for numerical values]
Two investigations of the specific conductancefor molten Inl3 have been reported [34, 189]. Thetabulated values were calculated from the data of
Grantham and Yosim [189] (504.2 to 880.2 °K, 18
points). Using the cubic equation for specific con
ductance the precision is 5 = 6.3 10 4(0.60%).
The maximum departure between the data of
Klemm [34] and Grantham [189] is 8 percent
(560 °K). The uncertainty of the specific conduct
ance values is estimated to be about 6 percent.
22
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.233 (4.6%).
The data of Klemm [34] were used to calculate
the densitites; no estimate of accuracy was at
tempted owing to the limited information.
Thallium (I) Iodide
[Refer: Table 104, p. 84, for numerical values]
Three investigations of the specific conductancefor molten Til have been reported [21, 125c, 189].
The tabulated values were calculated from the
data of Grantham and Yosim [189] (721.2 to 1333.2
°K, 23 points). Using the quadratic equation for
specific conductance the precision is 5 = 2.65 • 103
(0.35%). The maximum departure between the
results of Ubbelohde [125c] and Grantham [189]
is 1.5 percent (760 °K); the results of Tubandtand Lorenz [21] show larger departures. The un
certainty of the specific conductance values is
estimated to be about 1.5 percent.
Lead (II) Iodide
[Refer: Table 105, p. 84, for numerical values]
The tabulated values of specific conductance for
molten Pbl2 were calculated from the data of Karl
and Klemm [108] (676 to 873 °K, 5 points). Thequadratic equation expresses the data with a pre
cision 5 = 0.0018 (0.32%). The uncertainty of the
specific conductance values is estimated to beabout (5%).
Bismuth (III) Iodide
[Refer: Table 106, p. 85, for numerical values]
The tabulated values of the specific conductancefor molten Bil3 were calculated from the data of
Grantham and Yosim [104] (686.2 to 775.2 °K, 5
points). The quadratic equation expresses the data
of Grantham with a precision 5 = 2.13 • 103 (0.71%).
The uncertainty of the specific conductance values
is estimated to be about (3%).
Lithium Carbonate
[Refer: Table 107, p. 85, for numerical values]
The tabulated values of specific conductance for
molten Li 2C03 were calculated from the data of
Janz and Lorenz [101] (1017.9 to 1117.7 °K, 7 points,
omitting the value at 1017.4 °K). Using the quadractic equation for specific conductance the pre
cision is 5 = 3.00 10~4 (0.0066%). The uncertaintyof the specific conductance values is estimated to
be about (1.5%).
The exponential equation expresses the tabu
lated values of equivalent conductance with a
precision s = 0. 140 (0.15%).
Of the two density studies [3, 101], the data of
Janz [101] were selected to calculate the tabulatedvalues. The maximum departure between the densities reported by Janz [101] and Brunner [3] is
0.3 percent (1012 °K). The uncertainty of the densityvalues is judged to be about 0.2 percent.
Two investigations of the viscosity have beenreported [107, 128]. The tabulated values of
viscosity were calculated from the data of Janz andSaegusa [107] (1046.2 to 1122.2 °K, 7 points,
oscillating hollow cylinder technique). The cubicequation expresses the data of Janz and Saegusawith a precision 5 = 0.1022 (2.90%). The estimated
uncertainty of the viscosity values is about (3.0%).
The viscosities of the second study (Karpachevet al. [128], oscillating ball technique) are con
sistently higher than those obtained by Janz andSaegusa (e.g., 27.7%, 1050 °K; 64.7%, 1120 °K).
Sodium Carbonate
[Refer: Table 108, p. 85, for numerical values]
Two investigations of the specific conductancefor molten Na2C03 have been reported [4, 101].
The tabulated values were calculated from the dataof Janz and Lorenz [101] (1138.0 to 1239.7 °K, 10
points). Using the exponential equation for specific
conductance the precision is 5 = 0.00420 (0.13%).
The departure between the specific conductancevalues of Janz [101] and Arndt [4] is 2.3 percent(1173.2 °K). The uncertainty of the specific conductance values is estimated to be about 1.5 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.035 (0.040%).
Of the two density studies [3, 101], the data of
Janz [101] were selected to calculate the tabulated
values. The maximum departure between the densi
ties reported by Janz [101] and Brunner [3] is
0.41 percent (1170 °K). The uncertainty of the den
sity values is judged to be about 0.2 percent.
Two investigations of the viscosity have beenreported [107, 128]. The tabulated values werecalculated from the data of Janz and Saegusa [107](1152.2 to 1245.2 °K, 6 points, oscillating hollow cyl
inder technique). The exponential equation ex
presses the data of Janz and Saegusa with a pre
cision 5 = 0.0112 (0.49%). The estimated uncertainty
of the viscosity values is about 3.0 percent.
The viscosities of the second study (Karpachevet al. [128], 1123.2 to 1173.2 °K, 2 points, oscillat
ing ball technique) show departures of about 25percent from those of Janz and Saegusa.
Potassium Carbonate
[Refer: Table 109, p. 86, for numerical values]
Two investigations of the specific conductancefor molten K2C03 have been reported [4, 101].The tabulated values were calculated from the dataof Janz and Lorenz [101] (1183.7 to 1279.1 °K, 14
23
points). Using the exponential equation for specific
conductance the precision is 5 = 0.00173 (0.12%).The maximum departure between the specific
conductance values of Janz [101] and Arndt [4]is 3.9 percent (1173.2 °K). The uncertainty of thespecific conductance values is estimated to beabout 1.5 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5 = 0.0175 (0.021%).
Of the two density studies [3, 101] the data of
Janz and Lorenz [101] were selected to calculate
the tabulated values. The maximum departurebetween the densities reported by Janz [101] andBrunner [3] is 0.43 percent (1240 °K). The uncertainty of the density values is judged to be about0.2 percent.
Two investigations of the viscosity have been re
ported [107, 128]. The tabulated values of viscosity
were calculated from the exponential equation usingthe data of Janz and Saegusa [107] (1186.2 to 1257.2°K, 5 points, oscillating hollow cylinder technique).The precision is 5 = 0.0272 (1.23%). The estimateduncertainty of the viscosity values is about 3.0
percent. Karpachev et al. [128], using the oscil
lating ball technique, reports one viscosity point at
a temperature (1173.2 °K) which is lower than themeasurement of Janz and Saegusa.
Lithium Nitrite
[Refer: Table 110, p. 86, for numerical values]
The tabulated values of specific conductance for
molten LiNCU were calculated from the data of
Protsenko, Protsenko, and Razumovskaya [207](502.7 to 727.2 °K, 6 points). Using the quadratic
equation for specific conductance the precision is
5 = 4.14 • 104 (0.056%). The maximum departurebetween the data of Protsenko [207] and Bloom,Knaggs, Molloy, and Welch [66] is 5.6 percent
(570 °K). The uncertainty of the specific conductancevalues is estimated to be about (6%).
The tabulated values of viscosity have been cal
culated from the data of Protsenko, Protsenko, andRazumovskaya [207] (502.7 to 527.2 °K, 6 points,
capillary viscometer). The cubic equation expressesthe data with a precision s = 0.0354 (0.39%). The un
certainty of the viscosity values is considered to beabout (1.0%).
Sodium Nitrite
[Refer: Table 111, p. 86, for numerical values]
Three investigations of the specific conductancefor molten NaNCL have been reported [66, 110,125c, 207]. The tabulated values were calculatedfrom the exponential specific conductance equationreported by Bloom et al. [66] for the temperaturerange 554 to 723 °K. Neither the precision nor theexperimental data were given. Compared to the data
of Bloom et al. [66] the results of Ubbelohde [125c]and Protsenko et al. [207] show maximum departures of —1.6 percent (572.2 °K) and 5.6 percent(570 °K) respectively. The uncertainty of the specific conductance values is estimated to be about1.6 percent.
The exponential equation expresses the tabulated values of equivalent conductance with a pre
cision 5 = 0.108 (0.15%).
Of the two density studies [66, 110] the data ofBloom et al. [66] were selected to calculate thetabulated values. The maximum departure betweenthe densities reported by Bloom [66] and Ubbelohde[110] is 0.99 percent (720 °K). The uncertainty of
the density values is judged to be about 1.0 percent.
Two investigations of the viscosity for this salt
have been reported [110, 125c, 207]. The tabulatedvalues were calculated from the data of Protsenko,Protsenko, and Razumovskaya [207] (563 to 613°K, 6 points, capillary viscometer). The cubic equation expresses the data with a precision 5 = 0.0187(0.70%). The uncertainty of viscosity values is con
sidered to be about 1.0 percent.
The results of the second study (Frame, Rhodes,Ubbelohde [110, 125c] capillary viscometer) areconsistently lower than those of Protsenko (e.g.,
4.0%, 572.7 °K; 1.4%, 583.5 °K).
Potassium Nitrite
[Refer: Table 112, p. 87, for numerical values]
The tabulated values of specific conductance for
molten KNOo were calculated from the data of
Protsenko, Protsenko, and Razumovskaya [207]
(713 to 743 °K, 4 points). Using the quadratic equa
tion for specific conductance the precision is
5 = 4.70 • 10 4 (0.058%). The uncertainty of the spe
cific conductance values is estimated to be about
(6%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0617(0.075%).
The data of Protsenko and Malakhova [173] wereused to calculate the densities; no estimate of ac
curacy was attempted owing to the limited infor
mation.
Two investigations of the viscosity have beenreported [110, 125c, 207, 208] . The tabulated values
were calculated from the data of Frame, Rhodes,and Ubbelohde [110, 125c] (686.8 °K to 725.4 °K,
9 points, capillary viscometer). The cubic equation
expresses the data of Ubbelohde with a precision
5 = 0.0055 (0.30%). The uncertainty of the viscosity
values is judged to be about 1.5 percent.
The viscosities of the second study (Protsenko,
Protsenko, and Razumovskaya [207] and Protsenkoand Shokina [208], capillary viscometer), are con
sistently lower than those of Ubbelohde (e.g., 5.7%,713 °K).
24
Rubidium Nitrite
[Refer: Table 113, p. 87, for numerical values]
The tabulated values of specific conductance for
molten RbNC>2 were calculated from the data of
Protsenko, Protsenko, and Razumovskaya [207]
(712 to 758 °K, 7 points). Using the quadratic equation for specific conductance the precision is
5 = 0.0025 (0.25%). The uncertainty of the specific
conductance values is estimated to be about (6%).
The tabulated values of viscosity have been cal
culated from the data of Protsenko, Protsenko, andRazumovskaya [207] (712 to 758 °K, 7 points,
capillary viscometer). The exponential equationexpresses the data with a precision 5 = 0.0054(0.28%). The uncertainty of the viscosity values
is considered to be about (1.0%).
Cesium Nitrite
[Refer: Table 114, p. 87, for numerical values]
The tabulated values of specific conductance for
molten CsN02 were calculated from the data of
Protsenko, Protsenko, and Razumovskaya [207](688 to 739 °K, 9 points). Using the linear equation for
specific conductance the precision is 5 = 7.41 • 104
(0.096%). The uncertainty of the specific conductance values is estimated to be about (6%).The tabulated values of viscosity have been cal
culated from the data of Protsenko, Protsenko,and Razumovskaya [207] (688 to 739 °K, 9 points,
capillary viscometer). The cubic equation expressesthe data with a precision 5 = 0.0080 (0.39%). Theuncertainty of the viscosity values is considered to
be about (1.0%).
Barium Nitrite
[Refer: Table 115, p. 87, for numerical values]
The tabulated values of specific conductance for
molten Ba(N02)2 were calculated from the data ofProtsenko and Shokina [185] (553.2 and 573.2 °K,
2 points). Only a linear equation for specific conductance was used to calculate the values. Theuncertainty of the specific conductance values is
estimated to be about (6%).The exponential equation expresses the tabu
lated values of equivalent conductance with a precision 5 = 0.0601 (0.80%).The data of Protsenko and Malakhova [173] were
used to calculate the densities; no estimate of accuracy was attempted owing to the limited information.
Lithium Nitrate
[Refer: Table 116, p. 88, for numerical values]
Five investigations of the specific conductancefor molten LiNCL have been reported [26, 93, 116,
194, 224]. The tabulated values were calculated
from the quadratic equation reported by King andDuke [116] (558 to 653 °K). Using the quadratic
equation the precision is 5 = 0.001 (0.083%). Compared to the data of King and Duke [116], the re
sults of de Nooijer and Ketelaar [224] , Doucet andBizouard [93], Cowen and Axon [194] and Jaeger
and Kapma [26] show maximum departures of
0.4 percent (631 °K), —0.9 percent (579.8 °K), —0.8percent (573 °K) and 0.9 percent (640 °K) respec
tively. The uncertainty of the specific conductancevalues is estimated to be about 0.4 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.326 (0.60%).
Three density studies have been reported [26,
180, 224]. The density data of Jaeger and Kapma[26] were selected to generate the tabulated values.
The more recent results of Smith and Petersen
[180] and de Nooijer and Ketelaar [224] are in
good agreement with the data of Jaeger, the agree
ment being better than 0.1 percent over the entire
temperature range.
Four investigations of the viscosity have beenreported [5, 38, 139, 228]. The results of Dantuma[38] (533.2 to 702.2 °K, 37 points, oscillating ball
technique) appear to be the most thorough. Themore recent investigation of Murgulescu and Zuca[139] lacks details on the preparation, purity
and melting point of the salt. Protsenko andRazumovskaya [228] reported a higher (5 degrees)
melting point for LiNO:? and lower melting points
for the other alkali nitrates (except KNO:i ), silver
nitrate and thallous nitrate than the generally
accepted values; this may imply an error in ther
mometry and/or impurities in the salts. Goodwinand Mailey [5] reported a lower melting point for
LiNO.j.
Judging from the above considerations and in
view of the most precise work for the other nitrates
(NaNO.j and KNCG) the data of Dantuma wereselected to calculate the tabulated values. Using
the cubic equation for viscosity the precision is
5 = 0.1143 (3.12%). The uncertainty of the viscosity
values is estimated to be about 3.5 percent.
The investigator, reference, experimental methodand the maximum percent departure are as follows:
Goodwin and Mailey [5], vertical capillary, —24percent; Murgulescu and Zuca [139]. oscillating
ball,— 14 percent; and Protsenko and Razumovskaya[228], vertical capillary, — 23 percent.
Sodium Nitrate
[Refer: Table 117, p. 88, for numerical values]
Ten investigations of the specific conductancefor molten NaNO.3 have been reported [7, 26, 27,61, 66, 71, 75, 93, 192, 224], The tabulated valueswere calculated from the data of Byrne et al. [61](583.2 to 643.2 °K, 7 points) and Lorenz and Kalmus[7] (591.2 to 691.2 °K, 11 points). Using the linear
25
equation for specific conductance the precision is
5 = 7.83 • 104 (0.06%). Compared to the data of
Lorenz [7] the results of Byrne [61], de Nooijer andKetelaar [224] and Sandonnini [27] show maximumdepartures of 0.4 percent (633 °K), 0.6 percent (694
°K) and 0.9 percent (623 °K) respectively; the results
of the other investigators show larger departures.
The uncertainty of the specific conductance values
is estimated to be about 1.0 percent.
The exponential equation expresses the tabu
lated values of equivalent conductance with a pre
cision 5 = 0.0160 (0.028%).
Of the four density studies [15, 26, 61, 66], the
data of Bloom et al. [66] and Byrne [61] were se
lected to generate the tabulated values. The den
sity equation has been calculated from the average
of the coefficients of the linear density equations
reported by Bloom [66] and Byrne [61]. Comparedto the combined data of Bloom [66] and Byrne
[61] the results of Jaeger [26] and Lorenz, Frei, andJabs [15] show maximum departures of 0.7 percent
(700 °K) and 0.1 percent (673 °K) respectively. Theuncertainty of the density values is judged to beabout 1 percent.
Six investigations of the viscosity have been re
ported [5, 8, 12, 38, 102, 228]. The tabulated values
were calculated from the data of Dantuma [38] (589.2
to 731.2 °K, 33 points, oscillating ball technique).
The exponential equation expresses the data of
Dantuma with a precision 5 = 0.0284 (1.41%). Thedepartures of various viscosity determinations of
NaN03 from the values of Dantuma are presentedin figure 2. The estimated uncertainty of the vis
cosity values is about 1.5 percent.
Figure 2. Comparison of percent departure of the data ofvarious investigators with the Dantuma viscosity data for NaN03
Base lineDantuma [38]a Goodwin and Mailey [5]o Lorenz and Kalmus [8]o Fawsitt [12]v Murgulescu and Zuca [102]
1 he results of Protsenko and Razumovskaya [228] show departures of up to —0.4 percent from the base line.
The investigator, reference, experimental method,and the maximum percent departure from the values
of Dantuma are as follows: Goodwin and Mailey [5],
vertical capillary, —4.3 percent; Lorenz and Kal
mus [8], horizontal capillary, + 3.9 percent; Fawsitt
[12], oscillating disk, +3.6 percent; Murgulescuand Zuca [102], oscillating ball, —2.1 percent; andProtsenko and Razumovskaya [228], vertical capil
lary. — 0.4 percent.
The uncertainty of the viscosity of NaN03 couldbe greater than 3.0 percent at higher temperaturesdue to partial decomposition of the melt. All the
investigations of NaN03 were carried out in a
normal atmosphere; the agreement was good be
tween the different methods. If decomposition oc
curred in the melt it does not appear significantly
greater in any one method. While molten NaN03
undergoes decomposition at elevated temperatures(>660 °K) it has been generally used as a calibra
tion fluid for high temperature viscosity studies.
Potassium Nitrate
[Refer: Table 118, p. 89, for numerical values]
Twelve investigations of the specific conduct
ance for molten KN03 have been reported [7, 20.
26, 27, 66, 84, 92, 116, 192, 193, 194, 224]. Thetabulated values were calculated from the data of
Aten [20] (613.2 to 773.2 °K, 9 points) and Bloomet al. [66] (800 to 880 °K, 5 points, gained fromBloom’s exponential equation at 20 deg intervals).
Using the quadratic equation for specific conduct
ance the precision is 5 = 0.00369 (0.37%). Comparedto the data of Aten [20] and Bloom et al. [66]
,
the results of King and Duke [116], Sandonnini
[27], and Lorenz and Kalmus [7] show maximumdepartures of 0.3 percent (620 °K), —0.2 percent
(673 °K) and —1.6 percent (686 °K) respectively.
The departures of the various specific conductancedeterminations of KN03 from the tabulated values
are in figure 3A. The uncertainty of the tabulated
specific conductance values is estimated to be
about 0.8 percent.
Values of specific conductance (5 = 8. 10“+ 0.1%)for the temperature range 623 to 698 °K should becalculated from the following equation reported
by Duke [116]: k = 2.4566 + 6.72893 • 103r— 2.7583 • lO 6 /
12. The uncertainty of the specific
conductance values calculated from the equation
of Duke [116] is estimated to be about 0.3 percent.
The data of Duke [116] appears highly suitable for
a high temperature calibration reference standard.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0832 (0.14%).
Of the ten density studies [15, 26, 38, 66, 84,
173, 177, 184, 192, 210] the data of Bloom et al. [66]
were selected to calculate the tabulated values.
Compared to the density data of Bloom et al. [66]
the results of other investigators are as follows:
Dantuma [38], —0.2 percent (660 °K); Smith and
26
FIGURE 3. Comparison of percent departures of the data forKNOs
A. Specific Conductance: B. Viscosity:
Base Line — Aten [20] and Base Line — Dantuma [38]
Bloom [66] a Goodwin and Mailey [5]
a Angell [193] 0 iLorenz and Kalmus [8]
de Nooijer and Ketelaar[224] o Fawsitt [12]
Jaeger and Kapma [26] o Ogawa [57]
a King and Duke [116] v Murgulescu and Zuca [102]o Aten [20] O Janz and Saegusa [107]
7 Bloom, Knaggs, Molloy The results of Protsenko andand Welch [66] Razumovskaya [228] show
O Murgulescu and Zuca [192] departures of up to + 0.5• Smith and van Artsdalen [84] percent from the base line.
van Artsdalen [84], 0.2 percent (620 °K); Protsenkoand Malakhova [173], 0.3 percent (673 °K);Murgulescu and Zuca [192], 0.2 percent (673 °K);and Polyakov and Berul [184], — 0.4 percent(713 to 773 °K). The uncertainty of the density valuesis judged to be about 0.2 percent.
Eight investigations of the viscosity have been re
ported [5, 8, 12 , 38, 57, 102, 107, 228]. The tabulated
values of viscosity were calculated from the dataof Dantuma [38] (671.2 to 815.2 °K, 35 points, oscil
lating ball technique). The cubic equation expressesthe data with a precision 5 = 0.0234 (1.38%). Thedepartures of the various viscosity determinationsof KNO3 from the values of Dantuma are presentedin figure 3B. The uncertainty of the viscosity datais estimated to be about 1.5 percent.
The investigator, reference, experimental method,and the maximum percent departure from the values
of Dantuma are as follows: Goodwin and Mailey
[5], vertical capillary, —2.9 percent; Lorenz andKalmus [8 ], horizontal capillary, +2.5 percent;
Fawsitt [ 12 ], oscillating disk, — 2.8 percent;
Ogawa [57], restricted falling sphere, —2.4 per
cent; Murgulescu and Zuca [ 102 ], oscillating ball,
— 1.4 percent; Janz and Saegusa [107], oscillating
hollow sphere, —0.9 percent; and Protsenko andRazumovskaya [228], vertical capillary, +0.5percent.
The uncertainty of the viscosity of KNO3 couldbe greater than 2.7 percent at higher temperaturesdue to partial decomposition of the melt. All the
investigations of KN03 were carried out in a normalatmosphere; the agreement was good between the
different methods. Hence if decomposition occurredin the melt, it does not appear significantly greater
in any one method. While molten KN03 decomposesat elevated temperature (>780 °K), it has beenused as a high temperature viscosity calibration
fluid.
Rubidium Nitrate
[Refer: Table 119, p. 89, for numerical values]
Two investigations of the specific conductancefor molten RbN03 have been reported [26, 224],
The tabulated values were calculated from the
data of Jaeger and Kapma [26] (592.0 to 766.2 °K,
12 points). Using the quadratic equation for spe
cific conductance the precision is s = 0.00153
(0.25%). The uncertainty of the specific conduct
ance values is estimated to be about 6 percent.
De Nooijer and Ketelaar [224] report results for
the specific conductance for the temperature range
588.6 to 724.0 °K (10 points) which fall within the
limits of the above accuracy estimate.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.226 (0.57%).
The density data of Jaeger and Kapma [26] wereused to calculate the tabulated values; no estimate
of accuracy was attempted owing to the limited
information.
Two investigations of the viscosity have beenreported [139, 228], The tabulated values were calcu
lated from the data of Murgulescu and Zuca [139]
(623 to 698 °K, 5 points, oscillating ball technique).
The cubic equation expresses the data with a pre
cision 5 = 0.00717 (0.25%). The uncertainty of the
viscosity values is estimated to be about 1.0 percent.
The results of the second study (Protsenko andRazumovskaya [228], vertical capillary viscometer),
are consistently lower (about 7%) than those of
Murgulescu and Zuca. Protsenko reported a lowermelting point (158 °K) for RbNO :! than the generallyaccepted value (589 °K).
297268 068—327
Cesium Nitrate
[Refer: Table 120, p. 90, for numerical values]
Three investigations of the specific conductancefor molten CsNO,3 have been reported [26, 84,
224] . The tabulated values were calculated fromthe linear equation reported by van Artsdalen [84]
for the temperature range of 688.2 to 764.2 °K. Noprecision was reported. Compared to the data of
van Artsdalen the results of de Nooijer and Ketelaar
[224] and Jaeger and Kapma [26] show maximumdepartures of 0.5 percent (735 °K) and — 2.0 percent
(745.9 °K) respectively. The uncertainty of the spe
cific conductance values is estimated to be about
0.6 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.00503 (0.019%).
Of the two density studies [26, 84] the data of
van Artsdalen [84] were selected to calculate the
tabulated values. The maximum departure betweenthe densities reported by van Artsdalen [84] andJaeger [26] is 0.15 percent (780 °K). The uncer
tainty of the density values is judged to be about
0.15 percent.
Two investigations of the viscosity have beenreported
[139, 228]. The tabulated values were
calculated from the data of Protsenko and Razumovskaya [228] (698.2 to 776.2 °K, 15 points, vertical
capillary viscometer). Using the cubic equation
for viscosity the precision is s = 0.0033 (0.18%).
The uncertainty of the viscosity values is judged
to be about 4.5 percent.
The study of Murgulescu and Zuca [138] (oscillat
ing ball method) is limited to one temperature; their
value (2.43 cp, at 698 °K) is higher (12.5%) than
those of Protsenko and Razumovskaya.
Silver Nitrate
[Refer: Table 121, p. 90, for numerical values]
Eight investigations of the specific conductancefor molten AgNCU have been reported [5, 60, 78,
135, 181, 194, 219, 224]. The tabulated values werecalculated from the data of Spooner and Wetmore[60] (483.2 to 603.2 °K, 13 points). Using the quadratic equation for specific conductance the precision
is 5=1.11 • 10 3 (0.12%). Compared to the data of
Spooner and Wetmore the results of other investi
gators show the following maximum departures:Goodwin and Mailey [5] —1.0 percent (526 °K);
de Nooijer and Ketelaar [226], — 1.0 percent (523 °K);
Polyakov [78], — 1.7 percent (513 °K); Bizouard [181],
0.2 percent (573 °K); Duke and Fleming [135], — 1.6
percent (598 °K); the results of Sundheim and Berlin
[219], and Cowen and Axon [194] show larger departures. The uncertainty of the specific conductancevalues is estimated to be about 1 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.178 (0.45%).
Of the five density studies [25, 36, 54, 60, 224] the
data of Jaeger [25] were selected to calculate the
tabulated values. Compared to the density data of
Jaeger [25] the results of Klemm [36], Spooner andWetmore [60], Boardman et al. [54] and de Nooijerand Ketelaar [224] show maximum departures of— 0.1 percent (600 °K), — 0.4 percent (500 °K), — 0.4
percent (600 °K), and 1.5 percent (548 °K) respec
tively. The uncertainty of the density values is
judged to be about 0.3 percent.
Five investigations of the viscosity have been re
ported [5, 65, 69, 219, 228]. The tabulated values
were calculated from the data of Pugsley and Wetmore [69] (530.0 to 593.4 °K, 13 points, Ostwaldviscometer). The cubic equation for viscosity ex
presses the data with a precision 5 = 0.0054 (0.18%).
The uncertainty of the viscosity data is estimated
to be about 1.0 percent.
The investigator, reference, experimental method,and the maximum percent departure from the values
of Pugsley and Wetmore are as follows: Goodwinand Mailey [5], vertical capillary viscometer, —5.3percent; and Davis, Rogers, and Ubbelohde [65],
Ostwald type viscometer, —30 percent; Sundheimand Berlin [219], Ostwald type viscometer, 8.6
percent; and Protsenko and Razumovskaya [228],
vertical capillary, +3.4 percent.
Thallium (I) Nitrate
[Refer: Table 122, p. 91, for numerical values]
Seven investigations of the specific conductance
for molten TINO3 have been reported [110, 125c,
191, 215, 216, 217, 219, 224]. The tabulated values
were calculated from the data of Janz and Timidei
[191] (485.5 to 554.5 °K, 17 points). Using the linear
equation for specific conductance the precision is
5 = 9.59 10 4 (0.212%). Compared to the data of
Janz and Timidei [191] the results of other investi
gators show the following maximum departures:
Frame, Rhodes and Ubbelohde [110, 125c], 1.0 per
cent (524.4 °K); Sundheim and Berlin [219], 0.7 per
cent (491.9 °K); Bergman and Chagin [215], 5.9
percent (498 °K); and Bokhovkin [216], —4.6 per
cent (523 °K, 548 °K). Brillant [217] claims agreementwith Ubbelohde but the results are insufficiently
reported for a critical evaluation. The uncertainty
of the specific conductance values is estimated to
be about 0.7 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0843(0.35%).
Of the two density studies [25, 191], the data of
Janz [191] were selected to calculate the tabulated
values. The maximum departure between the densi
ties reported by Jaeger [25] and Janz [191] is 0.18
percent (552.6 °K). The estimated uncertainty of the
density values is about 0.15 percent.
28
Four investigations of the viscosity have been re
ported [110, 191, 219, 228]. The tabulated values
were calculated from the data of Janz and Timidei
[191] (492.5 to 553.7 °K, 16 points, modified Martinvsicometer). The cubic equation expresses the data
of Janz and Timidei with a precision 5 = 0.00876(0.31%). The uncertainty of the data is judged to beabout 1.0 percent.
The investigator, reference, experimental methodand the maximum percent deviation from the valuesof Janz and Timidei are as follows: Frame, Rhodes,and Ubbelohde [110], Ubbelohde viscometer, 5.3
percent; Sundheim and Berlin [219], Ostwald vis
cometer, 7.1 percent: and Protsenko and Razumovskaya [228], vertical capillary viscometer,
+ 12.0 percent.
Vanadium Pentoxide and Chromium Trioxide
[Refer: Tables 123 to 124, p. 91, for numericalvalues]
The tabulated values of specific conductance for
molten V2O5 and Cr03 were calculated from the
data of van Arkel, Flood and Bright [68]. The numberof data points, the temperature range, the precision
and the best equation are as follows:
V205  8 points, 1 1401237 °K,
5 = 0.00575(2.87%), linear equation.
Cr03 — 7 points, 491535 °K,
5 = 3.31 • 10 7 (0.007%), quadratic equation.
Molybdenum Trioxide
[Refer: Table 125, p. 91, for numerical values]
Two investigations of the specific conductance for
molten Mo03 have been reported [68, 76]. The tabu
lated values were calculated from the data of Morriset al. [76] (1096 to 1187 °K, 5 points). The exponentialequation for specific conductance expresses thedata of Morris with a precision 5 = 0.00208 (0.22%).The maximum departure between the specific conductance values of Morris [76] and van Arkel [68]
is 58 percent (1168 °K). The uncertainty of thespecific conductance values is estimated to be about60 percent.
Wiistite (Feo.asO)
[Refer: Table 126, p. 92, for numerical values]
The tabulated values of specific conductance for
molten FeO were calculated from the data of Inouye,Tomlinson and Chipman [159] (1648 to 1773 °K).
To cover the entire range it became necessary to
generate two equations; the number of data points,the temperature range, the precision appropriateto this subdivision are as follows:
quadratic equation; 5 points, 16481713 °K,
5=16.1 (6.0%)linear equation; 5 points, 17131773 °K,
5=1.18 (0.37%)
Liquid wiistite is a nonstoichiometric melt since anincrease in temperature above the melting pointresults in an increase in the Fe/O ratio although thelatter remains less than unity. Chipman [159] hasestimated an overall error of less than 8 percent for
his results. No estimate of the accuracy wasattempted owing to the limited information.
Boron Oxide
[Refer: Table 127, p. 92, for numerical values]
Two investigations of the density for molten B 203
have been reported [144, 201]. The density data of
Reibling [144] (1410 to 1890 °K, 14 points) wereselected to calculate the tabulated values. Usingthe quadratic equation for density the precision is
5=1.11 * 10 —
3
(0.074%). The maximum departure
between the densities reported by Riebling [144] andNapolitano, Macedo and Hawkins [201] is 0.82 per
cent (1473 °K). The estimated uncertainty of the
density values is about 0.8 percent. Densities
(5 = 4.52 • 10 3 (0.28%)) in the range 723 to 1400 °Kcan be gained from the following quadratic equation
based on the data of Napolitano [201] (723 to 1673
°K, 12 points):
p = 2.03833 6.67971 • 10 4T 2.08005 • 10~ 7r2.
Six investigations of the viscosity have been re
ported [137, 144, 145, 200, 201, 209, 222]. The tabu
lated values were calculated from the data of
Riebling [137] (1410 to 1893 °K, 14 points, restricted
falling ball viscometer). The cubic equation ex
presses the data of Riebling with a precision 5 = 70.8
(3.27%). The uncertainty of the viscosity values is
estimated to be about 5.0 percent.
The investigator, reference, temperature range
studied, experimental method and the departure
from the values of Riebling [137] are as follows:
Riebling [222] 1303 to 1583 °K, restricted falling ball,
+ 20 percent at 1550 °K; Arndt [200], 1023 to 1388 °K,
restricted falling ball, —30 percent at 1410 °K(extrapolated); Napolitano, Macedo, and Hawkins[201], 730 to 1677 °K, concentric cylinder technique,— 90 percent at 1677 °K; Li, Ghose, and Su [209],
784 to 1516 °K, concentric cylinder technique, —8percent at 1516 °K; Mackenzie [145], 786 to 1309 °K,
restricted falling ball viscometer, extrapolated
values of Mackenzie agree with those of Riebling
[137] (1% at 1410 °K).
Silicon Dioxide
[Refer; Table 128, p. 93, for numerical values]
Two investigations of the viscosity for molten
Si02 have been reported [205, 206]. The tabulated
values were calculated from the data of Bacon,
Hasapis, and Wholley [205] (2208 to 2595 °K, 12
points, restricted falling ball viscometer). The cubic
equation expresses the data of Bacon, Hasapis, andWholley with a precision 5 = 55,900 (49.3%). Theuncertainty of the viscosity values is estimated to
be about 60 percent.
The viscosities of the second study (Bockris,
Mackenzie, and Kitchener [206]; torque viscometer)
are consistently lower than those of Bacon, Hasapis,
and Wholley (e.g., 84% at 2210 °K; 90% at 2330 °K).
Germanium Dioxide
[Refer: Table 129, p. 93, for numerical values]
Two investigations of the specific conductancefor molten GeC>2 have been reported [146, 163].
The tabulated values were calculated from the
exponential equation reported by Riebling andGabelnick [163] (1389 to 1623 °K). No precision wasgiven. Comparison of the data of Riebling [163] andMackenzie [146] shows the maximum departure to
be 60 percent (1523 °K). The uncertainty of the
specific conductance values is estimated to beabout 20 percent.
Three investigations of the viscosity have beenreported [137, 140, 141, 146]. The tabulated values
were calculated from the combined data of Kurkjian
and Douglas [140] (1423 to 1773 °K, 8 points, con
centric cylinder viscometer) and Riebling [137]
(1745 to 1991 °K, 28 points, restricted falling ball
viscometer). The exponential equation generatedfrom the data of Kurkjian and Douglas expressesthe viscosity values in the range 1430 to 1750 °Kwith a precision s — 7.61 • 105 (41.6%) and the uncer
tainty of the data is considered to be about 50 per
cent, while the exponential equation from the data
of Riebling expresses the viscosities in the range1760 to 1990 °K with a precision 5 = 8376 (10.4%)and the uncertainty of the data is estimated to beabout 15 percent. The values generated fromRiebling’s data are higher than those of Kurkjianand Douglas in the region of overlap (e.g., 7.6%,1750 °K, 10.7%, 1770 °K).
The results of the third study (Mackenzie [146];
counter balance viscometer) are consistently higher
than those of Kurkjian and Douglas, and Riebling
(e.g., 100%, 1623 °K; 123%, 1823 °K).
Lead Oxide
[Refer: Table 130, p. 94, for numerical values]
The tabulated values of specific conductance for
molten PbO were calculated from the data of van
Arkel, Flood and Bright [68] (1164 to 1260 °K, 9
points). The exponential equation for specific
conductance expresses the data with a precision
5 = 0.010 (0.55%). No estimate of accuracy wasattempted owing to the limited information.
Arsenic Trioxide
[Refer: Table 131, p. 94, for numerical values]
The tabulated values of viscosity for molten AS2O3were calculated from the data of Karutz and Stran
ski [202] (601.1 to 702.9 °K, 6 points, restricted
falling ball viscometer). The exponential equationexpresses the data with a precision 5 = 7,681.9
(1.76%). No estimate of accuracy was attemptedowing to the limited information.
Antimony Sesquioxide, Bismuth Sesquioxide,and Tellurium Dioxide
[Refer: Tables 132 to 134, pp. 94 to 95, for numericalvalues]
The tabulated values of specific conductance for
molten Sb20 3 , Bi20 3 and Te02 were calculated fromthe data of van Arkel, Flood and Bright [68]. Thenumber of data points, the temperature range, the
precision and the best equation are as follows:
Sb203 — 6 points, 11011161 °K,
5 = 0.0038 (3.0%), linear equation.
Bi203— 18 points, 11021228 °K,
5 = 0.0816 (11.5%), linear equation.
Te0 2— 18 points, 10231233 °K,
5 = 0.0384 (2.0%), exponential equation.
Iron (II) Sulfide
[Refer: Table 135, p. 95, for numerical values]
Two investigations of the specific conductance for
molten FeS have been reported [153, 154, 155].
The tabulated values were calculated from the
quadratic specific conductance equation reported
by Velikanov [154, 155] for the temperature range1469.2 to 1493.2 °K. Neither the precision nor the
experimental data were given. Argyriades, Dergeand Pound [153] reported a value of 400 0 1cm _1
(1473.2 °K) for the specific conductance of iron sul
fide; this value is 72 percent lower than that of
Velikanov [155]. The uncertainty of the specific
conductance values is estimated to be about 50percent.
Cobalt (II) Sulfide
[Refer: Table 136, p. 95, for numerical values]
The tabulated values of specific conductance for
molten CoS were calculated from the graphicaldata of Velikanov [155] (1461.2 to 1497.2 °K, 5points). The data points, interpolated from Velikanov’s graph, were least squared to develop theexponential equation. The uncertainty of the specific
conductance values is estimated to be about (50%).
30
Nickel (II) Sulfide
[Refer: Table 137, p. 95, for numerical values]
The tabulated values of specific conductance for
molten NiS were calculated from the quadratic
equation reported by Velikanov [154] for the tem
perature range 1153.2 to 1398.2 °K. Neither the
precision nor the experimental data were given.
The uncertainty of the specific conductance values
is estimated to be about (50%).
Copper (I) Sulfide
[Refer: Table 138, p. 96, for numerical values]
Two investigations of the specific conductancefor molten Cu2S have been reported [155, 152]. Thetabulated values were calculated from the data of
Velikanov [155] (1402.2 to 1523.3 °K, 10 points).
Using the quadratic equation for specific conduct
ance the precision is s— 1.44 (2.3%). The maximumdeparture between the results of Velikanov [155]
and Bourgon, Derge and Pound [152] is 33 percent.
The uncertainty of the specific conductance values
is estimated to be about 40 percent.
Silver Sulfide
[Refer: Table 139, p. 96, for numerical values]
Two investigations of the specific conductance
for molten Ag2S have been reported [156, 166].
The tabulated values were calculated from the data
of Velikanov [156] (1105.2 to 1352.2 °K, 12 points).
Using the exponential equation for specific conduct
ance the precision is 5 = 0.783 (0.66%). The maxi
mum departure between the results of Velikanov
[155] and Bell and Flengas [166] is 70 percent (1233
°K). The uncertainty of the specific conductancevalues is estimated to be about 50 percent.
H
Germanium (II) Sulfide
[Refer: Table 140, p. 96, for numerical values]
The tabulated values of specific conductance for
molten GeS were calculated from the data of
Velikanov [155] (873.2 to 1073.2 °K, 3 points). Thequadratic equation expresses the data with an exact
fit. The uncertainty of the specific conductancevalues is estimated to be about (50%).
Tin (II) Sulfide
[Refer: Table 141, p. 97, for numerical values]
The tabulated values of specific conductance for
molten SnS were calculated from the data of
Velikanov [155] (1158.2 to 1411.2 °K, 13 points).
Using the quadratic equation for specific conduct
ance the precision is 5 = 0.363 (1%). The uncertainty
of the specific conductance values is estimated to
be about (50%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=18.2 (1.4%).
The density data of Velikanov [158] were used to
calculate the tabulated values; no estimate of accu
racy was attempted owing to the limited information.
Lead Sulfide
[Refer: Table 142, p. 97, for numerical values]
Two investigations of the specific conductancefor molten PbS have been reported [151, 154, 155].
The tabulated values were calculated from the
quadratic equation reported by Velikanov [154, 155]
for the temperature range 1388.2 to 1490.2 °K.
Neither the precision nor the experimental data
were given. The maximum departure between the
results of Velikanov [154] and Bell and Flengas [151]
is 22 percent (1420 °K). The uncertainty of the spe
cific conductance values is estimated to be about
20 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=12.3(0.66%).The data of Bell and Flengas [150] were used to
calculate the densities; no estimate of accuracywas attempted owing to the limited information.
Antimony (III) Sulfide
[Refer: Table 143, p. 98, for numerical values]
The tabulated values of the specific conductancefor molten Sb 2S3 were calculated from the data of
Velikanov [155] (830.2 to 1076.2 °K, 13 points). Usingthe quadratic equation for specific conductance the
precision is 5 = 0.00901 (1.7%). The uncertainty of
the specific conductance values is estimated to beabout (50%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.247(1.4%).
The density data of Velikanov [158] were used to
calculate the tabulated values; no estimate of accu
racy was attempted owing to the limited information.
Bismuth (III) Sulfide
[Refer: Table 144, p. 98, for numerical values]
The tabulated values of the specific conductancefor molten Bi2S 3 were calculated from the data of
Velikanov [157] (973.2 to 1198.2 °K, 10 points). Usingthe linear equation for specific conductance the
precision is 5 = 4.87 (0.12%). The accuracy of the
specific conductance values has not been estimated
due to unreliability of the data. Since the measure
31
merits were carried out in an atmosphere of air, the
decomposition of sulfides may have resulted in the
formation of metal molten sulfide solutions; a small
increase in the metal content of many sulfide melts,
in which electronic as well as ionic conduction is
known to occur, causes a large increase in the elec
trical conductance.The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=10.6 (0.012%).
The density data of Velikanov [158] were used to
calculate the tabulated values; no estimate of accu
racy was attempted owing to the limited information.
Lithium Sulfate
[Refer: Table 145, p. 99, for numerical values]
The tabulated values of specific conductance for
molten Li2S04 were calculated from the quadratic
specific conductance equation (converted to abso
lute temperature scale) reported by Kvist andLunden [115] for the temperature range of 848.3 to
1243.2 °K. No precision was given by Kvist andLunden. The uncertainty of the specific conductance values is estimated to be about (5%).The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.482 (0.42%).
The density data of Jaeger [25] were used to calcu
late the tabulated values. The uncertainty of the
density values is judged to be about (1%).
Sodium Sulfate
[Refer: Table 146, p. 99, for numerical values]
Two investigations of the specific conductance for
molten Na2S04 have been reported [4, 226]. Thetabulated values were calculated from the data of
Kvist [226] (1189.2 to 1232.0 °K, 4 points). Using the
exponential equation for specific conductance the
precision is 5 = 0.00119 (0.05%). The specific con
ductance values of Arndt [4] are all lower than those
of Kvist; the maximum departure between their
values is 4.5 percent (1220 °K). The uncertainty of
the specific conductance values is estimated to be
2 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0077 (0.0092%).
The density data of Jaeger [25] were used to calcu
late the tabulated values. The uncertainty of the
density values is judged to be about (1%).
Potassium Sulfate
[Refer: Table 147, p. 99, for numerical values]
Two investigations of the specific conductance for
molten K2S0 4 have been reported [4, 161]. The
tabulated values were calculated from the data of
Kvist [161] (1341.5 to 1359.6 °K, 7 points). Using the
quadratic equation for specific conductance the
precision is 5 = 0.00259 (0.13%). The specific con
ductance value of Arndt [4] (1373.2 °K) is lower
(5.6%, 1372.2 °K) than that of Kvist [161]. The uncer
tainty of the specific conductance values is esti
mated to be about 3 percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.070 (0.05%).
Of the two density studies [25, 178] the data of
Neithamer and Peake [178] were selected to calcu
late the tabulated values. The maximum departure
between the density data of Jaeger [25] and Peake
[178] is 0.96 percent (1350 °K). The uncertainty of
the density values is judged to be about 0.4 percent.
For temperatures above 1450 °K densities may becalculated using the following equation based onthe data of Jaeger [25] (1343 to 1929 °K, 15 points):
p =  0.900 + 2.00 • io 3r.
Rubidium Sulfate
[Refer: Table 148, p. 99, for numerical values]
The tabulated values of specific conductance for
molten RtoSCL were calculated from the data of
Kvist [226] (1340.2 to 1395.2 °K, 8 points). Theexponential equation for specific conductanceexpresses the data with a precision 5=0.00183(0.13%). The uncertainty of the specific conductancevalues is estimated to be (3%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.00709 (0.0093%).
The tabulated values of density were calculated
from the density equation reported by Jaeger [25].
The uncertainty of the density values is estimated
to be about (1%).
Cesium Sulfate
[Refer: Table 149a, p. 100, for numerical values]
The tabulated values of specific conductance for
molten Cs2S04 were calculated from the data of
Kvist [226] (1286.7 to 1354.7 °K, 6 points). Thelinear equation for specific conductance expresses
the data with a precision 5 = 0.0035 (0.30%). Theuncertainty of the specific conductance values is
estimated to be (3%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0223 (0.032%).
The tabulated values of density were calculated
from the density equation reported by Jaeger [25].
The uncertainty of the density values is estimated
to be about (1%).
32
Silver Sulfate
[Refer: Table 149b, p. 100, for numerical values]
The tabulated values of specific conductance for
molten Ag2S04 were calculated from the data of
Kvist [226] (942.0 to 1017.4 °K, 6 points). Theexponential equation for specific conductanceexpresses the data with a precision 5 = 0.00203
(0.11%). The uncertainty of the specific conductancevalues is estimated to be (3%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0067 (0.018%).
The tabulated values of density were calculated
from the density equation reported by Kvist [226].
The uncertainty of the density values is estimated to
be about (0.8%).
Tetrapropylammonium Tetrafluoroborate
[Refer: Table 150, p. 100, for numerical values]
The tabulated values of specific conductance for
molten PrjNBF4 were calculated from the data of
Lind, AbdelRehim and Rudich [190, 221] (522.73
to 554.58 °K, 16 points). Using the exponential
equation for specific conductance the precision is
5= 1.88 • 103 (1.7%). The uncertainty of the specific
conductance values is estimated to be about (10%)(see discussion for Bu4 NI).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0108(0.035%).The density data of Lind [190, 221] (525.6 to
547.3 °K, 14 points) were used to calculate the
tabulated values. The uncertainty of the density
values is judged to be about (1%).
The tabulated values of viscosity were calculated
from the data of Lind, AbdelRehim and Rudich[190, 221] (522.8 to 546.7 °K, 5 points, capillary
viscometer). The cubic equation expresses the data
with a precision 5 = 0.00032 (0.017%). While the
information is insufficient to estimate the accuracy,
the data can be considered reliable.
calculate the tabulated values. The uncertainty of
the density values is estimated to be about (1%).
The tabulated values of viscosity were calculatedfrom the data of Lind, AbdelRehim, and Rudich[190, 221] (517.5 to 541.9 °K, 5 points, capillary
viscometer). The cubic equation expresses the
data with a precision 5 = 0.00031 (0.012%). Whilethe information is insufficient to estimate the ac
curacy, the data can be considered reliable.
Tetrapropylammonium Tetraphenylborate
[Refer: Table 152, p. 101, for numerical values]
The density data of Lind, AbdelRehim andRudich [190, 221] for molten Fh^NBPfq were usedto calculate the tabulated values. The uncertaintyof the density values is estimated to be about (1%).
The tabulated values of viscosity were calculatedfrom the data of Lind, AbdelRehim, and Rudich[190, 221] (483.5 to 529.2 °K, 11 points, capillary
viscometer). The cubic equation expresses the datawith a precision 5 = 0.0166 (0.28%). While the infor
mation is insufficient to estimate the accuracy, the
data can be considered reliable.
Tetrabutylammonium Bromide
[Refer: Table 153, p. 101, for numerical values]
The tabulated values of specific conductance for
molten B^NBr were calculated from the data of
Lind, AbdelRehim and Rudich [190, 221] (390.3
to 407.7 °K, 7 points). Using the exponential equa
tion for specific conductance the precision is
5 = 9.42106(0.35%). The uncertainty of the
specific conductance values is estimated to beabout (7%) (see discussion for BojNI).
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision5=1.29 • 10 4 (0.017%).
The density data of Lind [190, 221] were used to
calculate the tabulated values. The uncertainty of
the density values is estimated to be about (1%).
Tetrapropylammonium Hexafluorophosphate
[Refer: Table 151, p. 100, for numerical values]
The tabulated values of specific conductance for
molten Pr4 NPFfi were calculated from the data of
Lind, AbdelRehim and Rudich [190, 221] (511.03
to 545.15 °K, 15 points). Using the exponentialequation for specific conductance the precision
is 5 = 8.86 • 105 (0.11%). The uncertainty of the
specific conductance values is estimated to beabout (6%) (see discussion for BuiNI).The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 3.24 • 10 3 (0.013%).The density data of Lind [190, 221] were used to
Tetrabutylammonium Iodide
[Refer: Table 154, p. 101, for numerical values]
Two investigations of the specific conductancefor molten BU4NI have been reported [190, 220,
221]. The tabulated values were calculated fromthe data of Lind, AbdelRehim and Rudich [190,
221] (420.70 to 440.13 °K, 13 points). Comparisonof the data of Walden and Birr [220] and Lind
[190, 221] shows the maximum departure to be2.4 percent (423 °K). Although the linear equation
for specific conductance expresses the data with a
precision 5 = 2.43 • 104 (3.6%), the reproducibility
is particularly poor near 428 °K (3.0% at 428.13 °Kand —7.6% at 428.66 °K). Lind attributes this poor
33
reproducibility to the decomposition of the salt.
The tetrafluoroborates are the most stable and the
halides are the least stable of the quaternary ammonium salts. The uncertainty of the specific
conductance values is estimated to be about 10
percent.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.047 (2.0%).
Of the two density studies [190, 220, 221], the
data of Lind [190, 221] were selected to calculate
the tabulated values. The maximum departure
between the densities reported by Lind [190, 221]
and Walden [220] is 1.0 percent (423.2 °K). Theestimated uncertainty of the density values is
1 percent.
Tetrabutylammonium Tetrafluoroborate
[Refer: Table 155, p. 101, for numerical values]
The tabulated values of density for molten
BU4NBF4 were calculated from the data of Lind,
AbdelRehim and Rudich [190, 221]. The uncertainty
of the density values is estimated to be about (1%).
The tabulated values of viscosity were calculated
from the data of Lind, AbdelRehim and Rudich
[190, 221] (435.4 to 539.1 °K, 17 points, capillary
viscometer). The cubic equation expresses the
data with a precision 5 = 0.0446 (1.22%). While the
information is insufficient to estimate the accuracy,
the data can be considered reliable.
Tetrabutylammonium Hexafluorophosphate
[Refer: Table 156, p. 102, for numerical values]
The tabulated values of specific conductance for
molten B114NPF6 were calculated from the data of
Lind, AbdelRehim and Rudich [190, 221] (529.5 to
548.5 °K, 5 points). Using the linear equation for
specific conductance the precision is 5= 1.06 • 104
(0.010%). The uncertainty of the specific conduc
tance values is estimated to be about (6%) (see
discussion for B114NI).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.041 (0.22%).
The density data of Lind [190, 221] were used to
calculate the tabulated values. The uncertainty of
the density values is estimated to be about (1%).
The tabulated values of viscosity were calculated
from the data of Lind, AbdelRehim, and Rudich[190, 221] (529.4 to 554.1 °K, 5 points, capillary
viscometer). The exponential equation expresses the
data with a precision 5 = 0.0035 (0.14%). While the
information is insufficient to estimate the accuracy,the data can be considered reliable.
Tetrabutylammonium Tetraphenylborate
[Refer: Table 157, p. 102, for numerical values]
The tabulated values of specific conductance for
molten BipNBPfp were calculated from the data of
Lind, AbdelRehim and Rudich [190, 221] (514.3
to 540.4 °K, 12 points). Using the exponential
equation for specific conductance the precision is
5=1.9510“ 5 (0.14%). The uncertainty of the
specific conductance values is estimated to beabout (6%) (see discussion for BipNI).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=1.62 • 10 3 (0.018%).
The density data of Lind [190, 221] were used to
calculate the tabulated values. The uncertainty of
the density values is estimated to be about (1%).
The tabulated values of viscosity were calculated
from the data of Lind, AbdelRehim, and Rudich[190, 221] (516.8 to 541.8 °K, 5 points, capillary
viscometer). The exponential equation expressesthe data with a precision 5 = 0.0064 (0.16%). Whilethe information is insufficient to estimate the
accuracy, the data can be considered reliable.
Tetrahexylammonium Tetrafluoroborate
[Refer: Table 158, p. 102, for numerical values]
The density data of Lind, AbdelRehim andRudich [190, 221] for molten HexiNBFt were usedto calculate the tabulated values. The uncertainty
of the density values is estimated to be about (1%).
The tabulated values of viscosity were calculated
from the data of Lind, AbdelRehim, and Rudich
[190, 221] (376.0 to 502.8 °K, 27 points, capillary
viscometer). The exponential equation expresses
the data with a precision 5 = 2.90 (20.7%). Whilethe information is insufficient to estimate the ac
curacy, the data can be considered reliable.
Tetranamvlammonium Thiocyanate
[Refer: Table 159, p. 102, for numerical values]
The tabulated values of specific conductance for
molten (namylfiNSCN were calculated from the
data of Kenausis, Evers and Kraus [172] (325.2
to 383.2, 7 points). The specific conductance values,
gained from the equivalent conductance anddensity data of Kraus [172] were least squared to
generate the quadratic equation. The precision is
5 = 2.77 • 10~5 (2.4%). No attempt to estimate the
accuracy was made owing to insufficient informa
tion; however, judging the experimental techniquesthe results can be considered reliable.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0532 (13%).
34
The density data of Kraus [172] (325.2 to 383.2,
7 points) were used to calculate the tabulated
values. No estimate of accuracy was attemptedowing to the limited information.
The tabulated values of viscosity were calculated
from the data of Kenausis, Evers, and Kraus [172]
(325.2 to 383.2 °K, 7 points, CannonUbbelohdeviscometer). The cubic equation expresses the
data with a precision 5 = 3.93 (5.18%). No estimate
of accuracy was made owing to the limitedinformation.
Lithium Molybdate
[Refer: Table 160, p. 103, for numerical values]
The tabulated values of specific conductance for
molten Li2Mo04 were calculated from the quadratic
equation reported by Kvist and Lunden [117] for
the temperature range 977 to 1223 °K. The precision
is 5 = 0.017 (0.79%). No estimate of accuracy wasattempted owing to the limited information.
Sodium Molybdate
[Refer: Table 161, p. 103, for numerical values]
The specific conductance of molten Na 2Mo04 hasbeen determined by Jaeger and Kapma [26] andMorris et al. [76] . The tabulated values were cal
culated from the data of Morris [76] (1024.2 to
1237.2 °K, 6 points). Using the quadratic equationfor specific conductance the precision is 5 = 0.00282(0.18%). The maximum departure between the spe
cific conductance values of Morris [76] and Jaeger
[26] is 13.6 percent (1198 °K). The uncertainty of
the specific conductance values is estimated to beabout 10 percent.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
5 = 0.142 (0.23%).
The density data of Jaeger and Kapma [26] wereused to calculate the tabulated values; no estimateof accuracy was attempted owing to the limited
information.
Potassium Molybdate
[Refer: Table 162, p. 104, for numerical values]
The tabulated values of density for molten K2M04
were calculated using the quadratic equation (after
conversion to the absolute temperature scale) givenby Jaeger [25] . No attempt to estimate the accuracywas made due to insufficient information.
Sodium Tungstate
[Refer: Table 163, p. 104, for numerical values]
The tabulated values of specific conductance for
molten Na2W04 were calculated from the data of
Jaeger and Kapma [26] (925.7 to 1774 °K, 11 points).
Using the quadratic equation for specific conductance the precision is 5 = 0.0064 (0.48%).
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.0352 (0.065%).
The density data of Jaeger and Kapma [26] wereused to calculate the tabulated values; no estimate
of accuracy was attempted owing to the limited
information.
Potassium Tungstate
[Refer: Table 164, p. 104, for numerical values]
The tabulated values of density for molten K2W04
were calculated using the quadratic equation (after
conversion to the absolute temperature scale) given
by Jaeger [25] . No attempt to estimate the accuracy
was made due to insufficient information.
Sodium Thiocyanate
[Refer: Table 165, p. 105, for numerical values]
The tabulated values of specific conductance for
molten NaSCN were calculated from the exponen
tial equation reported by Ubbelohde et al. [112].
Since the upper temperature limit was not given, it
was presumed that the equation is valid over the
temperature range cited for the viscosity studies bythe same authors [112]. Neither the precision nor
the experimental data was reported.
The tabulated values of viscosity were calculated
from the data of Plester, Rogers, and Ubbelohde
[112] (578.0 to 634.1 °K, 9 points, Ostwald viscom
eter). The cubic equation expresses the data with a
precision 5 = 0.0128 (0.57%). The uncertainty of the
viscosity values is estimated to be about (1.5%).
Potassium Thiocyanate
[Refer: Table 166, p. 105, for numerical values]
The tabulated values of specific conductance for
molten KSCN were calculated from the exponential
equation given by Plester, Rogers and Ubbelohde[112]. Since the upper temperature limit was not
reported, it was presumed that the equation is valid
over the temperature range cited for viscosity
studies by the same authors [112]. Neither the pre
cision nor the experimental data was reported.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5 = 0.00708(0.053%).The tabulated values of density were calculated
from the linear equation reported by Ubbelohde et
al. [110]. The upper temperature limit for this den
sity equation was not reported.
The tabulated values of viscosity were calculated
from the data of Plester, Rogers, and Ubbelohde
35
[112] (448.8 to 523.8 °K, 13 points, Ostwald viscom
eter). The cubic equation expresses the data with a
precision 5 = 0.0899 (1.33%). The uncertainty of the
viscosity values is estimated to be about (1.5%).
Sodium Hydroxide
[Refer: Table 167, p. 105, for numerical values]
The tabulated values of specific conductancefor molten NaOH were calculated from the linear
equation reported by Arndt and Ploetz [37] (593.2
to 723.2 °K). Neither the precision nor an accuracy
estimate can be gained owing to the limited infor
mation.
The exponential equation expresses the tabulated
values of equivalent conductance with a precision
5=0.0128 (0.020%).
The density data of Arndt and Ploetz [37] wereused to calculate the tabulated values; no estimate
of accuracy was attempted owing to the limited
information.
The tabulated values of viscosities were cal
culated from the data of Arndt and Ploetz [37]
(623.2 to 823.2 °K, 5 points, vertical capillary
viscometer). The cubic equation expresses the data
with a precision 5 = 0.0359 (1.66%). The uncertainty
of the viscosity values is estimated to be about
(1.5%).
Potassium Hydroxide
[Refer: Table 168, p. 106, for numerical values]
The tabulated values of specific conductancefor molten KOH were calculated from the linear
equation reported by Arndt and Ploetz [37] (673 to
873 °K). Neither the precision nor an accuracy
estimate can be gained owing to the limited infor
mation.
The exponential equation expresses the tabu
lated values of equivalent conductance with a
precision s — 0.490 (0.50%).
The density data of Arndt and Ploetz [37] wereused to calculate the tabulated values; no estimate
of accuracy was attempted owing to limited infor
mation.
The tabulated values of viscosity were calculated
from the data of Arndt and Ploetz [37] (673.2 to
873.2 °K, 5 points, vertical capillary viscometer).
The cubic equation expresses the data with a preci
sion 5 = 0.0120 (0.93%). The uncertainty of the
viscosity values is estimated to be about (1.5%).
Potassium Dichromate
[Refer: Table 169, p. 106, for numerical values]
Two investigations of the specific conductance
for molten K^C^Cb have been reported [8, 110].
The tabulated values were calculated from the
exponential equation for specific conductance
reported by Frame, Rhodes, and Ubbelohde [110].
No precision was given. The maximum departurebetween the values reported by Lorenz and Kalmus[8] and Ubbelohde [110] is 15.5 percent (780 °K).
The uncertainty of the specific conductance values
is estimated to be about 8.0 percent.
The exponential equation expresses the tabu
lated values of equivalent conductance with a
precision s = 0.0144 (0.056%).
Of the two density studies [25, 110], the data of
Jaeger [25] were selected to calculate the tabulated
values. The maximum departure between the den
sities reported by Jaeger and Ubbelohde et al. [110]
is less than 0.02 percent over the temperaturerange of 690 to 710 °K. The uncertainty of the
density values is judged to be about 0.1 percent.
Two investigations of the viscosity have beenreported [8, 110]. The tabulated values were cal
culated from the data of Lorenz and Kalmus [8]
(670.2 to 780.2 °K, 12 points, horizontal capillary
viscometer). Using the cubic equation for viscosity
the precision is 5 = 0.0084 (0.092%). The uncer
tainty of the viscosity values is estimated to beabout 1.5 percent.
The viscosities of the second study (Ubbelohde
et al. [110, 125c]; Ubbelohde viscometer) showincreasing departure from those of Lorenz andKalmus (e.g. —6% at 700 °K).
Sodium Metaphosphate
[Refer: Table 170, p. 107, for numerical values]
The tabulated values of viscosity for moltenNaP03 were calculated from the data of Arndt [200]
(916 to 1029 °K, 4 points, restricted falling ball
method). The exponential equaiion expresses the
data of Arndt with a precision 5 = 63.3 (8.62%). Noestimate of accuracy was attempted owing to the
limited information.
Uranyl Chloride
[Refer: Table 171, p. 107, for numerical values]
The tabulated values of specific conductancefor molten UCLCL were calculated from the linear
equation given by Ochs and Strassmann [64] (851
to 953 °K). No attempt to calculate the precision wasmade due to lack of experimental data.
Lithium Hydride
[Refer: Table 172, p. 107, for numerical values]
The tabulated values of specific conductance for
molten LiH were calculated from the data of Moers[165] (958.2 to 1027.2 °K, 5 points). Using the quadratic equation for specific conductance the precision
is 5 = 9.89 • 10~ 3 (12%). The recent work of Johnsonand Cairns [213] indicates a need for additional
studies since the specific conductivities are higher
36
than those of Moers [165]. An estimate of accuracy
was not attempted owing to the limited information
of this private communication [213].
Lithium Chlorate
[Refer: Table 173, p. 107, for numerical values]
The tabulated values of specific conductancewere calculated from the data of Campbell andWilliams [164, 174] (404.6 to 446.7 °K, 10 points).
Using the linear equation for specific conductancethe precision is 5=1.9910 3
(1.1%). Since noother conductance measurements are available
for comparison a critical estimate of the accuracyis not possible; however, judging the experimentaltechniques of Campbell and Williams, these results
can be considered reliable.
The exponential equation expresses the tabulatedvalues of equivalent conductance with a precision
s = 0.218 (3.2%).
The density data of Campbell [164, 175] wereused to calculate the tabulated values; no estimateof accuracy was attempted owing to the limited
information.
The tabulated values of viscosity were calculated
from the data of Campbell and Williams [175] (404.9
to 440.0 °K, 13 points, capillary viscometer). Thecubic equation expresses the data with a precision
5 = 0.446 (2.17%). No estimate of accuracy wasattempted owing to the limited information.
Lithium Perchlorate
[Refer: Table 174, p. 108, for numerical values]
The density data of Peterson, Ewing and Smith
[177] for molten LiClCR were used to calculate the
tabulated values; no estimate of accuracy wasattempted owing to the limited information.
r
37
fe;V M 1115vM BIB I I I \lm
.
'
List of Tables
Table
Page
FLUORIDES
LiF 1 Lithium fluoride 42NaF 2 Sodium fluoride 42KF 3 Potassium fluoride 43CsF 4 Cesium fluoride 43BeF2 5 Beryllium fluoride 44MgF2 6 Magnesium fluoride 44
CaF2 7 Calcium fluoride 44
SrF2 8 Strontium fluoride 45BaF2 9 Barium fluoride 45
LaFs 10 Lanthanum (III) fluoride 45
CeF3 11 Cerium (III) fluoride 45ThF4 12 Thorium (IV) fluoride 46
UF4 13 Uranium (IV) fluoride 46MnF2 14 Manganese (II) fluoride 46CuF2 15 Copper (II) fluoride 46AgF 16 Silver fluoride 47
ZnF2 17 Zinc fluoride 47PbF2 18 Lead (II) fluoride 47
CHLORIDES
LiCl 19 Lithium chloride 47NaCl 20 Sodium chloride 48KC1 21 Potassium chloride 48RbCl 22 Rubidium chloride 49CsCl 23 Cesium chloride 49
BeCl2 24 Beryllium (II) chloride 50MgCl2 25 Magnesium chloride 50CaCl2 26 Calcium chloride 50SrCl2 27 Strontium chloride 51
BaCl2 28 Barium chloride 51
ScCL 29 Scandium (III) chloride 51
YCI3 30 Yttrium (III) chloride 52LaCL 31 Lanthanum (III) chloride 52CeCL 32 Cerium (III) chloride 53PrCL 33 Praseodymium (III) chloride 53NdCl3 34 Neodymium (III) chloride 53GdCL 35 Gadolinium (III) chloride 54DyCL 36 Dysprosium (III) chloride 54H0CI3 37 Holmium (III) chloride 54ErCL 38 Erbium (III) chloride 54ThCL 39 Thorium (IV) chloride 55UCL 40 Uranium (IV) chloride 55MnCl2 41 Manganese (II) chloride 55TiCL 42 Titanium (IV) chloride 55CuCl 43 Copper (I) chloride 56AgCl 44 Silver chloride 56
ZnCl 2 45 Zinc chloride 57
CdCl2 46 Cadmium chloride 57
HgCl 47 Mercury (I) chloride 58
HgCl2 48 Mercury (II) chloride 58
AlCls 49 Aluminum (III) chloride 58GaCli 50 Gallium (III) chloride 59InCl 51 Indium chloride 59InCl2 52 Indium (II) chloride 60InCL 53 Indium (III) chloride 60T1C1 54 Thallium (I) chloride 61SnCl2 55 Tin (II) chloride 61SnCL 56 Tin (IV) chloride 62PbCl2 57 Lead (II) chloride 62BiCh 58 Bismuth (III) chloride 63TeCl2 59 Tellurium (II) chloride 63TeCh 60 Tellurium (IV) chloride 63
39
Table
BROMIDESPage
LiBr 61 Lithium bromide 64NaBr 62 Sodium bromide „ 64KBr 63 Potassium bromide 65RbBr 64 Rubidium bromide 65CsBr 65 Cesium bromide 66MgBr2 66 Magnesium bromide 66CaBr 67 Calcium bromide 67SrBr2 68 Strontium bromide 67BaBr2 69 Barium bromide 68LaBr3 70 Lanthanum (III) bromide 68PrBr3 71 Praseodymium (III) bromide 68NdBr3 72 Neodymium (III) bromide 69GdBr3 73 Gadolinium (III) bromide 69CuBr 74 Copper (I) bromide 69AgBr 75 Silver bromide 70ZnBr2 76 Zinc Bromide 70CdBr2 77 Cadmium bromide 71
HgBr2 78 Mercury (II) bromide 71
AlBr3 79 Aluminum bromide 72InBr3 80 Indium (III) bromide 72TIBr 81 Thallium (I) bromide 73PbBr2 82 Lead (II) bromide 74BiBr3 83 Bismuth (III) bromide 75
IODIDES
Lil 84 Lithium iodide 75Nal 85 Sodium iodide 76KI 86 Potassium iodide 76Rbl 87 Rubidium iodide 77Csl 88 Cesium iodide 77Mgl> 89 Magnesium iodide 78Cal2 90 Calcium iodide 78Srl2 91 Strontium iodide 79Bal2 92 Barium iodide 79AIL 93 Aluminum (III) iodide 79Lal3 94 Lanthanum (III) iodide 80Cel3 95 Cerium (III) iodide 80PrI.j 96 Praseodymium (III) iodide 80Ndl3 97 Neodymium (III) iodide 80Agl 98 Silver iodide 81Znl2 99 Zinc iodide 81Cdl2 100 Cadmium iodide 82Hgl2 101 Mercury (II) iodide 82Gal2 102 Gallium (II) iodide 83Inl3 103 Indium (III) iodide 83Til 104 Thallium (I) iodide 84Pbl2 105 Lead (II) iodide 84Bil3 106 Bismuth (III) iodide 85
CARBONATES
Li2C03 107 Lithium carbonate 85Na2C03 108 Sodium carbonate 85K2C03 109 Potassium carbonate 86
NITRITES
LiN02 110 Lithium nitrite 86NaN02 111 Sodium nitrite 86KN02 112 Potassium nitrite 87RbN02 113 Rubidium nitrite 87CsN02 114 Cesium nitrite 87Ba(N02 )2 115 Barium nitrite 87
NITRATES
LiN03 116 Lithium nitrate 88NaN03 117 Sodium nitrate 88KN03 118 Potassium nitrate 89RbN03 119 Rubidium nitrate 89CsN03 120 Cesium nitrate 90AgN03 121 Silver nitrate 90T1N03 122 Thallium nitrate 91
40
Table Page
OXIDES
V205 123 Vanadium pentoxide 91
Cr03 124 Chromium trioxide 91
MoO:j 125 Molybdenum trioxide 91
FeO 126 Wustite (Feo.ssO) 92
B2O3 127 Boron oxide 92
SiO '2 128 Silicon dioxide 93
Ge02 129 Germanium dioxide 93
PbO 130 Lead oxide 94
AS2O3 131 Arsenic trioxide 94
Sb203 132 Antimony sesquioxide 94
Bi203 133 Bismuth sesquioxide 94
Te02 134 Tellurium dioxide 95
SULFIDES
FeS 135 Iron (II) sulfide 95
CoS 136 Cobalt (II) sulfide 95
NiS 137 Nickel (II) sulfide 95
CuS 138 Copper (I) sulfide 96
Ag2S 139 Silver sulfide 96
GeS 140 Germanium (II) sulfide 96
SnS 141 Tin (II) sulfide 97
PbS 142 Lead sulfide 97
Sb2S3 143 Antimony (III) sulfide 98
Bi2S3 144 Bismuth (III) sulfide 98
SULFATES
Li2S04 145 Lithium sulfate 99
Na2S04 146 Sodium sulfate 99
K2SO4 147 Potassium sulfate 99
Rb2S04 148 Rubidium sulfate 99
Cs2S04 149a Cesium sulfate 190
Ag2S04 149b Silver sulfate 109
rQUATERNARY AMMONIUM SALTS
Pr4NBF4 150 Tetrapropylammonium tetrafluoroborate 100
Pr4NPF6 151 Tetrapropylammonium hexafluorophosphate 100
Pr4NBPh4 152 Tetrapropylammonium tetraphenylborate 101
Bu4NBr 153 Tetrabutylammonium bromide 101
Bu4NI 154 Tetrabutylammonium iodide 101
Bu4NBF4 155 Tetrabutylammonium tetrafluoroborate 101
Bu4NPF6 156 Tetrabutylammonium hexafluorophosphate 102
Bu4NBPh4 157 Tetrabutylammonium tetraphenylborate 102
Hex4NBF4 158 Tetrahexylammonium tetrafluoroborate 102(nAmyl) 4NSCN 159 Tetranamylammonium thiocyanate 102
MISCELLANEOUS
Li2Mo04 160 Lithium molybdate 103Na2Mo04 161 Sodium molybdate 103K2Mo04 162 Potassium molybdate 104Na2W04 163 Sodium tungstate 104K2W04 164 Potassium tungstate 104NaSCN 165 Sodium thiocyanate 105KSCN 166 Potassium thiocyanate 105NaOH 167 Sodium hydroxide 105KOH 168 Potassium hydroxide 106K2Cr207 169 Potassium dichromate 106NaP03 170 Sodium metaphosphate 107UO2CI2 171 Uranyl chloride 107LiH 172 Lithium hydride 107LiC103 173 Lithium chlorate 107LiC104 174 Lithium perchlorate 108
SUMMARY TABLES
175 Specific conductance — best equations 109
176 Density— best equations 114
177 Equivalent conductance 117
178 Viscosity— best equations 120
179 Specific conductance — exponential equations 122
180 Specific conductance — power series equations 126
181 Viscosity — exponential equations 131
182 Viscosity power series equations 133
41
6. Numerical Values of Electrical Conductance, Density, and Viscosity
Table 1. Lithium fluoride Table 2. Sodium fluoride
Eq wt 25.94 mp 845 °C (1118 °K)
k =  15.0389 + 3.53546 • 10 2T 1.28145 • lO’T2
p = 2.3581 0.4902 • 10" 3r
A = 320.71 exp ( 2U3.3/RT)
T A K P
1140 124.0 8.602 (1.7993)
1150 125.2 8.662 1.7944
1160 126.4 8.719 1.7895
1170 127.5 8.774 1.7846
1180 128.7 8.826 1.7797
1190 129.7 8.876 1.7748
1200 130.8 8.923 1.7699
1210 131.8 8.968 1.7650
1220 132.8 9.010 1.7601
1230 133.7 9.050 1.7552
1240 134.7 9.087 1.7502
1250 135.6 9.121 1.7454
1260 136.4 9.153 1.7404
1270 137.2 9.182 1.7355
1280 138.0 9.209 1.7306
1290 138.7 9.233 1.7257
1300 139.5 9.254 1.7208
1310 140.2 9.273 1.7159
Density: [25, 81, 83].
Conductance: [42, 83, 86. 88].
Melting point: [130].
Eq wt 41.99 mp 980 °C (1253 °K)
k= 1.4605 + 2.7374 lOT
p = 2.655 0.54 • 10 3TA = 344. 7 exp (2964/RT)
T A K P
1270 106.7 4.937 1.9438
1280 107.6 4.964 1.9382
1290 108.5 4.992 1.9326
1300 109.4 5.019 1.9270
1310 110.3 5.047 1.9214
1320 111.2 5.074 1.9158
1330 112.2 5.101 1.9102
1340 113.1 5.129 1.9046
1350 114.0 5.156 1.8990
1360 115.0 5.183 1.8934
1370 115.9 5.211 1.8878
1380 116.9 5.238 1.8822
1390 117.8 5.265 1.8766
1400 118.8 5.293 1.8710
1410 119.8 5.320 1.8654
1420 120.8 5.348 1.8598
Density:[25 , 31].
Conductance: [31, 46. 67, 86, 88].
Melting point: [131].
42
Table 3. Potassium fluoride Table 4. Cesium fluoride
Eq wt 58.10 mp 856 °C (1129 °K)
k = 9.2728 • 10~ 2 + 3.0628 • 10L3T
p = 2.6464 0.6515 • 10~ 3rA = 480.27 exp (— 3354.9/Z27’)
T A K P
1130 108.1 3.554 1.9102
1140 109.4 3.584 1.9037
1150 110.7 3.615 1.8972
1160 112.0 3.646 1.8907
1170 113.4 3.676 1.8841
1180 114.7 3.707 1.8776
1190 116.1 3.737 1.8711
1200 117.4 3.768 1.8646
1210 118.8 3.799 1.8581
1220 120.2 3.829 1.8516
1230 121.5 3.860 1.8451
1240 122.9 3.891 1.8385
1250 124.4 3.921 1.8320
1260 125.8 3.952 1.8255
1270 127.2 3.982 1.8190
1280 128.6 4.013 1.8125
1290 130.1 4.044 1.8060
Eq wt 151.90 mp 681 °C (955 °K)
k = 1.47691 + 3.997 • 10“ 3r
p = 4.8985 1.2806 • 10^ 3TA = 817.76 exp (4068.2/RT)
T A K P
1010 107.9 2.560 3.605
1020 110.0 2.600 3.592
1030 112.0 2.640 3.579
1040 114.1 2.680 3.567
1050 116.3 2.720 3.554
1060 118.4 2.760 3.541
1070 120.6 2.800 3.528
1080 122.7 2.840 3.515
1090 124.9 2.880 3.503
1100 127.1 2.920 3.490
1110 129.3 2.960 3.477
1120 131.5 3.000 3.464
1130 133.8 3.040 3.451
Density: [25, 83 J.
Conductance: [83, 182 ].
Melting point: [130].
Density: [26, 81, 83],
Conductance: [26, 31, 42, 73, 83, 86, 88, 198],
Melting point: [130].
297268 068 •443
Table 6. Magnesium fluoride
Eq wt 31.16 mp 1263 °C (1536 °K)
p = 3.235 5.24 • 10“4r
Table 5. Beryllium fluoride
Eq wt 23.51 mp 540 °C (813 °K)
k was obtained from a smooth curve through the experi
mental points of Mackenzie.
r]= 1.756 • 10 7 exp (58, 566/RT)
T k • 10 5T)
' 10 3
850 190,000.
870 85,600.
890 40,000.
910 19,400.
930 9,660.
950 4,960.
970 0.61 2,620.
990 1.36 1,420.
1010 2.63 788.
1030 4.64 448.
1050 7.87 260.
1070 13.77 154.
1090 22.3 92.9
1110 33.9 57.1
1130 51.9 35.7
1150 75.7 22.7
1170 106.2 14.7
1190 144.7 9.61
1210 194.5 6.39
1230 4.30
1250 2.93
Conductance: [143].
Viscosity: [143, 225 ]
.
Melting Point: [143],
T P
1650 2.370
1700 2.344
1750 2.318
1800 2.292
1850 2.266
1900 2.239
1950 2.213
2000 2.187
2050 2.161
2100 2.135
Density: [95]
.
Melting point: [130].
Table 7. Calcium fluoride
Eq wt 39.04 mp 1418 °C (1691 °K)
p = 3. 1793. 91 • 10~4T
T P
1650 2.534
1700 2.514
1750 2.495
1800 2.475
1850 2.456
1900 2.436
1950 2.417
2000 2.397
2050 2.377
2100 2.358
2150 2.338
2200 2.319
2250 2.299
2300 2.280
44
Density: [95, 197].
Melting point: [130],
TABLE 8. Strontium fluoride TABLE 10. Lanthanum (111) fluoride
Eq wt 62.81 mp 1400 °C (1673 °K) Eq wt 65.30 mp < 1477 °C ( < 1750 °K)
p= 4.784 7.51 • 104T p = 5.793 6.82 • 104T
T P
1750 3.470
1800 3.432
1850 3.395
1900 3.357
1950 3.320
2000 3.282
2050 3.244
2100 3.207
2150 3.169
2200 3.132
Density: [95].
Melting point: [130].
T P
1750 4.600
1800 4.565
1850 4.531
1900 4.497
1950 4.463
2000 4.429
2050 4.395
2100 4.361
2150 4.327
2200 4.293
2250 4.259
2300 4.224
2350 4.190
2400 4.156
2450 4.122
Density: [95] .
Melting point: [95].
Table 11. Cerium (III) fluoride
Table 9. Barium fluoride Eq wt 65.70 mp 1460 °C (1733 °K)
Eq wt 87.68 mp 1320 °C (1593 °K)
p= 5.775 9.99 • 10“4r
T P
1600 4.177
1650 4.127
1700 4.077
1750 4.027
1800 3.977
1850 3.927
1900 3.877
1950 3.827
2000 3.777
p = 6.253 9.36 • 10"4r
T P
1700 4.662
1750 4.615
1800 4.568
1850 4.521
1900 4.475
1950 4.428
2000 4.381
2050 4.334
2100 4.287
2150 4.241
2200 4.194
Density: [95]
.
Melting point: [130],
45
Density: [95].
Melting point: [130],
Table 12. Thorium (IV) fluoride Table 13. Uranium (IV) fluoride
Eq wt 77.03 mp 1110 °C (1383 °K)
p = 7. 108 7.590 • 104T
T P
1390 6.0530
1400 6.0454
1420 6.0302
1440 6.0150
1460 5.9999
1480 5.9847
1500 5.9695
1520 5.9543
1540 5.9391
1560 5.9240
1580 5.9088
1600 5.8936
1620 5.8784
1640 5.8632
Density: [167].
Melting point: [167].
Eq wt 78.52 mp 1036 °C (1309 °K)
p = 7.784 9.920 • 10 4T
T P
1310 6.4845
1320 6.4746
1340 6.4547
1360 6.4349
1380 6.4150
1400 6.3952
1420 6.3754
1440 6.3555
1460 6.3357
1480 6.3158
1500 6.2960
1520 6.2762
1540 6.2563
1560 6.2365
1580 6.2166
1600 6.1968
1620 6.1770
Density: [167].
Melting point: [167].
Table 14. Manganese (II) fluoride Table 15. Copper (II) fluoride
Eq wt 46.46 mp 856 °C (1129 °K) Eq wt 50.77 mp 856 °C (1129 °K)
k = 4.0 • \0~ 3T
Conductance: [86].
Melting point: [130]
k = 0.93+1.0 lO 3^
Conductance: [86]
.
Melting point: [130]
46
TABLE 16. Silver fluoride
Eq wt 126.88 mp 435 °C (708 °K)
k =— 5.2 + 12.0 • io 3r
Conductance: [86]
.
Melting point: [130].
Table 17. Zinc fluoride
Eq wt 51.69 mp 872 °C (1145 °K)
k =3 . 75 + 6.0 10~ 3T
Conductance: [86]
.
Melting point: [130],
Table 18. Lead (II) fluoride
Eq wt 122.60 mp 822 °C (1095 °K)
k = 0.7 + 4.0 • 103T
Table 19. Lithium chloride
Eq wt 42.4 mp 610 °C (883 °K)
k = 2.0647+ 12.1271 • 103T3.7641 • 10~ 6T2
p= 1.8842 0.4328 • \0~3TA = 508.2 exp (2015//?7]
7] = 3.306 • 10 2 exp (7007/RT)
Density: [3, 25, 55, 62, 66, 79, 81].’
Conductance: [33, 42, 44, 45, 55, 62, 66, 79, 85].
Viscosity: [12, 45, 47, 1211 .
Melting point: [130].
T K
1150 5.3
1200 5.5
1250 5.7
Conductance: [86]
.
Melting point: [130].
47
Table 20. Sodium chloride Table 21. Potassium chloride
Eq wt 58.45 mp 800 °C (1073 °K)
k = 2.4975 + 8.0431 • 103T 2.2227 • 10 6T 2
p = 2. 1393 0.5430 • 10“3rA = 544.6 exp ( 2990//?T)
17 = 81.90070.185538 T+ 1.42786 • 10~ 3r 2
3.70073 • 10 8T 3
T A K P V
10801090
135.4
137.1
3.596
3.629
1.553
1.547 1.38
1100 138.8 3.660 1.542 1.32
1110 140.4 3.692 1.537 1.27
1120 142.1 3.723] 1.531 1.22
1130 143.8 3.753 1.526 1.17
1140 145.4 3.783 1.520 1.12
1150 147.1 3.813 1.515 1.08
1160 148.8 3.842 1.509 1.04
1170 150.4 3.870 1.504 1.01
1180 152.1 3.898! 1.499 0.98
1190 153.7 3.926 1.493 .95
1200 155.3 3.954 1.488 .92
1210 157.0 3.980 1.483 .89
1220 158.6 4.007 1.477 .87
1230 160.2 4.033 1.471 .84
1240 161.8 4.058 1.466 .82
1250 163.4 4.083 1.461
1260 165.0 4.108 1.455
1270 166.6 4.132 1.450
1280 168.2 4.156 1.444
1290 169.8 4.179 1.439
Density: [3. 11. 25, 55, 62, 66, 79, 80, 81, 96, 126],
Conductance: [2, 4, 10, 27, 33, 42, 49, 52, 55, 62, 63,
71, 79, 82, 85, 199],
Viscosity: [12, 38, 57, 1211 .
Melting point: [130].
Eq wt 74.55 mp 770 °C (1043 °K)
k =  3.99005 + 9.0222 • 10 3T3.000 • KCT 2
p = 2. 1359 0.5831 • 10 3TA = 548.0 exp (3415.2/RT)
rj = 55.5632 0.127847T+ 9.99580 • 10 5T 2
2.62035 • 10 8T 3
T A K P 17
1060 108.2 2.203 1.5178 1.14s
1070 109.9 2.229 1.5120 1.108
1080 111.6 2.255 1.5062 ©r—
H
1090 113.3 2.280 1.5003 1.036
1100 114.9 2.304 1.4945 1.004
1110 116.6 2.328 1.4887 0.975
1120 118.2 2.352 1.4828 •94g
1130 119.8 2.374 1.4770 •92.1
1140 121.4 2.396 1.4712 .90,
1150 123.0 2.418 1.4653 0000
1160 124.6 2.439 1.4595 .863
1170 126.1 2.459 1.4537 .847
1180 127.6 2.479 1.4478 .832
1190 129.1 2.498 1.4420 •81s
1200 130.6 2.517 1.4362 .80
Density: [3, 11, 26, 62, 66, 70, 79. 80, 81, 126, 178],
Conductance: [2, 4, 10, 26, 27, 42, 44. 49. 50, 55, 62,
63, 66, 79, 85. 123, 124, 125, 129],
Viscosity: [12, 102 , 111].
Melting point: [130].
48
Table 22. Rubidium chloride Table 23. Cesium chloride
Eq wt 120.94 mp 715 °C (988 °K) Eq wt 168.37 mp 645 °C (918 °K)
* = 3.6290 + 7.3405 • 10 3T2.1918 • 10 6T 2
p = 3. 1210 0.8832 lO^TA = 754.1 exp (4401 /RT)
r] = 40.8082  9.61807 • 10 2T+ 7.83918 • 10~ 5T 2
2.16855 • 10 8T 3
T A K P P T A K P V
990 80.2 1.490 2.2466 940 71.0 1.167 2.7681 1.28
1000 82.1 1.520 2.2378 950 73.2.5 1.200 2.7575 1.23
1010 84.0 1.549 2.2290 1.29 960 75.4.5 1.231 2.7468 1.19
1020 86.0 1.578 2.2201 1.25 970 77.7 1.263 2.7362 1.15
1030 87.9 1.606 2.2113 1.21 980 79.9.5 1.294 2.7255 1.12
1040 89.8 1.634 2.2025 1.18 990 82.1.5 1.325 2.7149 1.08
1050 91.6 1.662 2.1936 1.14 1000 84.4 1.355 2.7042 1.05
1060 93.5 1.689 2.1848 1.11 1010 86.6 1.385 2.6936 1.02
1070 95.4 1.716 2.1760 1.08 1020 88.8 1.415 2.6829 0.99
1080 97.2 1.742 2.1671 1.05 1030 91.0.5 1.445 2.6723 .97
1090 99.1 1.768 2.1583 1.03 1040 93.2.5 1.474 2.6616 .94
1100 100.9 1.793 2.1495 1.00 1050 95.5 1.503 2.6510 .82
1110 102.7 1.818 2.1406 0.98 1060 97.7 1.532 2.6403 .90
1120 104.6 1.843 2.1318 .95 1070 99.9 1.560 2.6297 .88
1130 106.4 1.867 2.1230 .93 1080 100.2 1.588 2.6190 .86
1140 108.2 1.891 2.1142 .91 1090 104.3 1.616 2.6084 .84
1150 119.9 1.914 2.1053 1100 106.5 1.644 2.5977 .82
1160 111.7 1.937 2.0965 1110 108.7 1.671 2.5871 .80
1170 113.5 1.959 2.0877 1120 110 9 1 698 2 57641180 115.2 1.981 2.0788 1130 113 2 1 724 2 56581190 117.0 2.002 2.0700 1140 115 3 1 751 2 55511200 118.7 2.023 2.0612 1150 117 6 1 777 2 54451210 1160 119.8 1.802 2.53381220 1170 122.0 1.828 2.5232
k =  3.2034 + 6.0802 • lO3^ 1.5216 • 10"6Pp = 3. 7692  1.065 • 103TA = 1102 exp (—5110IRT)
r) = 30.0396  7.09298 • 10 2T+ 5.80038 • 10 5T 2
 1.60636 • 10~ ST 3
Density: [25, 35, 36, 82]
.
Conductance: [33, 82, 129].
Viscosity: [109, 121].
Melting point: [131],
Density: [25, 59, 80, 81, 821 .
Conductance: [33, 82, 129, 199]
Viscosity: [109, 1211 .
Melting point: [130].
49
Table 24. Beryllium {II) chloride Table 26. Calcium chloride
Eq wt 39.96 mp 440 °C (713 °K)
ic =  0.075392 + 1.0576 • 10 4T
p = 2.2761. 10 • 10 3TA= 5.3567 • 10 13 exp (50479/RT)
T A • 10 2 k 10 3P
720 2.03 0.755 1.484
730 4.92 1.81 1.473
740 7.84 2.87 1.462
750 10.8 3.93 1.451
760 13.8 4.99 1.440
Density: [361 .
Conductance: [32, 1861 .
Melting Point: [131].
Table 25. Magnesium chloride
Eq wt 47.62 mp 714 °c (987 °K)
k— 0.6049+ 1.352 • 10 3 T+ 0.2911 • 10~ 6 T
p= 1.9760.302 • 10 3 TA= 263.7 exp (4363/RT)
T A K P
1000 (29.51) 1.038 (1.675)
1020 30.75 1.077 1.668
1040 31.98 1.116 1.662
1060 33.21 1.155 1.656
1080 34.49 1.195 1.650
1100 35.77 1.235 1.644
1120 37.04 1.274 1.638
1140 38.37 1.315 1.632
1160 39.68 1.355 1.626
1180 (41.04) 1.396 (1.620)
1200 (42.40) 1.437 (1.614)
1220 (43.77) 1.478 (1.608)
1240 (45.15) 1.519 (1.602)
Eq wt 55.49 mp 782 °C (1055 °K)
k= 19.628 exp (4749/RT)
p= 2.5261 0.4225 • 10~ 3rA =675.3 exp (5285/RT)
r) = 619.541 1.54489 T+ 1.29259 • 10 3 r2
3.61856 • 10 7 P
T A K P
1060 54.9« 2.059 2.0783 3.34
1070 56.26 2.103 2.0740 3.11
1080 57.5s 2.147 2.0698 2.90
1090 58.8s 2.191 2.0656 2.72
1100 60.
1
6 2.235 2.0614 2.57
1110 61.4s 2.279 2.0571 2.43
1120 62. 80 2.323 2.0529 2.31
1130 64.
1
3 2.368 2.0487 2.20
1140 65A 2.412 2.0445 2.11
1150 66.8, 2.456 2.0402 2.03
1160 COH000 2.501 2.0360 1.96
1170 69.5, 2.545 2.0318 1.89
1180 70.8t 2.590 2.0276 1.83
1190 72.2., 2.634 2.0233 1.77
1200 73.6, 2.679 2.0191 1.72
1210 74.99 2.723 2.0149 1.66
1220 76.3s 2.767 2.0107 1.59
1230
1240
77.76 2.812 2.0064 1.52
1.44
Density: [11, 17, 63, 831 .
Conductance: [2, 4, 11, 35, 42, 50, 71, 83, 85. 94].
Viscosity: [47, 1091 .
Melting Point: [130].
Density: [36, 63, 91, 1131 .
Conductance: [35, 63, 941 .
Melting Point: [130],
50
Table 27. Strontium chloride Table 28. Barium chloride
Eq wt 79.27 nip 875 °C (1148 °K)
k— 17.792 exp (4987IRT)
p= 3.3896 0.5781 • 10~ 3 T
A = 689.6 exp (— 5646//?71
)
rj = 4.401 • 10 4 exp (20655IRT)
T A K P V
1160 3.43
1170 60.85 2.082.5 2.7132 3.18
1180 62.09 2.120s 2.7074 2.95
1190 63.35 2.1590 2.7017 2.74
1200 64.61 2.1973 2.6959 2.54
1210 65.88 2.235« 2.6901 2.37
1220 67.15 2.2740 2.6843 2.21
1230 68.43 2.3123 2.6785 2.06
1240 69.72 2.3507 2.6728 1.92
1250 71.01 2.389, 8.6670 1.80
1260 72.31 2.427., 2.6612
1270 73.61 2.465s 2.6554
1280 74.92 2.504, 2.6496
1290 76.23 2.542s 2.6439
1300 77.55 2.5809 2.6381
1310 78.88 2.6192 2.6323
Density: [11, 81, 83, 91].
Conductance: [4, 83, 941 .
Viscosity:[1091 .
Melting Point: [130].
Eq wt 104.14 mp 962 °C (1235 °K)
k= 17.479 exp (5274IRT)
p = 4.0152 0.6813 10~ 3 TA= 772.5 exp (6004AR7
1
)
t? = 1.643 • 10~ 3 exp (20029/RT)
T A K P t?
1240 67.5s 2.058 3.1704
1250 68.
9
0 2.093 3.1636
1260 70.2., 2.129 3.1568
1270 71.5s 2.164 3.1499 4.60
1280 72.8s 2.200 3.1431 4.32
1290 74.23 2.236 3.1363 4.07
1300 75.5s 2.271 3.1295 3.83
1310 76.
9
3 2.307 3.1227 3.61
1320 78.29 2.343 3.1159
1330 79.66 2.378 3.1091
1340 81.0.3 2.414 3.1023
1350 82.4, 2.450 3.0954
1360 83. 80 2.485 3.0886
Density: [11, 63, 70, 81, 831 .
Conductance: [4, 63, 83, 85, 94].
Viscosity:[109 . 210],
Melting Point: [130].
TABLE 29. Scandium (III) chloride
Eq wt 50.49 mp 939 °C (1212 °K)
k =  2.890 + 2.796 • 10 3 7’
T°K K P
1213 1.67
1223 0.53
1273 .67 1.63
Density: [36]
.
Conductance: [30]
.
Melting Point: [131].
51
Table 30. Yttrium (III) chloride Table 31. Lanthanum (III) chloride
Eq wt 65.09 mp 700 °C (973 °K)
k = 3. 7071 + 5. 9576 • \0~ 3T 1.8199 • 10~ 6 T^
p = 3.0070.50 • io 3rA = 959.2 exp ( 8827/RT)
T A K P
980 9.9 0.384 2.517
990 10.5s .407 2.512
1000 11.2 .431 2.507
1010 11.8 .454 2.502
1020 12.4 .476 2.497
1030 13.0 .498 2.492
1040 13.6 .520 2.487
1050 14.2 .542 2.482
1060 14.8 .563 2.477
1070 15.4 .584 2.472
1080 15.9s .604 2.467
1090 16.5 .624 2.462
1100 17.0s .644 2.457
1110 17.6 .664 2.452
1120 18.1 5 .683 2.447
1130 (18.7) .701 (2.442)
1140 (19.2) .719 (2.437)
1150 (19.7s) .737 (2.432)
1160 (20.2s) .755 (2.427)
Eq wt 81.76 mp 870 °C (1143 °K)
k = 13.538 + 22.487 • 10 3T8.167 • 10 6r2
p = 4.0895 0.7774 • 10 3TA =469.4 exp (5678/RT)
tj = 2.061 • 10 2 exp (13049/RT)
T A K P
1140 37.86 1.483 3.2033
1150 38.92 1.521 3.1955
1160 39.95 1.557 3.1877
1170 40.93 1.592 3.1799
1180 41.88 1.625 3.1722
1190 42.79 1.656 3.1644 5.14
1200 43.67 1.686 3.1566 4.91
1210 44.50 1.714 3.1488 4.69
1220 45.30 1.740 3.1411 4.49
1230 46.06 1.765 3.1333 4.29
1240 46.78 1.788 3.1255 4.11
1250 47.46 1.810 3.1178 3.94
1260 48.10 1.830 3.1100 3.78
Density: [36, 831 .
Conductance: [35, 83, 118].
Viscosity:[1361 .
Melting Point: [130].
Density: [36]
.
Conductance: [35] .
Melting Point: [130],
52
Table 32. Cerium {III) chloride
Eq wt 82.17 mp 822 °C (1095 °K)
k= 10.03815+1.707017 • 10~ 2 T6.301668 • 10 6 T1
p= 4.248 0.920 lO^ 3 TA = 460.7 exp (6078.0jRT)
T A K P
1100 28.3 1.114 3.236
1110 29.2 1.145 3.227
1120 30.0 1.176 3.218
1130 30.8 1.204 3.208
1140 31.6 1.232 3.199
1150 32.4 1.259 3.190
1160 33.2 1.284 3.181
1170 33.9 1.308 3.172
1180 34.6 1.330 3.162
1190 35.2 1.352 3.153
1200 35.8 1.372 3.144
1210v
36.4 1.390 3.135
Density: [99].
Conductance: [99, 1191 .
Melting Point: [130].
Table 33. Praseodymium {III) chloride
Eq wt 82.43 mp 823 °C (1096 °K)
k= 36.17 exp (8258/RT)
T K
1100 0.827
1110 •856
1120 .885
1130 ,914
1140 .944
1150 •975
1160 I.OO5
1170 1.037
1180 1.06s
1190 1.10!
1200 1.13a
1210 1.166
1220 1.19a
1230 1.23a
1240 1.267
Conductance: [32 , 120],
Melting Point: [130],
Table 34. Neodymium {III) chloride
Eq wt 83.55 mp 760 °C (1033 °K)
>< =— 2.018 + 2.527 • 10~ 3r
T K
1050 0.635
1060 .661
1070 .686
1080 .712
1090 .736
1100 .762
1110 .787
1120 .812
1130 .838
1140 .863
1150 .888
1160 .913
1170 .939
Conductance: [32 , 118].
Melting Point: [130],
53
Table 35. Gadolinium, (III) chloride Table 37. Holmium (III) chloride
Eq wt 87.7 mp 602 °C (875 °K)
k = 22.247 exp ( 1300.6/RT)
T K
900 0.375
910 .392
920 .410
930 .428
940 .446
950 .465
960 .484
970 .504
980 .524
Conductance: [171].
Melting Point: [170].
Eq wt 90.45 mp 720 °C (993 °K)
k =~ 1.4081 + 1.79896 • 10“ 3 T
T K
1020 0.432
1030 .450
1040 .468
1050 .486
1060 .504
1070 .522
1080 .540
1090 .558
1100 .576
Conductance: [ 171] .
Melting Point: [ 1701 .
Table 36. Dysprosium (III) chloride
Eq wt 89.61 mp 647 °C (910 °K)
k = 1.37966+ 1.8417 • lO" 3 T
T K
950 0.370
960 .388
970 .407
980 .425
990 .444
1000 .462
1010 .480
Conductance: [ 1711 .
Melting Point: [ 1701 .
Table 38. Erbium (III) chloride
Eq wt 91.22 mp 776 °C (1046 °K)
k =  1.31353+ 1.6584 • 10“ 3 T
T K
1070 0.461
1080 .478
1090 .494
1100 .511
1110 .527
1120 .544
Conductance: [ 171] .
Melting Point: [ 1701 .
54
Table 39. Thorium (IV) chloride Table 41. Manganese (II) chloride
Eq wt 93.49 mp 770 °C (1043 °K)
k=  13.1887 + 22.5705 • 10 3T9.0973 • 10 6r2
p = 3.3, (1090 °K— 1190 °K)
A = 395.0 exp (6764/RT)
T A K P
1090 17.0 0.60 3.3,
1100 17.8 .63 3.3,
1110 18.5 .66 3.3,
1120 19.1 .69 3.32
1130 19.7 .70 3.3,
1140 20.2 .72 3.32
1150 20.7 .74 3.3,
1160 21.2 .75 3.3,
1170 21.6 .77 3.3,
1180 21.9 .78 3.3,
1190 22.2 .79 3.32
Density: [36]
.
Conductance: [32]
.
Melting Point: [130].
Eq wt 62.92 mp 650 °C (923 °K)
k= 1.572640 1.669355 • 10 3T+ 1.698935 • 10 6r2
p = 2. 75701 4.3766 • 10 4TA = 169.53 exp (2694.3/RT)
T A K P
930 39.88 1.490 2.350
940 40.36 1.505 2.346
950 40.85 1.520 2.341
960 41.35 1.536 2.337
970 41.86 1.552 2.332
980 42.39 1.569 2.328
990 42.92 1.585 2.324
1000 43.47 1.602 2.319
1010 44.02 1.620 2.315
1020 44.59 1.638 2.311
1030 45.17 1.656 2.306
1040 45.76 1.674 2.302
1050 46.37 1.693 2.297
1060 46.98 1.712 2.293
1070 47.60 1.732 2.289
1080 48.24 1.752 2.284
1090 48.89 1.772 2.280
1100 49.55 1.792 2.276
1110 50.2 1.813 2.271
1120 50.9 1.834 2.267
1130 51.6 1.856 2.262
Conductance: [85, 192 ]
.
Density: [ 192 ]
.
Melting Point: [130].
Table 40. Uranium (IV) chloride
Eq wt 94.98 mp < 570 °C (< 843 °K)
* = 2.023 + 2.803 • lO^T
T K
850 0.360
860 .388
870 .416
880 .444
890 .472
Table 42. Titanium (IV) chloride
Eq wt 47.43 mp  23 °C (250 °K)
17 = 4.952 • 10~ 2 exp (1643/RT)
T V
300 0.779
310 .713
320 .656
330 .607
Conductance: [32].
Melting Point: [32].
55
Viscosity:[204 ]
.
Melting Point: [130].
Table 43. Copper (/) chloride Table 44. Silver chloride
Eq wt 99.00 mp 422 °C (695 °K)
K=  1.290779 + 1.2137306 • 10“ 2r  9.126581 • 10 6F+ 2.196380 • 10 9F
p = 4.226 — 0.76 • 10 3r
A= 153.6 exp (—650A/RT)
p = 50.4565  0.140175 T + 1.37677 • 10 4F 4.66667 • 10

8F
T A K P V
740
760
96.83
98.40
3.583
3.626
3.664
3.648
780 99.89 3.666 3.633
800 101.3 3.703 3.618 2.54
810 102.0 3.720 3.610 2.44
820 102.7 3.736 3.603 2.36
830 103.3 3.752 3.595 2.27
840 103.9 3.767 3.588 2.19
850 104.6 3.781 3.580 2.12
860 105.1 3.794 3.572 2.05
870 105.7 3.807 3.565 1.98
880 (106.3) 3.819 (3.557) 1.92
890 (106.8) 3.831 (3.550) 1.86
900 (107.4) 3.841 (3.542) 1.80
910 (107.9) 3.852 (3.534) 1.74
920 (108.4) 3.861 (3.527) 1.69
930 (108.9) 3.870 (3.519) 1.63
940 (109.3) 3.878 (3.512) 1.58
950 (109.8) 3.886 (3.504) 1.53
960 (110.2) 3.893 (3.496) 1.48
970 (110.7) 3.900 (3.489) 1.44
1000 (111.9) 3.916 (3.466)
1050 (113.6) 3.934 (3.428)
1100 (115.1) 3.940 (3.390)
1150 (116.3) 3.938 (3.352)
1200 (117.3) 3.927 (3.314)
1250 (118.2) 3.910 (3.276)
1300 (118.9) 3.889 (3.238)
1350 (119.6) 3.865 (3.200)
1400 (120.2) 3.840 (3.162)
1430 (120.6) 3.825 (3.139)
Density: [36 . 212].
Conductance: [33, 35, 85, 189 . 212].
Viscosity:[471 .
Melting Point: [131].
Eq wt 143.34 mp 455 °C (728 °K)
k= 1.578+ 1.0697 • 10 2r4.51 • 10 6Fp= 5.5058.7 • 10 4TA = 268.22 exp ( 1252.3/RT)
Tj = 6.91305 — 4.47411 • 10~ 3r 6.49368 • 106F+ 5.41584 • 10 9F
T A K P V
730 2.29
740 114.1 3.868 4.861 2.24
750 115.4 3.908 4.852 2.19
760 116.8 3.947 4.844 2.14
770 118.1 3.985 4.835 2.09
780 119.4 4.022 4.826 2.04
790 120.7 4.058 4.818 2.00
800 122.0 4.093 4.809 1.95
810 123.3 4.128 4.800 1.91
820 125.5 4.161 4.792 1.86
830 125.7 4.194 4.783 1.82
840 126.9 4.225 4.774 1.78
850 128.0 4.256 4.765 1.74
860 129.1 4.286 4.757 1.71
870 130.3
,
4.315 4.748 1.67
880 131.3 4.343 4.739 1.64
890 132.4 4.370 4.731 1.61
900 133.5 4.396 4.722 1.57
910 134.5 4.422 4.713 1.55
920 135.5 4.446 4.705 1.52
930 136.4 4.470 4.696 1.49
940 137.4 4.492 4.687 1.47
950 138.3 4.514 4.678 1.45
960 139.2 4.535 4.670 1.43
970 140.1 4.555 4.661 1.41
980 140.9 4.574 4.652
1000 142.5 4.609 4.635
1020 144.1 4.641 4.618
Density: [22, 54, 60, 81. 166, 212],
Conductance: [1, 10, 21, 23, 60, 72, 100. 166, 212],
Viscosity: [24, 721 .
Melting Point: [130].
56
Table 45. Zinc chloride Table 46. Cadmium chloride
Eq wt 68.15 mp 275 °C (548 °K) Eq wt 91.66 mp 568 °C (841 °K)
k= 0.423433 1.53761 • 10" 3r+ 1.39393 • 1Q 6P
p = 2. 7831 4.48 • 10“ 4rA = 5.3419 • 10 7 exp (24343/RT)
A = 4.8591 • 104 exp (15153/RT)
A= 6096.5 exp (11785/7?D
17 Obtained from smooth curve through experimental
points of Mackenzie and Murphy, since fit to both
exponential and cubic equations is poor.
(593.3672.5 °K)
• io 6P(672.5824.7 °K)10ep
(824.7969.7 °K)
(593.3672.5 °K)
(672.5824.7 °K)
(824.7969.7 °K)
T A K P V
590 0.0398 0.00147 2.519
600 .0727 .00268 2.514 2900
610 .113 .00417 2.510 1760
620 .162 .00594 2.505 1100
630 .218 .00799 2.501 810
640 .282 .0103 2.496 635
650 .353 .0129 2.492 515
660 .433 .0158 2.487 424
670 .521 .01897 2.483 360
680 .635 .0231 2.478
700 .892 .0323 2.469
720 1.235 .0446 2.461
740 1.665 .0599 2.452
760 2.183 .0782 2.443
780 2.789 .0996 2.434
800 3.485 .1240 2.425
820 (4.272) .1514 (2.416)
840 (5.189) .1832 (2.407)
860 (6.188) .2177 (2.398)
880 (7.277) .2551 (2.389)
900 (8.455) .2953 (2.380)
920 (9.724) .3383 (2.371)
940 (11.08) .3842 (2.362)
960 (12.54) .4329 (2.353)
k = 1.9571 + 6.1834 • \0~ 3T 1.9576 • 10 6Fp = 4.078 0.82 • 10 3TA =224.4 exp (2499/RT)
/ 7) = 24.05 • 10 2 exp (3912/RT)
T A K P V
840 50.19 1.8557 3.389
850 51.09 1.8844 3.381
860 51.98 1.9128 3.373
870 52.87 1.9408 3.365 2.31
880 53.75 1.9683 3.356 2.25
890 54.63 1.9955 3.348 2.20
900 55.50 2.0223 3.340 2.14
910 56.36 2.0487 3.332 2.09
920 57.22 2.0747 3.324 2.04
930 58.06 2.1003 3.315 2.00
940 58.91 2.1256 3.307 1.95
950 59.75 2.1504 3.299 1.91
960 60.58 2.1748 3.291 1.87
970 61.40 2.1989 3.283
980 62.22 2.2226 3.274
990 63.02 2.2458 3.266
1000 63.83 2.2687 3.258
1010 64.62 2.2912 3.250
1020 65.41 2.3133 3.242
1030 66.19 2.3350 3.233
1040 66.97 2.3563 3.225
1050 67.73 2.3772 3.217
1060 68.49 2.3977 3.209
1070 69.24 2.4179 3.201
Density: [15, 54, 661 .
Conductance: [19, 27, 33, 51, 66, 941 .
Viscosity: [47, 531 .
Melting Point: [130].
Density: [36, 40, 56, 87, 91, 98, 113],
Conductance: [33, 87, 94, 98, 189].
Viscosity:[981 .
Melting Point: [130].
57
Table 47. Mercury (I) chloride Table 48. Mercury (II) chloride
Eq wt 236.07 mp 306 °C (579 °K) Eq wt 135.76 mp 277 °C (550 °K)
*= 5.255 exp (2644/RT)
p = 9.09284.0 • 10 3T
A = 353.5 exp (3469//?D
T A K P
800 39.88 0.995 5.89
810 40.96 1.015 5.85
820 42.06 1.035 5.81
Density: [36]
.
Conductance: [35]
.
Melting Point: [131].
Table 49. Aluminum (III) chloride
Eq wt 44.45 mp 191.8 °C (465.0 °K)
p=  5.71 1383 + 2.859744 • 10 2T 2.953960 • lO^T 2
p — 10.5980 — 5. 14676 • 10^ 2r+ 8.59674 • 10 5 T 2
4.86480 • lO^ 3
T P V
470 0.348
480 1.2094 .320
490 1.2088 .296
500 1.2024 .275
510 1.1900 .256
520 1.1717 .240
530 1.1476 .226
540 1.1175 .213
550 1.0815 .202
560 1.0395'
570 0.9917
580 .9380
590 .8784
600 .8128
610 .7413
620 .6640
630 .5807
k = 2.060513 • 10 3  1.061468 • 10 5T+ 1.793902 • 108T 2
9.720443 • 10 12T 3
p = 5.9391 2.8624 • 10 37A = 0.1775 exp (5626.7/RT)
r}=  4341.632 + 22.96096 T  4.043872 • 10 2T 2
+ 2.372690 • 10 5T 3
T A • 103 k • 105P V
550 0.9876 3.175 4.3648
560 1.093 3.490 4.336 1.74
570 1.209 3.837 4.306 1.63
580 1.336 4.211 4.279 1.54
590 1.471 4.605 4.250
600 1.612 5.014 4.222
610 (1.758) 5.431 (4.193)
620 (1.907) 5.852 (4.164)
630 (2.058) 6.270 (4.136)
640 (2.207) 6.678 (4.107)
650 (2.354) 7.073 (4.079)
660 (2.496) 7.447 (4.050)
670 (2.632) 7.795 (4.021)
680 (2.758) 8.111 (3.993)
690 (2.873) 8.390 (3.964)
700 (2.975) 8.624 (3.935)
710 (3.061) 8.810 (3.907)
Density: [18, 103, 127],
Conductance: [35, 94, 103, 189 ]
.
Viscosity: [ 103 ]
.
Melting Point: [130].
Density: [ 149 ]
.
Viscosity: X 149 ]
.
Melting Point: [130].
58
Table 50. Gallium (III) chloride Table 51. Indium chloride
Eq wt 58.69 mp 77.6 °C (350.7 °K)
p = 2. 7841 2.0826 • 10" 3r
r) — 42.1652 — 0.251746 T+5. 13276 • 10~ 4 T
3.53160 • 10 7 T3
Eq wt 150.22 mp 225 °C (498 °K)
k =— 2. 0281 + 5.2188 • 103r+ 1.0942 • 10

6T 2
p = 4.43 7 1.40 • 10 3TA = 1208 exp (3528/RT)
T P V
360 2.034 1.58
370 2.014 1.40
380 1.993 1.24
390 1.972 1.10
400 1.951 0.99
410 1.930 .89
420 1.909 .81
430 .74
440 .68
450 .64
460 .60
470 .56
480 .53
490 .50
500 .47
510 .43
520 .39
T A K P
500 (34. 4 ) 0.85 (3.73 7 )
510 (37. 0 ) .92 (3.72s)
520 (39. 8 ) .98 (3.709 )
530 (42. 5 ) 1.05 (3.69 5 )
540 4^CnCO 1.11 3.68,
550 48., 1.17 3.66 7
560 50. 9 1.24 3.65s
570 53. 8 1.30 3.63 9
580 56. 6 1.37 3.62 5
590 59. 6 1.43 3.61,
600 62.5 1.50 3.59 7
610 65.5 1.56 3.58s
620 ON00tit 1.63 3.569
Density: [34]
.
Conductance: [34]
.
Melting Point: [130],
Density: [ 148 . 149].
Viscosity: [149 , 148].
Melting Point: [130].
297268 068 5
59
Table 52. Indium (II) chloride Table 53. Indium (III) chloride
Eq wt 92.84 mp 235 °C (508 °K)
k = 1.2783 + 3.6986 • 10 3T 1.4444 • lO" 6? 2
p = 3. 863 1.60 • lOsT
A = 288.4 exp (3687/RT)
T A K P
510 (7.1) 0.23 2 (3.04 7 )
520 (7.8) ,254 (3.03,)
530 (8.5) .276 ( 3 .OI 5 )
540 9.2 •298 2.99«
550 9.9 •31 9 2.983
560 10.6 •34o 2.96 7
570 11.3 .36, 2.95,
580 12.1 .38, 2.935
590 12.8 .40, 2.919
600 13.5 .42, 2.90s
610 14.2 .440 2.88
620 14.9 •460 2.87,
630 15.6 479 2.855
640 16.3 ,49 7 2.83y
650 17.0 51s 2.82 3
660 17.6 .534 2.807
670 18.3 .55, 2.79,
680 19.0 .569 2.775
690 19.7 586 2.75h
700 20.4 bN0W 2.743
710 21.1 • 62o 2.72 7
720 (21.8) • 636 (2.71,)
730 (22.5) .652 (2.695 )
740 (23.1) •66 s (2.679 )
750 (23.8) COCOMD
( 2 . 663 )
760 (24.5) • 698 (2.64 7 )
770 (25.2) •71.3 (2.63,)
780 (25.8) • 72 8 (2.61 5 )
Eq wt 73.71 mp 586 °C (859 °K)
k= 1.1840.883 • 10

3T
p = 3.944— 2.10 • 10 3TA = 4.112 exp (+ 2181/RT)
T A K P
860 14.64 0.425 2.138
870 14.4a .416 2.11 7
880 14.3, .407 2.096
890 I4 .I 4 .398 2.075
900 13.
9
7 .389 2.05 4
910 13.
7
9 .380 2.03 3
920 13.
6
2 .372 2.01 2
930 13.
4
3 .363 1.99,
940 13.
2
4 .354 1.970
950 (13.05 ) .345 ( 1.94h )
960 (12.86 ) .336 (192s)
970 (12.66 ) .327 (1.90V)
Density: [34].
Conductance: [34],
Melting Point: [130].
Density: [34]
.
Conductance: [34]
.
Melting Point: [130],
60
Table 54. Thallium (I) chloride Table 55. Tin (II) chloride
Eq wt 239.85 mp 429 °C (702 °K)
k= 2.073997 + 4.839529 • 10" 3r+ 4.677176 • lO^'T2
6.884975 • 10"T 3
p = 6.893 1.80 • 10 3 7’
A = 546.0 exp ( 342 1.0/ft T)
T A K P
720 49.44 1.154 5.597
740 52.99 1.228 5.561
760 56.53 1.302 5.525
780 60.06 1.374 5.489
800 63.58 1.445 5.453
820 67.09 1.515 5.417
840 70.58 1.583 5.381
860 74.06 1.650 5.345
880 77.52 1.716 5.309
900 80.97 1.780 5.273
920 84.39 1.843 5.237
940 (87.79) 1.904 (5.201)
960 (91.17) 1.963 (5.165)
980 (94.52) 2.021 (5.129)
1000 (97.84) 2.078 (5.093)
1020 (101.13) 2.132 (5.057)
1040 (104.38) 2.185 (5.021)
1060 (107.60) 2.236 (4.985)
1080 (110.79) 2.286 (4.949)
1100 (113.93) 2.334 (4.913)
1120 (117.03) 2.380 (4.877)
1140 (120.08) 2.424 (4.841)
1160 (123.09) 2.466 (4.805)
Density: [36]
.
Conductance: [21, 189 ]
.
Melting Point: [130],
Eq wt 94.81 mp 245 °C (518 °K)
k = 4.734129 1.434825 • 10 2T 7.776484 • 10 fiT 2
+ 8.757843 • 10 10T3
p = 4.016 1.253 • 10 3T
A = 361.8 exp (2726.9/RT)
T A K P
520 21.06 0.7473 (3.364)
540 25.10 .8842 3.339
560 29.06 1.016 3.314
580 32.94 1.143 3.289
600 36.73 1.264 3.264
620 40.43 1.381 3.239
640 44.04 1.493 3.214
660 47.57 1.600 3.189
680 51.01 1.702 3.164
700 54.36 1.800 3.139
720 57.61 1.892 3.114
740 60.78 1.980 3.089
760 63.85 2.063 3.064
780 66.83 2.142 (3.039)
800 69.71 2.216 (3.014)
820 72.50 2.285 (2.989)
840 75.20 2.350 (2.963)
860 77.79 2.411 (2.938)
880 80.29 2.467 (2.913)
900 82.68 2.519 (2.888)
950 88.22 2.629 (2.826)
1000 93.11 2.713 (2.763)
1050 97.32 2.772 (2.700)
1100 100.8 2.805 (2.638)
1150 103.6 2.814 (2.575)
1200 105.6 2.799 (2.512)
1220 106.2 2.787 (2.487)
1240 106.7 2.770 (2.462)
Density: [25, 36].
Conductance: [35, 189],
Melting Point: [131].
61
Table 56. Tin (IV) chloride Table 57. Lead (II) chloride
Eq wt 65.13 nip 33.3 °C (239.9 °K)
p = 3.01852.687 • 10^ 3Tr? = 3.187 • 10 2 exp (1928/RT)
T P V
280 1.02
290 0.90
300 .81
310 2.186 .73
320 2.159 .66
330 2.132 .60
340 2.105 .55
350 2.078 .51
360 2.051 .47
370 2.024 .44
380 1.997 .41
390 1.971 .38
400 1.944 .36
410 1.917 .34
420 1.890 .32
Density: [ 147 ].
Viscosity: [ 147 , 204].
Melting Point: [130].
Eq wt 139.06 mp 498 °C (771 °K)
* = 0.487664+11.2124 10~3 T 3.9156 • 10“ 6 T 2
p = 6.112 — 1.50 • 10“3 TA = 588.1 exp (4093/RT)
y] = 5.619 • IQ 2 exp (6762//? 7]
T A K P V
780 41.8 1.486 4.942 4.41
790 43.4 1.537 4.927 4.17
800 44.9 1.586 4.912 3.95
810 46.4 1.635 4.897 3.75
820 48.0 1.684 4.882 3.56
830 49.5 1.731 4.867 3.39
840 51.0 1.778 4.852 3.23
850 52.4 1.824 4.837 3.08
860 53.9 1.869 4.822 2.94
870 55.4 1.913 4.807 2.81
880 56.8 1.957 4.792 2.69
890 58.2 2.000 4.777 2.57
900 59.6 2.042 4.762 2.47
910 61.0 2.083 4.747 2.36
920 62.4 2.123 4.732 2.27
930 63.8 2.163 4.717 2.18
940 65.1 2.202 4.702 2.10
950 4.687 2.02
960 4.672 1.95
Density: [15, 40, 54, 150, 212],
Conductance: [7, 51, 72, 85, 97, 151, 212],
Viscosity: [8, 72]
.
Melting Point: [130],
62
Table 58. Bismuth (III) chloride Table 59. Tellurium (II) chloride
Eq wt 105.12 mp 232 °C (505 °K)
k = 4.0243+ 1.6574 • 10 2T 1.9059 10"5 T 2
+ 6.8368 • 10 9 T 3
p= 5.0732.30 10
3 TA = 32.36 exp (981.3IRT)
r}= 0.3787 exp (4693//?T)
T A K P V
510 10.18 0.3780 3.900
520 10.90 .4019 3.877
530 11.57 .4240 3.854
540 12.20 .4445 3.831 30.2
550 12.79 .4635 3.808 27.7
560 13.35 .4808 3.785 25.6
570 13.88 .4967 3.762 23.7
580 14.37 .5110 3.739 22.0
590 14.82 .5240 3.716 20.7
600 15.24 .5355 3.693 19.4
610 15.63 .5457 3.670 18.3
620 15.99 .5546 3.647
630 16.31 .5622 3.624
640 (16.60) .5686 (3.601)
660 (17.09) .5779 (3.555)
680 (17.46) .5827 (3.509)
700 (17.71) .5835 (3.463)
720 (17.86) .5805 (3.417)
740 (17.90) .5741 (3.371)
760 (17.85) .5645 (3.325)
780 (17.70) .5522 (3.279)
800 (17.47) .5374 (3.233)
850 (16.59) .4920 (3.118)
900 (15.34) .4384 (3.003)
Density: [25, 321
.
Conductance: [114,32],
Viscosity: [16].
Melting Point: [130],
Eq wt 99.26 mp 175 °C (448 °K)
k = 0.2949 + 0.3715 • 10 3T+0.6918 • lO" 6! 2
T K
480 0.043
490 .053
500 .064
510 .075
520 .085
530 .096
540 .107
550 .119
560 .130
570 .142
580 .153
Conductance: [ 321 .
Melting Point: [131],
Table 60. Tellurium (IV) chloride
Eq wt 67.36 mp 224 °C (497 °K)
* = 0.6702+1.930 10 3T 0.7617 • 10<T2
T K
510 0 . 11 60
520 .127.5
530 .138.5
540 .150o
550 .161,,
560 •171.5
570 .182.5
580 • 193o
590 .203.5
Conductance: [ 321 .
Melting Point: [130],
63
Table 61. Lithium bromide Table 62. Sodium bromide
Eq wt 86.86 mp 550 °C (823 °K)
k = 1.1362 + 8.6159 • 10 3jT 1.86212 • 10 6T 2
p = 3.0658 0.6520 • 103TA= 585.3 exp ( 2117/RT)
t)= 6.868 • 10 2 exp (5355IRT)
T A K P V
830 162.83 4.7328 2.5246
840 165.16 4.7879 2.5181
850 167.47 4.8426 2.5116
860 169.79 4.8969 2.5051
870 172.11 4.9509 2.4986 1.52,
880 174.43 5.0045 2.4920 1.46a
890 176.75 5.0577 2.4855 1.41 9
900 179.06 5.1105 2.4790 1.372
910 181.38 5.1630 2.4725 1.32
920 183.69 5.2151 2.4660 1,28s
930 186.01 5.2668 2.4594 1.24a
940 188.34 5.3187 2.4529 1.20s
950 190.63 5.3692 2.4464 1.17,
960 192.94 5.4198 2.4399 1.13s
970 195.25 5.4700 2.4334 1.10b
980 197.57 5.5199 2.4268 1.074
990 199.88 5.5694 2.4203 1.04®
1000 202.18 5.6185 2.4138 1.016
1010 204.48 5.6672 2.4073 0.99o
1020 206.79 5.7156 2.4008 •96s
1030 .94o
1040 ,91 7
Density: [3, 81, 821 .
Conductance: [821 .
Viscosity: [47, 1021.
Melting Point: [130]
Eq wt 102.91 mp 750 °C (1023 °K)
k— 9.097 exp (2324/RT)
p = 3. 17480.8169 • 10~ 3rA = 622.7 exp (3228IRT)r,= 64.3240 0.152525 T+ 1.23215 • 10 47 2
3.34241 • 10_8 7’ 3
T A K P V
1030 128.9 2.92i 2.3334
1040 130.8 2.954 2.3252
1050 132.6 2.986 2.3171
1060 134.5 3.018 2.3089 1.28a
1070 136.4 3.049 2.3007 1.24s
1080 138.3 3.080 2.2925 1.21o
1090 140.1 3.111 2.2844 1.178
1100 142.0 3.141 2.2762 1.149
1110 143.9 3.172 2.2680 1.12a
1120 145.8 3.202 2.2599 1.098
1130 147.7 3.231 2.2517 1.07e
1140 149.6 3.261 2.2435 1.05a
1150 151.5 3.290 ’2.2353 1.03a
1160 153.4 3.319 2.2272 1.022
1170 155.3 3.348 2.2190 1.00b
1180 157.2 3.376 2.2109 0.992
1190 159.1 3.404 2.2027 97a
1200 161.0 3.432 2.1945 .96t
1210 162.9 3.460 2.1864 •95s
1220 164.8 3.488 2.1782
Density: [3, 25, 81, 821 .
Conductance: [10, 52, 82, 129, 199].
Viscosity: [12, 102],
Melting Point: [130],
64
Table 63. Potassium bromide Table 64. Rubidium bromide
Eq wt 119.01 mp 735 °C (1008 °K)
k = _6.6001 + 13.1823 10 3r 5.0051 • 10 6r2
p = 2.9583 0.8253 • 103rA = 591.1 exp (
— 3747//?T)
77 = 128.3990.334905 T+ 2.94450 • 10~ 4 T
8.66540 • 10 8T3
T A K P V
1020 92.1 1.639 2.1165 1 . 18s
1030 94.1 1.668 2.1082 1.140
1040 96.1 1.696 2.1000 1.10,
1050 98.0 1.723 2.0917 1.067
1060 99.9 1.749 2.0835 1.037
1070 101.8 1.775 2.0752 1.01,
1080 103.6 1.799 2.0670 0.989
1090 105.3 1.822 2.0587 .969
1100 107.0 1.844 2.0505 .95,
1110 108.7 1.865 2.0422 .93«
1120 110.3 1.886 2.0340 .92,
1130 111.9 1.905 2.0257 •907
1140 113.4 1.923 2.0175 • 89:s
1150 114.9 1.940 2.0092 XCO
1160 116.4 1.957 2.0010 .86:,
1170 117.8 1.972 1.9927 t'00
1180 119.1 1.986 1.9844 .82*
1190
1200
120.4
121.6
1.999
2.011
1.9762
1.9679
Density: [3, 15, 26, 66, 81, 821 .
Conductance: [10, 26, 33, 52, 66, 82, 100, 125, 129],
Viscosity: [12, 47, 1021 .
Melting Point: [130],
Eq wt 165.40 mp 680 °C (953 °K)
k = 5.6453 + 11.1780 • lO^T 4.3285 • 10T 2
p = 3. 7390 1.0718 • 10“3r\= 611.1 exp (4171 /RT)
77 = 51.93960.131564 T+ 1.14887 • 10" 4P3.39298 • 10 8P
T A K P V
960 IA%970 68.9 1.125 2.6994 1.45.3
980 70.9 1.152 2.6886 1.410
990 72.8 1.179 2.6779 1.370
1000 74.7 1.204 2.6672 1.33.3
1010 76.5 1.229 2.6565 1.29s
1020 78.3 1.253 2.6458 1.26e
1030 80.1 1.276 2.6350 1.23e
1040 81.8 1.298 2.6243 1.20b
1050 83.5 1.319 2.6136 1.18,
1060 85.1 1.340 2.6029 1.15s
1070 86.7 1.359 2.5922 1.13.5
1080 88.3 1.378 2.5815 l.lls
1090 89.8 1.396 2.5707 1.09,
1100 91.3 1.413 2.5600 1.07,
1110 92.7 1.429 2.5493 1.052
1120 94.1 1.444 2.5386 1.03.3
1130 95.4 1.459 2.5279 1.01 4
1140 96.7 1.472 2.5171
1150 98.0 1.485 2.5064
1160 99.2 1.497 2.4957
1170 100.4 1.508 2.4850
1180 101.5 1.518 2.4743
Density: [25, 821 .
Conductance: [821 .
Viscosity:[1021 .
Melting Point: [130],
65
Table 65. Cesium bromide Table 66. Magnesium bromide
Eq wt 212.83 mp 636 °C (909 °K) Eq wt 92.08 mp 711 °C (984 °K)
k = 2. 5553 + 4.7068 • 103r 1.1218 • 10" 6Pp = 4.2449 1.2234 • lO^TA = 1169 exp (5533/RT)
T A K P
910 54.3 0.799 3.1316
920 56.3 .826 3.1194
930 58.3 .852 3.1071
940 60.4 .878 3.0949
950 62.4 .904 3.0827
960 64.4 .929 3.0704
970 66 .
4
5 .955 3.0582
980 68.5 .980 3.0460
990 70.5 1.005 3.0337
1000 72.5 1.030 3.0215
1010 74.6 1.054 3.0093
1020 76.6 1.079 2.9970
1030 78.6 1.103 2.9848
1040 8O.65 1.126 2.9726
1050 82.7 1.150 2.9603
1060 84.7 1.173 2.9481
1070 86.7.5 1.197 2.9359
1080 88.8 1.220 2.9236
1090 90.8 1.242 2.9114
1100 92.85 1.265 2.8992
1110 94.9 1.287 2.8869
1120 96.9 1.309 2.8747
1130 99.0 1.331 2.8625
1140 101.0 1.353 2.8502
k = — 0.4257 + 0.5717 • 103r+ 0.5784 • 10 6T 2
p = 3.087 0.478 • 10~3rA = 385.5 exp (5404IRT)
T A K P
1000 (25.
5
6 ) 0.724 (2.510)
1020 (26.8;,) .759 (2.600)
1040 28.2, .795 2.590
1060 29.6> .830 2.581
1080 31.02 .866 2.571
1100 32.46 .903 2.562
1120 33.
9
2 .940 2.552
1140 35.4, .978 2.542
1160 36.
9
3 1.016 2.533
1180 38.
4
7 1.054 2.523
1200 40.04 1.093 2.514
1220 (41.65 ) 1.133 (2.504)
1240 (43.28 ) 1.173 (2.495)
Density: [91, 1 13 1
.
Conductance: [94]
.
Melting Point: [130]
Density: [25,74,82],
Conductance: [82, 199].
Melting Point: [130].
66
Table 67. Calcium bromide TABLE 68. Strontium bromide
Eq wt 99.91 mp 730 °C (1003 °K)
k= 12.820 exp (—4475/RT)
p = 3.618 0.500 • 103rA =506.7 exp (4901 /RT)
T A K P
1020 45.
3
0 1.409 3.108
1040 47.42 1.470 3.098
1060 49.56 1.532 3.088
1080 (51.7,) 1.593 (3.078)
1100 (53.8k) 1.655 (3.068)
1120 (56.
0
7 ) 1.716 (3.058)
1140 (58.28) 1.778 (3.048)
1160 (60.50 )1.840 (3.038)
1180 (62.7a) 1.901 (3.028)
1200 (64.97) 1.963 (3.018)
1220 (67.2a) 2.024 (3.008)
1240 (69.4s) 2.085 (2.998)
1260 (71.
7
6 ) 2.146 (2.988)
1280 (74.a») 2.207 (2.978)
Density: [91, 1131 .
Conductance: [94]
.
Melting Point: [132]
Eq wt 123.73 mp 643 °C (916 °K)
k = 4.0086 + 6.8056 • 10 3T 1.7296 • lO eT 2
p = 4.390 0.745 • 10 3rA = 806.5 exp (6183/^T)
T A K P
940 28.8.5 0.800 3.690
960 31.3a .931 3.675
980 33.7„ 1.000 3.660
1000 36.2a 1.067 3.646
1020 38.6a 1.134 3.631
1040 41.0, 1.198 3.616
1060 43.36 1.262 3.601
1080 45.69 1.324 3.586
1100 47.9s 1.385 3.571
1120 50.
2
4 1.444 3.556
1140 52.4s 1.502 3.541
1160 54.6s 1.559 3.526
1180 56.8s 1.614 3.511
Density: [91, 1131 .
Conductance: [94],
Melting Point: [130]
67
Table 69. Barium bromide Table 70. Lanthanum (III) bromide
Eq wt 148.60 mp 850 °C (1123 °K)
k = 2.4631 + 3.736 • 103T 0.4410 • 106 T2
p = 5.035 0.924 • 103TA = 691.8 exp (6153/RT)
T A K P
1150 46.8 1.250 3.972
1160 47.9 1.277 3.963
1170 49.0 1.304 3.954
1180 50.1 1.331 3.945
1190 (51.3) 1.358 (3.935)
1200 (52.4) 1.385 (3.926)
1210 (53.6) 1.412 (3.917)
1220 (54.7) 1.438 (3.908)
1230 (55.8) 1.465 (3.898)
1240 (57.0) 1.491 (3.889)
1250 (58.1) 1.518 (3.880)
1260 (59.3) 1.544 (3.871)
1270 (60.4) 1.570 (3.862)
1280 (61.6) 1.596 (3.852)
1290 (62.7) 1.622 (3.843)
1300 (63.9) 1.648 (3.834)
1310 (65.1) 1.674 (3.825)
1320 (66.2) 1.700 (3.815)
1330 (67.4) 1.726 (3.806)
Eq wt 126.22 mp 783 °C (1056 °K)
k= 4.7336 10.8289 • 103T+ 6.700 • 1067’2
p = 5.0351 0.096 • 103 TA = 2652 exp ( 10296/RT)
T A K P
1060 20.0 0.783 4.9333
1070 20.9 .818 4.9324
1080 21.8 .853 4.9314
1090 22.8 .890 4.9305
1100 23.8 .929 4.9295
1110 24.8 .969 4.9285
1120 25.9 1.010 4.9276
1130* 27.0 1.052 4.9266
1140 28.1 1.096 4.9257
1150 29.2 1.141 4.9247
1160 30.4 1.188 4.9237
1170 31.7 1.236 4.9228
1180 32.95 1.285 4.9218
1190 34.2 1.335 4.9209
Density: [831 .
Conductance:[83 . 171].
Melting Point: [130].
Density: [66 . 91],
Conductance:[94] .
Melting Point: [130].
TABLE 71. Praseodymium (III) bromide
Eq wt 126.89 mp 691 °C (964 °K)
k =  1.3387+ 1.8574 10~3 T
T K
1000 0.519
1010 .537
1020 .556
1030 .574
1040 .593
1050 .612
Conductance: [ 1711 .
Melting Point: [170],
68
TABLE 72. Neodymium (III) bromide Table 73. Gadolinium (III) bromide
Eq wt 128.01 mp 684 °C (957 °K)
k = 3.2271  7.6760 • 10~3 T+ 4.800 • 10"6 T 1
p = 4.9750 0.7779 • 10~3 TA = 3973 exp (11749/RT)
T A K P
960 8.53 0.282 4.2282
970 9.03 .298 4.2204
980 9.56 .315 4.2127
990 10.12 .332 4.2049
1000 10.71 .351 4.1971
1010 11.33 .371 4.1893
1020 11.99 .392 4.1815
1030 12.67 .413 4.1738
1040 13.40 .436 4.1660
1050 14.14 .460 4.1582
1060 14.92 .484 4.1504
1070 15.74 .509 4.1426
1080 16.59 .536 4.1349
1090 17.47 .563 4.1271
1100 18.38 .592 4.1193
1110 19.33 .621 4.1115
1120 20.31 .651 4.1038
1130 21.32 .682 4.0960
1140 22.37 .714 4.0882
1150 23.46 .748 4.0804
Density: [83].
Conductance: [83,171].
Melting Point: [130].
Eq wt 132.2 mp 770 °C (1043 °K)
#c = 0.98898 +1.3356 • 10"3 T
T K
1070 0.440
1080 .453
1090 .467
1100 .480
1110 .493
1120 .507
Conductance: [ 171] .
Melting Point: [170],
Table 74. Copper (I) bromide
Eq wt 143.46 mp 488 °C (761 °K)
k = 6.342 exp (—1416/RT)
T K
770 2.514
780 2.544
790 2.573
800 2.602
810 2.631
820 2.659
Conductance: [41]
.
Melting Point: [130],
69
Table 75. Silver bromide Table 76. Zinc bromide
Eq wt 187.0 mp 430 °C (703 °K)
k= 0.32105 + 4.8157 • 10 3 T 1.72064 • 10“6 T
p = 6.307  1.035 • 10“3 T
A= 210.2 exp (1104IRT)
v = 37.17470.100768 T+ 9.80868 • 10“ 5r 2
3.25971 • 10~ 8 T3
T A K P V
720 97.4 2.896 5.562 3.30
730 98.35 2.920 5.551 3.20
740 99.3 2.942 5.541 3.11
750 100.2.5 2.965 5.531 3.02
760 101.2 2.987 5.520 2.94
770 102.1 3.009 5.510 2.86
780 103.0 3.030 5.500 2.78
790 104.0 3.052 5.489 2.71
800 104.9 3.072 5.479 2.65
810 105.8 3.093 5.469 2.58
820 106.6 3.113 5.458 2.53
830 107.5 3.133 5.448 2.47
840 108.4 3.152 5.438 2.42
850 109.3 3.171 5.427 2.37
860 110.1 3.190 5.417 2.33
870 111.0 3.208 5.407
880 111.8 3.226 5.396*
890 112.6 3.244 5.386
900 113.5 3.261 5.376
910 114.3 3.278 5.365
920 115.1 3.295 5.355
930 115.9 3.311 5.344
Density: [2, 22, 54s 81].
Conductance: [1, 10, 21. 23, 72, 1001 .
Viscosity: [24, 721 .
Melting Point: [130].
Eq wt 112.61 mp 394 °C (667 °K)
k= 1.22203.9416 10 3T+ 3.1971 • 10 6T 2
p = 4. 113 0.959 • 10~3T
A = 35684 exp ( 14604/7? T)
r) = 400 cp at 400 °C.
T A K P
670 (0.52g) 0.016 (3.470)
680 ( 652 ) .020 (3.461)
690( .797) .024 (3.451)
700 .964 .029 3.442
710 1.152 .035 3.432
720 1.363 .041 3.423
730 1.5% .048 3.413
740 1.85, .056 3.403
750 POi—
1
DO .064 3.394
^760 2.430 .073 3.384
770 2.754 .083 3.375
780 3.10, .093 3.365
790 3.47, .103 3.355
800 3.86b .115 3.346
810 4.284 .127 3.336
820 4.72« .140 3.327
830 5.19, .153 3.317
840 5.684 .167 3.307
850 6.199 .182 3.298
860 6.74o .197 3.288
870 7.30b .213 3.279
880 7.896 .229 3.269
890 (8 .5 I3 ) .246 (3.259)
900 (9.15s) .264 (3.250)
Density: [43, 1 131 .
Conductance: [94, 98].
Viscosity: [981 .
Melting Point: [130],
70
Table 77. Cadmium bromide Table 78. Mercury (II) bromide
Eq wt 136.12 mp 568 °C (841 °K)
k = 1.6351 + 4.1892 • KW 1.1777 • 10“6Pp = 4.9831 — 1.08 • 10 3T
A = 243.4 exp (3226/RT)
r] = 110. 000 + 0.40904271— 4.84560 • 10" 4P
+ 1.87613 • 10~ 7P
T A K P V
850 35.99 1.075 4.065
860 36.82 1.097 4.054 2.73
870 37.64 1.118 4.043 2.65
880 38.46 1.139 4.033 2.57
890 39.27 1.160 4.022 2.49
900 40.09 1.181 4.011 2.41
910 40.89 1.202 4.000 2.34
920 41.70 1.222 3.990 2.28
930 42.50 1.242 3.979 2.22
940 43.30 1.262 3.968 2.17
950 44.09 1.282 3.957 2.13
960 44.88 1.301 3.946
970 45.67 1.320 3.936
980 46.45 1.339 3.925
990 47.2?
48.00
1.358 3.914
1000 1.376 3.903
1010 (48.77) 1.395 (3.892)
1020 (49.54) 1.413 (3.882)
1030 (50.30) 1.430 (3.871)
1040 (51.06) 1.448 (3.860)
1050 (51.81) 1.465 (3.849)
1060 (52.56) 1.482 (3.838)
Eq wt 180.22 mp 237 °C (510 °K)
k = 2.203887 • 103 1.489099 • 10 5T
+ 3.099289 • 10"8P 1.913523 • 10”Pp=6. 77153. 2331 • lO^TA = 0.310523 exp (4065.3/RT)
r]= 1.801 • 10~ 2 exp (5040/RT)
T A • 10 2 k • 104P V
520 0.5328 1.505 5.090
530 .6013 1.688 5.057 2.16
540 .6712 1.872 5.025 1.98
550 .7419 2.056 4.993 1.81
560 .8132 2.239 4.961
570 .8845 2.419 4.928
580 .9556 2.596 4.896
590 1.026 2.769 4.864
600 1.095 2.935 4.831
610 1.162 3.095 4.799
620 (1.227) 3.247 (4.767)
630 (1.290) 3.389 (4.735)
640 (1.350) 3.522 (4.702)
650 (1.406) 3.642 (4.670)
660 (1.457) 3.750 (4.638)
670 (1.505) 3.845 (4.605)
680 (1.546) 3.924 (4.573)
690 (1.583) 3.987 (4.541)
700 (1.612) 4.033 (4.508)
710 (1.635) 4.061 (4.476)
720 (1.650) 4.069 (4.449)
730 (1.657) 4.056 (4.411)
Density: [54].
Conductance: [94]
.
Viscosity: [53]
.
Melting Point: [130].
Density: [18, 103] .
Conductance: [94, 103, 189 ]
.
Viscosity: [6, 58]
.
Melting Point: [131].
71
TABLE 79. Aluminum bromide Table 80. Indium (III) bromide
Eq wt 88.91 mp 97.5 °C (370.7 °K)
rj = 3.491 • 10 2 exp (3123/RT)
T V
380 2.18
390 1.96
400 1.78
410 1.61
420 1.47
430 1.35
440 1.24
450 1.15
460 1.06
470 0.99
480 .92
490 .86
500 .81
510 .76
520 .72
Viscosity: [138,203].
Melting Point: [130].
Eq wt 118.17 mp 436 °C (709 °K)
k =  0.1914+ 1.0056 • 103T 0.7065 • 10~6T 2
p = 4. 184 1.50 • 10~3TA = 6.766 exp (
— 91/RT)
T A K P
710 6.31 0 . 1 664 3.II9
720 6.33 .1664 3.IO4
730 6.36 .166, 3.089
740 6.38 .165s 3.074
750 6.39 • 1654 3.059
760 6.40 .164* 3.044
770 6.40 .164o 3.029
780 6.40 .163! 3.OI4
790 6.39 .162, 2.99a
800 6.37 • 160y 2.984
810 6.35 • 1596 2.96)
Density: [34] .
Conductance: [34]
.
Melting Point: [130].
72
Table 81. Thallium (/) bromide
Eq wt 284.31 mp 459 °C (732 °K)
k= 1.663401 + 4.171786 • 103T 1.098403 • 106Pp = 7.4335  1.922 • 10“3rA = 425.8 exp (3510.8/RT)
T A K P
740 38.89 0.8222 6.011
760 41.54 .8727 5.973
780 44.19 .9223 5.934
800 46.82 .9710 5.896
820 49.46 1.0189 5.857
840 52.08 1.0659 5.819
860 54.69 1.1120 5.781
880 57.29 1.1572 5.742
900 59.89 1.2015 5.704
920 62.48 1.2450 5.665
940 65.06 1.2875 5.627
960 67.62 1.3292 5.588
980 70.18 1.3700 5.550
1000 72.73 1.4100 5.511
1020 75.27 1.4490 5.473
1040 77.80 1.4872 5.435
1060 (80.32) 1.525 (5.396)
1080 (82.83) 1.561 (5.358)
1100 (85.33) 1.596 (5.319)
1120 (87.82) 1.631 (5.281)
Density: [1961 .
Conductance: [21, 1891 .
Melting Point: [130],
73
Table 82. Lead (II) bromide
Eq wt 183.52 mp 370 °C (643 °K)
k = 3.4892 + 8.7490 • 10~3 T 3.7998 • 10"6 T1
p = 6.789 1.65 • 103 TA = 660.8 exp ( 4559/^7’)
7) = 112.439 0.329572 T+ 3.31646 • 10~ 4 P 1.12536 • 10~ 7 P
T A K P T V T ">?
650 (19.01) 0.592 (5.717) 700 5.65 870 2.63
660 (20.28) .630 (5.700) 710 5.35 880 2.55
670 (21.53) .667 (5.684) 720 5.07 890 2.48
680 (22.77) .703 (5.667) 730 4.81 900 2.42
690 (23.99) .739 (5.651) 740 4.56 910 2.36
700 (25.19) .773 (5.634) 750 4.33 920 2.31
710 (26.37) .807 (5.618) 760 4.12 930 2.26
720 (27.53) .840 (5.601) 770 3.93 940 2.21
730 (28.68) .873 (5.585) 780 3.74 950 2.17
740 (29.81) .904 (5.568) 790 3.57 960 2.13
750 (30.91) .935 (5.552) 800 3.42 970 2.09
760 (32.00) .965 (5.535) 810 3.27 980 2.05
770 33.08 .995 5.519 820 3.14 990 2.02
830 3.02 1000 1.98
840 2.91 1010 1.94
850 2.81 1020 1.90
860 2.71
Density: [15, 541 .
Conductance: [7, 72].
Viscosity: [8, 72, 1421 ,
Melting Point: [130].
74
Table 83. Bismuth (III) bromide TABLE 84. Lithium iodide
Eq wt 149.58 mp 218 °C (491 °K)
k=  1.99453 + 8.17416 10~3T 8.99735 • KW 2
+ 3.02196 • 10 9r 3
p = 5.958 2.6 • 103T
A= 16.67 exp (— 535.6/RT)
T A K P
510 7.587 0.2349 4.632
530 8.502 .2603 4.580
550 9.327 .2823 4.528
570 10.064 .3011 4.476
590 10.714 .3169 4.424
610 11.281 .3297 4.372
630 11.765 .3398 4.320
650 12.168 .3472 4.268
670 12.494 .3521 4.216
690 12.743 .3547 4.164
710 12.919 .3551 4.112
730 (13.024) .3535 (4.060)
750 (13.061) .3500 (4.008)
770 (13.032) .3447 (3.956)
790 (12.941) .3378 (3.904)
810 (12.790) .3294 (3.852)
830 (12.583) .3197 (3.800)
850 (12.323) .3088 (3.748)
870 (12.014) .2969 (3.696)
890 (11.660) .2841 (3.644)
910 (11.265) .2705 (3.592)
930 (10.832) .2564 (3.540)
950 (10.368) .2418 (3.488)
970 (9.876) .2269 (3.436)
Eq wt 133.86 mp 449 °C (722 °K)
k = — 3.4283 + 1 .4264 • lO2^ 0.59652 • lO^T 2
p = 3.7902 0.9176 • 10~3T
A = 569.49 exp ( 1809.9/RT)
7]— 17.1272 — 3.14251 • 10" 2r+ 1.54596 • lOT 2
1.34806 • lO'T 3
T A K P V
760 171.7 3.9668 3.0928 2.17
770 174.4 4.0182 3.0836 2.09
780 177.1 4.0683 3.0745 2.01
790 179.8 4.1173 3.0653 1.94
800 182.4 4.1651 3.0561 1.87
810 185.0 4.2117 3.0469 1.81
820 187.6 4.2571 3.0378 1.75
830 190.1 4.3013 3.0286 1.69
840 192.6 4.3444 3.0194 1.63
850 195.0 4.3862 3.0102 1.58
860 197.5 4.4268 3.0011 1.53
870 199.8 4.4663 2.9919 1.48
880 202.2 4.5045 2.9827 1.44
Density: [82].
Conductance: [82, 108,227],
Viscosity: [47],
Melting Point: [130].
Density: [25] .
Conductance: [114].
Melting Point: [130],
297268 068 675
Table 85. Sodium iodide Table 86. Potassium iodide
Eq wt 149.92 mp 662 °C (935 °K)
k = 2.8948 +7.5861 • KW 2.2381 • 10"6 T2
p = 3.6274 0.9491 • 103TA = 694.5 exp (3221/RT)
77= 7.171 • 102 exp (5673/RT)
T A K P V
940 123.8 2.259 2.7352
950 126.1 2.292 2.7258 1.45
960 128.3 2.325 2.7163 1.40
970 130.6 2.358 2.7068 1.36
980 132.8 2.390 2.6973 1.32
990 135.1 2.422 2.6878 1.28
1000 137.3 2.453 2.6783 1.25
1010 139.5 2.484 2.6688 1.21
1020 141.8 2.514 2.6593 1.18
1030 144.0 2.545 2.6498 1.15
1040 146.2 2.574 2.6403 1.12
1050 148.3 2.603 2.6308 1.09
1060 150.5 2.632 2.6214 1.06
1070 152.7 2.660 2.6119 1.03
1080 154.8 2.688 2.6024 1.01
1090 157.0 2.715 2.5929 0.98
1100 159.1 2.742 2.5834 .96
1110 161.2 2.768 2.5739
1120 163.3 2.794 2.5644
1130 165.4 2.820 2.5549
1140 167.5 2.845 2.5454
1150 169.6 2.869 2.5359
1160 171.7 2.894 2.5264
1170 173.8 2.917 2.5170
1180 175.8 2.940 2.5075
1190 177.8 2.963 2.4980
Eq wt 166.02 mp 685 °C (958 °K)
k = 6.1952+ 12.6232 • 10"3r5.0591 • 10 6r2
p = 3.3594 0.9557 • 103TA= 541.2 exp (3442/RT)
7j = 9.836 IQ 2 exp (5343/RT)
T A K P V
980 1.53
990 1.49
1000 94.5 1.36a 2.4037 1.45
1010 96.6 1.393 2.3941 1.41
1020 98.7 1.41 7 2.3846 1.37
1030 100.6 1.43a 2.3750 1.34
1040 102.5 1.46, 2.3655 1.30
1050 104.4 1.48, 2.3559 1.27
1060 106.2 1.50, 2.3464 1.24
1070 108.0 1.51a 2.3368 1.21
1080 109.6 1.537 2.3272 1.19
1090 111.3 1.553 2.3177 1.16
1100 112.8 1.56a 2.3081 1.13
1110 114.4 1.583 2.2986 1.11
1120 115.8 1.597 2.2890 1.09
1130 117.2 1.60a 2.2795 1.06
1140 118.5 1.620 2.2699 1.04
1150 119.8 1.63, 2.2603 1.02
1160 121.0 1.64u 2.2508 1.00
1170 122.1 1.64a 2.2412
1180 123.2 1.656 2.2317
Density: [26, 66, 79, 81],
Conductance: [10, 26, 33, 66, 79, 125, 129],
Viscosity: [47, 1221 .
Melting Point: [130],
Density: [25, 66, 82].
Conductance: [2, 10, 66, 82, 129],
Viscosity: [47, 122] .
Melting Point: [130],
76
Table 87. Rubidium, iodide Table 88. Cesium iodide
Eq wt 212.40 mp 640 °C (913 °K)
K= 2.5050 + 5.3229 • 103r 1.8114 • 106T2
p= 3.9499 1.1435 • 10~3:T
A = 568.1 exp (3999IRT)
r}= 35. 1934 8.85769 • 10 2T+ 7.79282 • 10 5r2
2.34005 • 10r*T*
T A K P V
930 64.7 0.879 2.8864 1.39
94Q 66.3 .898 2.8750 1.35
950 68.0 .917 2.8636 1.31
960 69.7 .936 2.8521 1.27
970 71.3 .954 2.8407 1.24
980 73.0 .972 2.8293 1.21
990 74.6 .989 2.8178 1.17
1000 76.2 1.007 2.8064 1.14
1010 77.8 1.023 2.7950 1.12
1020 79.3 1.040 2.7835 1.09
1030 80.9 1.056 2.7721 1.06
1040 82.4 1.072 2.7607 1.04
1050 84.0 1.087 2.7492 1.01
1060 85.5 1.102 2.7378 0.99
1070 87.0 1.117 2.7264 .97
1080 88.5 1.131 2.7149 .95
1090 89.9 1.145 2.7035 .93
1100 91.4 1.158 2.6921 .91
1110 92.8 1.172 2.6806 .89
1120 94.3 1.184 2.6692 .86
1130 95 7 1.197 2.6577
1140 97 0 1 209 2.6463
1150 98.4 1.221 2.6349
1160 99.8 1.232 2.6234
Density: [25, 821 .
Conductance: [82].
Viscosity: [1221 .
Melting Point: [130],
Eq wt 259.83 mp 621 °C (894 °K)
k= 2.4630 + 4.5942 • 10 3T 1.2749 • 10~ GT 2
p = 4.2410 1.1834 • 103TA =1125 exp (5450//? T)
77= 41.8211 — 0.101 156T+ 8.49570 • 10“5r2
2.42543 • 10 8T3
T A K P V
910 1.84
920 1.78
930 58.49 0.7069 3.1404 1.72
940 60.55 .7290 3.1286 1.66
950 72.60 .7509 3.1168 1.60
960 64.64 .7725 3.1049 1.55
970 66.68 .7938 3.0931 1.50
980 68.71 .8149 3.0813 1.45
990 70.75 .8357 3.0694 1.41
1000 72.77 .8563 3.0576 1.37
1010 74.78 .8766 3.0458 1.33
1020 76.79 .8967 3.0339 1.29
1030 78.80 .9165 3.0221 1.26
1040 80.79 .9360 3.0103 1.23
1050 82.78 .9553 2.9984 1.19
1060 84.77 .9744 2.9866 1.17
1070 86.75 .9932 2.9748 1.14
1080 88.72 1.0117 2.9629 1.11
1090 90.68 1.0300 2.9511 1.09
1100 92.64 1.0480 2.9393 1.06
1110 94.59 1.0658 2.9274 1.04
1120 96.54 1.0833 2.9156 1.02
1130 98.48 1.1005 2.9038
Density: [25, 74, 82].
Conductance:[821 .
Viscosity: [122].
Melting Point: [130],
77
Table 89. Magnesium iodide Table 90. Calcium iodide
Eq wt 139.08 mp < 637 °C (< 910 °K) E9 wt 14696 mp 575 °C (848 °K)
k = 0.7656 + 0.8785 • 10 3T+ 0.4299 • lO^T 2
p = 3.642 0.651 • 103T
A= 751.1 exp (— 6752IRT)
T A K P
920 18.5s 0.406 3.043
940 20.
2
0 .440 3.030
960 21.85 .474 3.017
980 23.5s .508 3.004
1000 25.
2
4 .543 2.991
1020 26.% .578 2.978
1040 28.
7
6 .613 2.965
1060 30.
5
6 .649 2.952
1080 (32.40 ) .685 (2.939)
1100 (34.
2
7 ) .721 (2.926)
1120 (36.
1
7 ) .758 (2.913)
1140 (38.1,) .795 (2.900)
1160 (40.0k) .832 (2.887)
1180 (42.
0
9 ).870 (2.874)
Density: [91, 1131.
Conductance: [94].
Melting Point: [94],
k= 4.6282 + 8.2567 • lO3/1 2.6610 • 10 67 2
p= 4.233 0.751 • 103TA = 440.3 exp (4617AR7
1
)
T A K P
1060 48.49 1.1340 3.437
1070 49.70 1.159a 3.429
1080 50.90 1.185 2 3.422
1090 52.08 1.210, 3.414
1100 53.25 1.2344 3.407
1110 54.39 1.258, 3.399
1120 55.52 1.281s 3.392
1130 56.63 1.304o 3.384
1140 57.72 1.3262 3.377
1150 58.79 1.3478 3.369
1160 59.84 1.3689 3.362
1170 60.88 1.3895 3.354
1180 61.89 1.409,5 3.347
1190 62.89 1.429o 3.339
1200 63.86 1 .448o 3.332
1210 64.83 1.4664 3.324
1220 65.76 1.484s 3.317
1230 66.96 1.501 7 3.309
1240 67.59 1.518b 3.302
1250 68.48 1.5349 3.294
1260 69.33 1.5506 3.287
1270 70.18 1.565a 3.279
1280 70.99 1.5806 3.272
1290 71.81 1.594k 3.264
Density: [91, 113 ],
Conductance: [94].
Melting Point: [131]
78
Table 91. Strontium iodide Table 92. Barium iodide
Eq wt 170.74 mp 515 °C (788 °K)
k=  1.8747 + 3.3276 • 10“ 3:T 0.5169 • 106T 2
p = 4.803 0.885 • lO'T
A = 610.1 exp (5409IRT)
T A K P
820 21 . 2 0 0.506 4.077
840 23.
3
7 .556 4.060
860 25.5s .605 4.042
880 27.
7
2 .653 4.024
900 29 . 89 .701 4.007
920 32.
0
7 .749 3.989
940 34.2s .797 3.971
960 36.4a .843 3.953
980 38.6, .890 3.936
1000 40.7,, .936 3.918
1020 42.
9
7 .982 3.900
1040 45.
1
6 1.027 3.883
1060 47.3s 1.072 3.865
1080 49.
5
4 1.116 3.847
1100 51.73 1.160 3.830
1120 53.
9
2 1.204 3.812
1140 56.
1
2 1.247 3.794
1160 58.3, 1.290 3.776
1180 60.5, 1.332 3.759
1200 62.7, 1.374 3.741
1220 64.
9
2 1.416 3.723
1240 67.
1
2 1.457 3.706
1260 69.3a 1.497 3.688
1280 71.
5
4 1.538 3.670
Density: [91, 113].
Conductance: [94]
.
Melting Point: [130]
Eq wt 195.59 mp 740 °C (1013 °K)
* = 2.1845 + 3.3755 • 10~3T 0.4666 • lO^T 2
p = 5.222 0.977 • lO^rA =831.2 exp (6367IRT)
T A K P
1020 (35.7s) 0.77a (4.225)
1040 38. 2„ .82, 4.206
1060 40.6, .869 4.186
1080 43.0a • 91 7 4.167
1100 45.4s .964 4.147
1120 47.89 1 . 01 , 4.128
1140 50.3a 1.05 7 4.108
1160 52.
7
7 1 . 10a 4.089
1180 55.
2
2 1.14s 4.069
1200 57. 68 1.194 4.050
1220 60.
1
4 1.23s 4.030
1240 62.
6
0 1.284 4.011
1260 (65.0 8 ) 1.32 8 (3.991)
1280 (67.5s) 1 .37 2 (3.971)
Density: [91, 113 ]
.
Conductance: [94]
.
Melting Point: [130]
Table 93. Aluminum (III) iodide
Eq wt 135.91 mp 191 °C (464 °K)
k= 0.1721 • 10“ 4 + 0.8131 • 10«r+ 0.6801 • lO'T 2
p = 4.383 — 2.50 • 10~3T
A = 1 18670 exp (  1 1160IRT)
T A • 104 k • 10yP
470 0.69 I .63 3.20b
480 1.01 2.36 3.18a
490 1.33 3.1o 3.15b
500 1.67 3.8k 3.13a
510 2.02 4.6a 3.10s
520 2.38 5.4, 3.08a
530 2.75 6 . 20 3.05s
79
Density: [35]
.
Conductance: [35] .
Melting Point: [130].
Table 94. Lanthanum (III) iodide Table 96. Praseodymium (III) iodide
Eq wt 173.23 mp 761 °C (1034 °K)
k = 0.9535+ 1.319 • 10~*T
T K
1070 0.4578
1080 • 471o
1090 .4842
1100 ,4974
1110 ,5106
1120 .5238
1130 ,537o
1140 .5502
Conductance: f 106]
.
Melting Point: [130],
Table 95. Cerium (III) iodide
Eq wt 173.63 mp 752 °C (1025 °K)
k = 0.8580+ 1.221 • lOT
T K
1070 0.448,5
1080 .4607
1090 •4729
1100 .485i
1110 4973
1120 •5095
1130 ,521 7
Eq wt 173.89 mp 743 °C (1006 °K)
k = 0.7724+ 1.1304 • lO^T
T K
1030 0.3919
1040 .4033
1050 .4146
1060 .4259
1070 .4372
1080 .4485
1090 .4598
Conductance: [1061 .
Melting Point: [130],
Table 97. Neodymium (III) iodide
Eq wt 175.01 mp 775 °C (1048 °K)
k — 0.71933 1.040 • 10 3T
T K
1080 0.4039
1090 .4143
1100 .4247
1110 .435,
Conductance: [ 1061 .
Melting Point: [130],
Conductance: f 106]
.
Melting Point: [130],
80
Table 98. Silver iodide Table 99. Zinc iodide
Eq wt 234.80 mp 558 °C (831 °K)
k = 4.674 exp (— 1146//?7’)
p=6.415 i.oi • io3r
A = 239.9 exp (U75/RT)
v = 1 16. 161  0.3336407’+ 3.30383 • 10~ 4T2
1.10721 • 10

7 T 3
T A K V
840 (99) 2.35 (5.567)
850 (100 )2.37 (5.557)
860 (101 )2.39 (5.546)
870 102 2 41 5 536
880 103 2.43 5.526 2.95
890 104 2.45 5.516 2.86
900 105 2.46 5.506 2.78
910 106 2.48 5.496 2.70
920 107 2.50 5.486 2.63
930 108 2.52 5.476 2.56
940 109 2.53 5.466 2.50
950 110 2.55 5.456 2.44
960 110.5 2.56 5.445 2.39
970 111.5 2.5P 5.435 2.34
980 112 2.60 5.425 2.28
990 113 2.61 5.415 2.23
1000 114 2.63 5.405 2.18
1010 115 2.64 5.395 2.13
1020 116 2.66 5.385 2.08
1030 117 2.67 5.375 2.03
1040 117.5 2.69 5.365 1.97
1050 118.5 2.70 5.355 1.91
1060 119 2.71 5.344 1.85
1070 120 2.73 5.334 1.78
1080 121 2.74 5.324 1.71
1090 1.63
1100 1.55
Eq wt 159.61 mp 446 °C (719 °K)
k = 0.6723 2.6838 • lO^TT 2.5446 • 10 fiT 2
p = 4.856 1.360 • 103rA= 17880 exp (  12636/RT)
T A K P
720 2.43 0.059 3.877
730 2.86 .069 3.864
740 3.30 .080 3.850
750 3.78 .091 3.837
760 4.27 .102 3.823
770 4.80 .114 3.809
780 5.34 .127 3.796
790 5.92 .140 3.782
800 6.51 .154 3.767
810 7.14 .168 3.755
820 7.79 .183 3.741
830 8.47 .198 3.728
840 9.17 .213 3.714
850 9.90 .230 3.701
860 10.66 .246 3.687
870 11.45 .263 3.673
Density: [91, 113 1
.
Conductance: [94, 189],
Melting Point: [130],
Density: [22].
Conductance: [1, 10, H, 21, 23, 35].
Viscosity: [24]
.
Melting Point: [130],
81
Table 100. Cadmium iodide Table 101. Mercury (II) iodide
Eq wt 183.13 mp 387 °C (660 °K)
k=  1.0841 + 1.7574 • 103r+ 0.2449 • 106r2
p = 5. 1331. 117 • 103TA= 1109.0 exp (6365ART)
T A K P
680 9.4 0.224 4.373
690 10.3 .245 4.362
700 11.2 .266 4.351
710 12.1 .287 4.340
720 13.0.5 .308 4.329
730 13.
9
5 .329 4.318
740 14.9 .351 4.306
750 15.8s .372 4.295
760 16.8 .393 4.284
770 17.7s .414 4.273
780 18.7 .436 4.262
790 19.7 .457 4.251
800 20.6s .479 4.239
810 21.6s .500 4.228
820 22.6s .522 4.217
830 23.65 .543 4.206
840 24.6s .565 4.195
850 25.7 .587 4.184
860 26.7 .608 4.172
870 27.7s .630 4.161
880 28.7s .652 4.150
890 29.8 .674 4.139
900 30.8s .696 4.128
910 31.9s .718 4.117
Density: [661 .
Conductance: [66, 941 .
Melting Point: [130],
Eq wt 227.23 mp 257 °C (530 °K)
k= 0.3033113 1.075096 • 10“3r+ 1.411112 • 10“6r 2
6.651402 • 10 1(T 3
P = 6.9435 3.2351 • 103TA = 0.07345 exp (3114.3/A7
7
)
rj = 4.00 • 10 2 exp (4531/RT)
T A K P
530 1.341 0.03087 5.229
540 1.290 .02950 5.197
550 1.241 .02821 5.164 2.53
560 1.194 .02697 5.132 2.35
570 1.150 .02580 5.099 2.19
580 1.107 .02468 5.067 2.04
590 1.065 .02361 5.035 1.91
600 1.026 .02258 5.002 1.79
610 0.9877 .02160 4.970 1.68
620 .9508 .02066 4.938 1.58
630 .9151 .01975 4.905 1.49
640 DO DOODO .01888 4.873
650 .8463 .01803 4.841
660 (.8130) .01720 (4.808)
670 (.7800) .01640 (4.776)
680 (.7474) .01560 (4.744)
690 (.7148) .01482 (4.711)
700 (.6821) .01405 (4.679)
710 (.6491) .01327 (4.647)
720 (.6156) .01250 (4.614)
730 (.5813) .01172 (4.582)
Density: [18, 78, 1031 .
Conductance: [29, 94, 103. 1891 .
Viscosity: [6, 78, 103] ,
Melting Point: [130],
82
Table 102. Gallium (II) iodide Table 103. Indium (III) iodide
Eqwt 161.78 mp < 150 °C (< 423 °K)
k= 0.4546+ 1.149 • 10~3T
p = 4.841 1.688 • 10 3TA= 771.8 exp (5121 /RT)
T A K P
430 1.6 0.04 4.115
440 2.o .05 4.098
450 25 .06 4.081
460 2.9 .07 4.064
470 3.4 .08 4.048
480 3.9 .10 4.031
490 4.4 .11 4.014
500 4.9 .12 3.997
510 5.3 .13 3.980
520 5.8 .14 3.963
530 63 .15 3.946
540 6.8 .17 3.929
550 (7.3) .18 (3.913)
560 (7.8) .19 (3.896)
570 ( 8 . 4 ) .20 (3.879)
580 ( 8 . 9 ) .21 (3.862)
590 (9.4) .22 (3.845)
600 (9.9) .23 (3.828)
610 ( 10 . 4 ) .25 (3.811)
620 (ll.o) .26 (3.794)
Density: 1 105] .
Conductance: [105].
Melting Point: [105].
Eq wt 165.17 mp 210 °C (483 °K)
k= 0.4380474 +1.734687 • lO^T 1.759083 • 10 6T 2
+ 5.775249 • 10 ,07’3
p = 4.5448 1.50 • 10 3TA= 18.26 exp ( 1779.9/RT)
T A K P
500 2.686 0.06172 3.795
520 3.051 .06954 3.765
540 3.391 .07667 3.735
560 3.707 .08315 3.705
580 4.000 .08900 3.675
600 4.271 .09424 3.645
620 4.519 .09891 3.615
640 4.747 .1030 3.585
660 (4.954) .1066 (3.555)
680 (5.142) .1097 (3.525)
700 (5.311) .1124 (3.495)
720 (5.462) .1146 (3.465)
740 (5.596) .1164 (3.435)
760 (5.714) .1178 (3.405)
780 (5.817) .1188 (3.375)
800 (5.905) .1196 (3.345)
820 (5.980) .1200 (3.315)
840 (6.043) .1202 (3.285)
860' (6.095) .1201 (3.255)
880 (6.136) .1198 (3.225)
Density: [34]
.
Conductance: [34, 189]
.
Melting Point: [130],
83
TABLE 104. Thallium (/) iodide Table 105. Lead (//) iodide
Eq wt 331.31 mp 440 °C (713 °K)
k =  1.261276 + 3.023831 • 10“ 3r 7.494862 • 10~ 7T2
Eq wt 230.53 mp 402 °C (675 °K)
k = ~ 0.6501 + 1 .0054 • 10 3T+ 0.7888 10 6T2
T K T K
720 0.527 680 0.399
740 .566 690 .419
760 .604 700 .440
780 .641 710 .442
800 .678 720 .483
820 .714 730 .504
840 .750 740 .526
860 .785 750 .548
880 .819 760 .570
900 .853 770 .592
920 .886 780 .614
940 .919 790 .636
960 .951 800 .659
980 .982 810 .682
1000 1.013 820 .704
1020 1.043 830 .727
1040 1.073 840 .751
1060 1.102 850 .775
1080 1.130 860 .798
1100 1.158 870 .822
1120 1.185
1140 1.212
1160 1.238 Conductance: [1081.
1180 1.263 Melting Point: [131].
1200 1.288
1250 1.347
1300 1.403
1340 1.445
Conductance: [21, 125c, 189 ]
.
Melting Point: [130],
84
Table 106. Bismuth ( III ) iodide Table 108. Sodium carbonate
Eq wt 199.59 mp 418 °C (681 °K)
k =  0.9306 + 3.0374 • 10 3T 1.8477 • 10 6P
T K
690 0.286
700 .290
710 .295
720 .298
730 .302
740 .305
750 .308
760 .311
770 . .313
Conductance:(1041 .
Melting Point: [104],
Table 107. Lithium carbonate
Eq wt 36.94 mp 618 °C (891 °K)
k = 0.9877 1.3529 • 10 3r+ 4.3873 • 10 6r2
p = 2.2026 0.3729 • 10 3rA = 754.5 exp (4438//?7
T
)
7j=  5259. 12 +14.8091 T 1.38581 • 10“ 2r2
+ 4.31294 • 10 6P
Eq wt 53.00 mp 854 °C (1127 °K)
k— 13.758 exp (3527/K7V
p = 2.4797 0.4487 • 10“ 3rA = 550.2 exp ( 4199/RT)
rj = 3.832 10” 5 exp (26260/RT)
T A K P V
1140 78.08 2.900 1.9682
1150 79.33 2.939 1.9637
1160 80.5 7 2.978 1.9592 3.40
1170 00 h
J
boto 3.018 1.9547 3.08
1180 83.
0
7 3.057 1.9502 2.80
1190 84.32 3.096 1.9457 2.55
1200 85.
5
7 3.134 1.9413 2.32
1210 86.83 3.173 1.9368 2.12
1220 88.0s 3.211 1.9323 1.94
1230 89.34 3.249 1.9278 1.78
1240 90.5y 3.288 1.9233 1.63
1250 1.9188
1260 1.9143
1270 1.9099
1280 1.9054
Density: [3, 101 j.
Conductance: [4, 101]
Viscosity: [107, 128].
Melting Point: [130].
T A K P V
1010 82.88 4.097 1.8260
1020 84.58 4.172 1.8222
1030 86.31 4.249 1.8185
1040 88.06 4.326 1.8148
1050 89.83 4.404 1.8111 4.64
1060 91.63 4.483 1.8073 4.34
1070 93.46 4.563 1.8036 4.01
1080 95.31 4.644 1.7999 3.67
1090 97.19 4.726 1.7961 3.36
1100 99.09 4.808 1.7924 3.10
1110 101.02 4.892 1.7887 2.91
1120 102.98 4.976 1.7850 2.83
Density: [3, 101 ].
Conductance: [101].
Viscosity: [107, 128],
Melting Point: [131].
85
Table 109. Potassium carbonate Table 111. Sodium nitrite
Eq wt 69.1 mp 896 °C (1169 °K) Eq wt 69.01 mp 285 °C (558 °K)
k= 11.027 exp (3941 /RT)
p = 2.4141 0.4421 • 10 3 r’
A = 544.6 exp (4650/RT)= 1.161 • 10 3 exp (29,487/RT)
T A K P V
1180 74.98 2.053 1.8924
1190 76.
2
2 2.083 1.8880 3.03
1200 77.
4
7 2.112 1.8836 2.73
1210 78.7 2 2.141 1.8792 2.46
1220 79.9 7 2.170 1.8747 2.23
1230 81.
2
3 2.199 1.8703 2.02
1240 82. 4y 2.227 1.8659 1.83
1250 83.7s 2.256 1.8615 1.66
1260 85.0! 2.285 1.8571
1270 86.28 2.313 1.8526
1280 87.5s 2.342 1.8482
Density: [3, 101 ],
Conductance: [4, 101]
Viscosity: [107, 128],
Melting Point: [130],
k= 13.2 exp (2600/RT)
p = 2.226 0.746 10 3T
A = 685.7 exp (2949/RT)rj= 187.1180.8760947’+ 1.41024 • 10“ 3r 2 T  7.71
7.71608 10 7r3
T A K P f)
570 50.9 1.329 1.801 3.04
580 53.2 1.38s 1.793 2.84
590 55.5 1.43 7 1.786 2.66
600 57.9 1.49! 1.778 2.48
610 60.2 1.54s 1.771 2.31
620 62.6 1.60o 1.763
630 65.0 1.654 1.756
640 67.4 1.704 1.749
650 69.9 1.76s 1.741
660 72.4 1.81s 1.734
670 74.9 1.872 1.726
680 77.4 1.92? 1.719
690 79.9'
COO)r—
1
1.711
700 82.5 2.036 1.704
710 85.0 2.09,, 1.696
720 87.6 2.144 1.689
Density: [66, 110],
Table 110. Lithium nitrite Conductance: [66, 110, 125c* 207],
Viscosity: [110, 125c, 2071 .
Eq wt 52.94 mp 220 °C (493 °K) Melting Point: [207],
k =  0.397585 1.51836 • 10 3T+ 7.33374 • 10 6Prj = 14909.1 + 87.5812T 0.1710737’ 2
+ 1.11184 • 10 4T 3
Conductance: [66, 2071 .
Viscosity:[207] .
Melting Point: [207].
86
Table 112. Potassium nitriteTable 114. Cesium nitrite
Eq wt 105.11 mp 419 °C (692 °K) EcIwt 178 92 mp 406 °C (679 °K)
k = 4.167433 +1.148389 • lO 2^ 5.451471 • lOT 2
p = 2. 1676.6 • lO*/’
A = 776.99 exp (3267.2/RT)
rj = 864. 798 3.617607’+ 5.06274 • 10 3T 2
2.36530 • 10~«T3
T A K P i?
700 1.92
710 76.62 1.238 1.698 1.86
720 79.21 1.275 1.692 1.81
730 81.75 1.311 1.685
740 84.25 1.345 1.679
750 86.69 1.379 1.672
Conductance:[207 ],
Density:[173 ].
Viscosity: [110, 125c, 207, 208].
Melting Point: [110].
k= 0.92278 + 2.39945 • 103 Tt) — 1 82.963 + 0.828051 T 1.21 823 • 10 3 r 2
+ 5.90224 • 107T3
T K V
690 0.7328 2.29
700 .7568 2.19
710 .7808 2.09
720 .8048 2.00
730 .8288 1.93
740 1.86
Conductance: [207] ,
Viscosity: [2071 .
Melting Point: [207].
Table 113. Rubidium nitrite
Eq wt 131.49 mp 418 °C (691 °K)
k = 4.54416 +1.189408 • lO" 2 /1 5.890905 • lO'T 2
7}= 8.754 • 10 2 exp (4495/RT)
T K V
720 0.966 2.03
730 .999 1.94
740 1.031 1.86
750 1.063 1.79
760 1.093
Conductance:[207 1.
Viscosity: [207] .
Melting Point: [207].
Table 115. Barium nitrite
Eq wt 114.69 mp 267 °C (540 °K)
k = 1.284 + 2.65 • 10 3 T
p = 3.6397.0 • 10 4 T
A= 10217 exp (—8103.8/RT)
T A K P
550 6.115 0.1735 3.254
560 7.064 .2000 3.247
570 8.017 .2265 3.240
580 8.975 .2530 3.233
590 3.226
600 3.219
610 3.212
620 3.205
87
Conductance:[1851 .
Density: [1731 .
Melting Point: [39].
Table 116. Lithium nitrate Table 117. Sodium nitrate
Eq wt 68.95 mp 254 °C (527 °K)
k= 1.5242 + 3.4674 • 10 3T+ 1.8027 • 10“ 6 T2
p = 2.068 0.546 • 10~ 3TA = 967.8 exp (3589jRT)
r] = 20.4645 + 1.34189 • 10 2T 1.31061 • 104P+ 1.06106 10~7T S
T A K P V
550 36.2 0.928 1.768 5.85
560 38.5 .983 1.762 5.51
570 40.7 1.038 1.757 5.18
580 43.0 1.093 1.751 4.86
590 45.4 1.149 1.746 4.55
600 47.7 1.205 1.740 4.25
610 50.1 1.262 1.735 3.97
620 52.6 1.318 1.729 3.69
630 55.0 1.376 1.724 3.43
640 57.5 1.433 1.719 3.18
650 1.713 2.95
660 1.708 2.74
670 1.702 2.53
680 1.697 2.35
690 1.691 2.18
700 2.03
Density: [26. 180, 224].
Conductance: [26, 93, 116 , 195, 224],
Viscosity: [5, 38, 139, 228].
Melting Point: [130].
Eq wt 85.01 mp 310 °C (583 °K)
k =  1.5713 + 4.3835 • 10“ 3 T
p = 2.3200.715 • 10 3 TA = 705.6 exp (3215IRT)
7]= 10.41 • IQ 2 exp (3886jRT)
T A K P V
590 45.
4
5 1.015 1.898 2.86
600 47.6 1.059 1.891 2.71
610 49.7s 1.103 1.884 2.57
620 51.9s 1.146 1.877 2.44
630 54.1 1.190 1.870 2.32
640 56.3s 1.234 1.862 2.21
650 (58.5s) 1.278 (1.855) 2.11
660 (60.8 ) 1.322 (1.848) 2.01
670 (63.0s) 1.366 (1.841) 1.93
680 (65.3s) 1.409 (1.834) 1.85
690 (67.6s) 1.453 (1.827) 1.77
700 (69.9s) 1.497 (1.820) 1.70
710 1.63
720 1.57
730 1.52
Density: [15, 26, 61, 661 .
Conductance: [7, 26, 27, 61, 66, 71, 75, 93, 192, 224].
Viscosity: [5, 8, 12, 38, 102, 228].
Melting Point: [130].
88
Table 118. Potassium nitrate Table 119. Rubidium nitrate
Eq wt 101.10 mp 337 °C (610 °K)
k= 1.4347 + 3.7376 • 10 3T 0.5779 • 10“ 6r2
p = 2.3150. 729 10 3T
A = 657.4 exp (3577/RT)
r] = 50.1676  0.164572 T+ 1.86335 • 10~ 4 T1
7.12497 • 108 T3
T A K P V
620 35.8,5 0.660 1.863
630 37.6 .691 1.856 2.63
640 39.4 .721 1.848 2.49
650 41.2 .751 1.841 2.36
660 43.0 .780 1.834 2.23
670 44.85 .810 1.827 2.12
680 46.65 .840 1.819 2.02
690 48.5 .869 1.812 1.92
700 50.35 .898 1.805 1.88
710 52.2 .928 1.797 1.75
720 54.05 .957 1.790 1.69
730 55.9 .986 1.783 1.61
740 57.8 1.015 1.776 1.55
750 59.65 1.043 1.768 1.49
760 61.55 1.072 1.761 1.44
770 63.
4
5 1.101 1.754 1.40
780 65.
3
5 1.129 1.746 1.36
790 67.3 1.157 1.739 1.32
800 69.2 1.186 1.732 1.28
810 71.
1
5 1.214 1.725. 1.25
820 73.1 1.242 1.717
830 75.05
77.0
1.269 1.710
840 1.297 1.703
850 79.0 1.325 1.695
860 81.0 1.352 1.688
870 83.0 1.380 1.681
Density: [15, 26, 38, 66, 84, 173, 177, 184, 192, 210],
Conductance: [7, 20„ 26, 27, 66, 84, 92, 116, 192, 193,
194, 224],
Viscosity: [5, 8, 12, 38, 57, 102, 107, 228],
Melting Point: [130],
Eq wt 147.49 mp 316 °C (589 °K)
k — 1.3769 + 3.8156 • 10 3T 1.2658 • 10T2
p = 3.049 0.972 • 10 3TA = 515.7 exp (3496/RT)
r\ = 190.972  0.791802 T + 1.11940 • 10" 3r2
 5.33333 • 10T3
T A K P V
590 25.8 0.434 2.476
600 27.3 .457 2.466 3.68
610 28.8 .480 2.456 3.45
620 30.3 .502 2.446 3.24
630 31.7 .525 2.437 3.07
640 33.2 .547 2.427 2.92
650 34.7 .568 2.417 2.78
660 36.1 .590 2.407 2.66
670 37.6 .611 2.398 2.56
680 39.1 .632 2.388 2.46
690 40.5 .653 2.378 2.37
700 42.0 .673 2.369
710 43.4 .694 2.359
720 44.8 .714 2.349
730 46.3 .734 2.339
740 47.7 .753 2.330
750 49.1 .773 2.320
760 50.6 .792 2.310
Density:[261 .
Conductance: [26, 224].
Viscosity: [ 139 , 228],
Melting Point: [130],
89
Table 120. Cesium nitrate Table 121. Silver nitrate
Eq wt 194.92 mp 414 °C (687 °K)
* = 0.7610+ 1.887 • 10 3T
p = 3. 6206 1.16605 • 10 3rA = 552.4 exp (— 3688//?7
1
)
17= — 41.3159 + 0. 2 14037
1— 3.32966 • 10~4T 2
+ 1.65583 • \0~ 7T3
T A K P V
690 37.49 0.5416 2.8160 2.23
700 38.96 .5605 2.8044 2.15
710 40.44 .5794 2.7927 2.06
720 41.93 .5983 2.7810 1.98
730 43.44 .6171 2.7694 1.90
740 44.95 .6360 2.7577 1.83
750 46.48 .6549 2.7461 1.77
760 48.03 .6738 2.7344 1.71
Density: [26, 84J.
Conductance: [26, 84, 224],
Viscosity: [139, 228].
Melting Point: [131],
Eq wt 169.89 mp 210 °C (483 °K)
k = 1.9314 + 6.2321 • 10 3T 1.7924 • 10 6T2
p = 4.454 1.02 • 10 3TA = 587.9 exp (2898/RT)
t? = 81.7743 0.336741 7+4.80289 • 10 4T 2
2.32448 • 10 7 T 3
T A K P V
490 (29.
7
3 ) 0.692 (3.954)
500 (31.
7
3 ) .737 (3.944 )
510 (33.72 ) .781 (3.934)
520 (35.7,) .825 (3.924)
530 (37.69) .868 (3.913) 3.61
540 (39.6fi ) .911 (3.903) 3.38
550 41.
6
3 .954 3.893 3.18
560 43.6 (, .996 3.883 3.00
570 45.
5
6 1.038 3.873 2.83
580 47.5 2 1.080 3.862 2.68
590 49.
4
7 1.122 3.852 2.55
600 51.4, 1.163 3.842
Density: [25 , 36, 54, 60, 224],
Conductance: [5, 60, 78, 135, 181, 194, 219, 224].
Viscosity: [5, 65, 69, 219, 228],
Melting Point: [130].
90
Table 122. Thallium nitrate Table 124. Chromium trioxide
Eq wt 266.40 mp 207 °C (480 °K)
k = 0.906043 + 2.6094 lO^T
p = 5.8041  1.8737 • lO'T
A = 633.25 exp ( 3348.3/RT)
7i= 26.2068 + 0.2763047
7 7.00275 • \0 4 T*
+ 5.31820 • 107T3
T A KCl.
77 V
480
490
18.82
20.31
0.3465
.3726
4.905
4.885
500 21.82 .3987 4.867 3.35
510 23.34 .4248 4.849 3.11
520 24.87 .4508 4.830 2.90
530 26.41 .4769 4.811 2.70
540 27.96 .5030 4.792 2.54
550 29.53 .5291 4.773 2.41
560 31.11 .5552 4.755
mp 196 °C (469 °K)
k = 0.1952 + 0.4032 • 10~ 3r 0.0391 • IQT2
T K
510 0.00026
520 .00389
530 .00751
540 .01113
Conductance:[681 .
Melting Point: [133].
Density: [25, 191, 224].
Conductance: [110, 125c, 191, 215, 216, 217, 219, 224],
Viscosity: [110, 191, 219, 228],
Melting Point: [130].
Table 123. Vanadium pentoxide
mp 670 °C (943 °K)
k =  2.056 + 1.890 10 3T
T K
1140 0.0%
1150  1 Is
1160 .13e
1170 •15.5
1180 .174
1190 .19.3
1200 •21 2
1210 .23,
1220 •25o
1230 .26,
1240 .28s
Table 125. Molybdenum trioxide
mp 795 °C (1068 °K)
k= 11.642 exp (—5586/RT)
T K
1080 0.862
1090 .883
1100 .904
1110 .925
1120 .946
1130 .967
1140 .989
1150 1.010
1160 1.032
1170 1.053
1180 1.075
Conductance: [68], Conductance: [76, 68].
Melting Point: [130]. Melting Point: [130],
297268 068—791
Table 126. JFilstite (Feo.usO) Table 127. Boron oxide
mp 1368 °C (1641 °K)
k = 31771.7 + 36.3092 T 0.0102617 P (16481700 °K)
k= 171.25 + 0.27981 T ( 17101773 °K)
T K
1650 201
1660 225
1670 246
1680 265
1690 283
1700 298
1710 307
1720 310
1730 313
1740 316
1750 318
1760 321
1770 324
Conductance: [159].
Melting Point: [130],
Eq wt 23.21 mp 450 °C (723 °K)
P = 1.822163.45772 • 10 4T+ 8.71571 • 10~ 8P7}— 97913.6  135.257 T + 6.32685 • 10~ 2P
 9.97755 • 10 6P
T P V
1410 1.508 5020
1430 1.506 4700
1450 1.504 4400
1470 1.502 4110
1490 1.500 3840
1510 1.499 3580
1530 1.497 3340
1550 1.496 3110
1570 1.494 2900
1590 1.493 2700
1610 1.491 2510
1630 1.490 2330
1650 1.489 2170
1670 1.488 2010
1690 1.487 1870
1710 1.486 1740
1730 1.485 1610
1750 1.484 1500
1770 1.483 1400
1790 1.482 1300
1810 1.482 1210
1830 1.481 1130
1850 1.481 1050
1870 1.480 981
1890 1.480 918
Density: [144, 201].
Viscosity: [137, 144, 145, 200, 201, 209, 222],
Melting Point: [133].
92
Table 128. Silicon dioxide Table 129. Germanium dioxide
Eq wt 15.02 mp 1723 °C (1996 °K)
r) = 2.52255 • 10 8  294897 T + 114.935 T1
 1.49316 • 10 2 T3
T V T 17
2210 717,000 2390 127,000
2220 663,000 2400 114,000
2230 610,000 2410 102,000
2240 561,000 2420 91,900
2250 515,000 2430 83,400
2260 472,000 2440 75,400
2270 432,000 2450 69,000
2280 394,000 2460 63,700
2290 359,000 2470 59,100
2300 325,000 2480 55,100
2310 295,000 2490 52,300
2320 267,000 2500 50,200
2330 241,000 2510 48,900
2340 217,000 2520 47,700
2350 195,000 2530 46,900
2360 176,000 2540 46,500
2370 158,000 2550 46,400
2380 141,000
Viscosity:[205 . 206].
Melting Point: [133].
Eq wt 26.15 mp 1116 °C (1389 °K)
k = 29.758 exp (37957/RT)
77=1.316 • 10“ 4 exp (74254//?T) (14301750 °K)
77= 1.967 10~ 3 exp (65143//?D (17601990 °K)
T k • 10 + 4r, • IO 3
1390 0.320
1420 .428
1450 .565 20,500
1480 .738 12,200
1510 .954 7,370
1540 1.220 4,550
1570 1.547 2,860
1600 1.943 1,830
1630 2.420. 1,190
1660 787
1690 528
1720 359
1750 247
1760 242
1790 177
1820 131
1850 97.7
1880 73.7
1910 56.0
1940 43.0
1970 33.2
1990 28.1
Conductance: [ 163 . 146].
Viscosity: [137 . 140 . 141, 146].
Melting Point: [133].
297268 068—8 93
Table 130. Lead oxide Table 132. Antimony sesquioxide
K
Eq wt 65.94
mp 886 °C (1159 °K)
= 1.750 • 10 5 exp (27629/RT)
T K
1170 1.2,
1180 1.33
1190 1.47
1200 I.62
1210 1.7»
1220 1.9«
1230 2.1 6
1240 2.36
1250 2.5«
1260 2.82
mp 655 °C (928 °K)
</< =  1.086+ 1.062 • 10 3T
T K
1110 0.093
1120 • 103
1130 • 114
1140 •12s
1150 •13s
1160 • 146
Conductance: [681 .
Melting Point: [130],
Conductance:[681 .
Melting Point: [130].
Table 131. Arsenic trioxide Table 133. Bismuth sesquioxide
mp 312.3 °C (585.5 °K) mp 817 °C (1090 °K)
17= 1.679 • 102 exp (22,21 l/RT)
T V
610 1,550,000
620 1,150,000
630 841,000
640 617,000
650 460,000
660 354,000
670 285,000
680 236,000
690 195,000
700 145,000
Viscosity: [2021 .
Melting Point: [133],
k =  11.668+ 10.764 • 10 3T
T K
1100 0.1 7
1110 •2»
1120
1130 •50
1140 .60
1150 .7,
1160 .82
1170 •93
1180 1.03
1190 1.14
1200 1.25
1210 1.3«
Conductance:[681 .
Melting Point: [130].
94
Table 134. Tellurium dioxide Table 136. Cobalt (II) sulfide
mp 733 °C (1006 °K) Eq wt 45.50 mp 1100 °C (1373 °K)
k= 1.454 • 10 2 exp (9656/RT) k = 6.2884 exp ( 15494/RT)
T K
1020 1.24
1030 1.30
1040 1.36
1050 1.42
1060 1.48
1070 1.55
1080 1.62
1090 1.68
1100 1.75
1110 1.82
1120 1.90
1130 1.97
1140 2.05
1150 2.12
1160 2.20
1170 2.28
1180 2.37
1190 2.45
1200 2.53
1210 2.62
1220 2.71
1230 .2.80
Conductance: [681 .
Melting Point: [133].
Table 135. Iron (II) sulfide
Eqwt 43.96 mp 1195 °C (1468 °K)
k= 24462.0 30.289 T+ 9.9715 • 10 3T2
T K
1460 1495
1470 1485
1480 1476
1490 1469
1500 1464
T K
1460 1312
1470 1265
1480 1221
1490 1178
1500 1138
Conductance: [155 ],
Melting Point: [130].
Table 137. Nickel (II) sulfide
Eq wt 48.38 mp 797 °C (1070 °K)
k= 19337.0 20.810 T+ 6.000 • 10" 3 T1
T K
1150 3340
1160 3271
1170 3203
1180 3136
1190 3070
1200 3005
1210 2941
1220 2879
1230 2818
1240 2758
1250 2699
1260 2642
1270 2586
1280 2531
1300 2424
1320 2322
1340 2225
1360 2134
1380 2045
1400 1963
Conductance: [153, L54, 155]. Conductance: [ 154 ],
Melting Point: [132]. Melting Point: [130].
95
Table 138. Copper (I) sulfide Table 139. Silver sulfide
Eq wt 47.81 mp 1127 °C (1400 °K)
k= 1923.062.8871 T+ 1.1055 • 10' 3 T2
' T K
1400 47.94
1410 50.13
1420 52.55
1430 55.19
1440 58.04
1450 61.12
1460 64.42
1470 67.94
1480 71.69
1490 75.65
1500 79.83
1510 84.24
1520 88.86
1530 93.71
Conductance:[155 , 152].
Melting Point: [130],
Eq wt 123.91 mp 825 °C (1098 °K)
k = 41.5109 exp (2569.13//?r)
T K
1120 131.7
1140 129.0
1160 126.5
1180 124.2
1200 121.9
1220 119.8
1240 117.8
1260 115.8
1280 114.0
1300 112.2
1320 110.6
1340 108.9
1360 107.4
Conductance: [156 , 166].
Melting Point: [166],
Table 140. Germanium (II) sulfide
Eq wt 52.33 mp 625 °C (898 °K)
k= 0.616343 1.56399 • 10 3r+ 1.009032 • 10 6T 2
T K
870 0.01939
890 .02363
910 .02868
930 .03453
950 .04119
970 .04866
990 .05693
1010 .06601
1030 .07590
1050 .08660
1070 .09810
Conductance: [ 155 ].
Melting Point: [130],
96
Table 141. Tin (II) sulfide Table 142. Lead sulfide
Eq wt 150.77 mp 880 °C (1153 °K)' Eq wt 119.64 mp 1114 °C (1387 °K)
k = 12.9486.28321 • 1027+7 81646 • 10 5 r 2 k= 1815.4 2.26067+ 7.4254 • 10 4T 2
p = 5. 1 1 1—6.83 • lOT p= 7.260 5.400 • io_4r
A = 25730 exp ( 13618/flT) A = 338.66 exp (4867.0/K71
)
T A K P T A K P
1160 675 19.35 (4.319) 1390 1982 107.8 6.509
1170 718 20.54 4.312 1400 1949 105.9 6.504
1180 762 21.75 4.305 1410 1918 104.2 6.499
1190 806 22.97 4.298 1420 1891 102.6 6.493
1200 851 24.21 4.291 1430 1866 101.2 6.488
1210 896 25.47 4.285 1440 1843 99.87 6.482
1220 942 26.74 4.278 1450 1824 98.72 6.477
1230 989 28.02 4.271 1460 1807 97.72 6.472
1240 1037 29.33 4.264 1470 1792 96.87 6.466
1250 1085 30.64 4.257 1480 1781 96.17 6.461
1260 1134 31.98 4.250 1490 1772 95.62 6.455
1270 1184 33.33 4.244
1280 1235 34.69 4.237
1290 1286 36.07 4.230 Density: [150].
1300 1338 37.47 4.223 Conductance: [151, 154, 155].
1320 1444 40.31 4.209 Melting Point: [132],
1340 1553 43.21 4.196
1360 1665 46.17 (4.182)
1380 1780 49.20 (4.168)
1400 1897 52.29 (4.155)
1420 2019 55.44 (4.141)
Density: [ 158 ]
.
Conductance: [155].
Melting Point: [130],
97
TABLE 143. Antimony (III) sulfide Table 144. Bismuth (III) sulfide
Eqwt 113.25 mp 547 °C (820 °K)
k = 4.0712 1.12847 • 10~ 2 T+ 7.9857 • 10"6 T 2
p = 4.3876.5 • 10~ 4 TA = 14940 exp ( 12846/flT)
T A K P
830 6.07 0.206 3.847
840 6.69 .227 3.841
850 7.35 .249 3.834
860 8.06 .273 3.828
870 8.83 .298 3.821
880 9.64 .325 3.815
890 10.51 .353 3.808
900 11.42 .383 3.802
910 12.39 .415 3.795
920 13.40 .448 3.789
930 14.47 .483 3.782
940 15.59 .520 3.776
950 16.76 .558 3.769
960 17.98 .598 3.763
970 19.26 .639 3.756
980 20.59 .682 3.750
1000 23.40 .772 3.737
1020 26.43 .869 3.724
1040 29.67 .972 3.711
1060 33.14 1.082 3.698
1080 36.83 1.198 3.685
Density: [158],
Conductance: [ 155 ].
Melting Point: [130],
Eq wt 171.40 mp 747 °C (1020 °K)
k = 3955.2 0.598558 T
p = 7.237 9.72 • 10~4 TA = 89320 exp (55.18/RT)
T A K P
970 91893 3374 (6.294)
980 9187 2 3369 (6.284)
990 9185, 3363 (6.275)
1000 91829 3357 6.265
1010 9180« 3351 6.255
1020 9178 7 3345 6.246
1030 9176s 3338 6.236
1040 91744 3333 6.226
1050 9172 2 3327 6.216
1060 9170, 3321 6.207
1070 9167y 3315 6.197
1080 9165 7 3309 6.187
1090 9163s 3303 6.177
1100 9161a 3297 6.168
1110 9159, 3291 6.158
1120 9156y 3285 6.148
1130 91547 3279 6.139
1140 9152s 3273 6.129
1150 91503 3267 6.119
1160 91480 3261 (6.109)
1170 91 458 3255 (6.100)
1180 9143s 3249 (6.090)
1190 9141 3 3243 (6.080)
1200 91390 3237 (6.071)
Density: [ 158 ],
Conductance: [157],
Melting Point: [132],
98
Table 145. Lithium sulfate Table 147. Potassium sulfate
Eqwt 54.97 mp 859 °C (1132 °K)
k =  24.544 + 4.4630 10 2T 1.7251 • lO"5 T 2
p = 2.464 0.000407 TA = 394.8 exp (2932/RT)
T A K P
1140 107.5 3.915 2.000
1150 109.1 3.966 1.996
1160 110.6 4.014 1.992
1170 112.1 4.058 1.987
1180 113.5 4.099 1.984
1190 114.7 4.136 1.980
1200 115.9 4.170 1.976
1210 117.0 4.201 1.972
1220 118.0 4.228 1.967
1230 118.9 4.252 1.964
1240 119.7 4.272 1.959
1250 120.4 4.289 1.955
Density: [25]
.
Conductance: [ 115 ]
.
Melting Point: [130],
Table 146. Sodium sulfate
Eqwt 71.03 mp 889 °C (1157 °K)
k= 11.893 exp (— 3819.9/RT)
p = 2.628 4.83 • 10~4rA = 550. 19 exp (4507.0/RT)
T A K P
1180 80.48 2.332 2.058
1190 81.79 2.364 2.053
1200 83.09 2.396 2.048
1210 84.40 2.428 2.044
1220 85.71 2.460 2.039
1230 87.02 2.492 2.034
1240 88.34 2.523 2.029
1250 2.440
1300 2.576
1350 2.712
Eq wt 137.13 mp 1069 °C (1342 °K)
* =— 23.5770 + 3.57269 • Kh 2 T 1.24807 • 10~ 5 T 2
p = 2.4697 4.473 • 10~4 TA = 814.95 exp (4721.6/RT)
T A K P
1350 140.2 1.908 1.866
1360 142.0 1.927 1.861
1370 1.857
1380 1.853
1390 1.848
1400 1.843
1410 1.839
Density: [25, 178 ],
Conductance: [4, 161].
Melting Point: [130].
Table 148. Rubidium sulfate
Eq wt 133.52 mp 1074 °C (1347 °K)
k= 6.2394 exp (3977.2/RT)
p = 3.442 6.65 • 10~ 4rA = 471.72 exp (4956.6/RT)
T A K P
1340 73.33 1.401 2.551
1350 74.34 1.416 2.544
1360 75.35 1.432 2.538
1370 76.36 1.447 2.531
1380 77.38 1.463 2.524
1390 78.40 1.478 2.518
1400 79.42 1.493 2.511
1450 2.478
1500 2.445
1550 2.411
1600 2.378
1650 2.345
1700 2.312
1750 2.278
1800 2.245
Density: [25]
.
Conductance: [4,226].
Melting Point: [131].
99
Density: [25]
.
Conductance: [226 ]
.
Melting Point: [130],
Table 149a. Cesium sulfate Table 149b. Silver sulfate
Eq wt 180.95 mp 1019 °C (1292 °K)
k = 0.46852+ 1.2287 • 10 3r
p = 3. 116 + 5.86 • 104r4.94 • lO’T 2
A = 387.47 exp (  4528.7//?T)
T A K P
1300 67.12 1.129 3.043
1310 68.01 1.141 3.036
1320 68.90 1.153 3.029
1330 69.80 1.166 3.021
1340 70.71 1.178 3.014
1350 71.63 1.190 3.007
1360 72.55 1.202 2.999
1400 2.968
1450 2.927
1500 2.884
1550 2.837
1600 2.789
1650 2.738
1700 2.685
1750 2.629
Density: [25]
.
Conductance: [226 ]
.
Melting Point: [130],
Table 150. Tetrapropylammonium tetrafluoroborate
Eq wt 273.17 mp 248 °C (521 °K)
k = 6.673 1 exp (4472.7//J71
)
p= 1.24676.415 • 10 4TA = 2973.9 exp (4884.8/R T)rj — 539.745 — 2.888737’+ 5.20040 • 103 T 2
3.13987 • 10 6T3
T A K P V
530 28.76 0.09546 0.9067 2.06
540 31.34 .10328 .9003 1.85
550 34.04 .11141 .8939
560 36.89 .11985 .8875
Density: [ 190 . 2211 .
Conductance: [ 190 , 221 ],
Viscosity: [ 190 , 2211 .
Melting Point: [ 190 ]
.
Eq wt 101.97 mp 660 °C (933 °K)
k = 7.4568 exp (2754.1/RT)
p = 5.843 1.089 • 103TA = 199.04 exp (3188.5/RT)
T A K P
940 36.11 1.707 4.819
950 36.76 1.733 4.808
960 37.41 1.760 4.798
970 38.06 1.786 4.787
980 38.70 1.813 4.776
990 39.35 1.839 4.765
1000 40.00 1.865 4.754
1010 40.64 1.890 4.743
1020 41.29 1.916 4.732
Density: [226].
Conductance: [226 ]
.
Melting Point: [130],
Table 151. Tetrapropylammonium hexafluorophosphate
Eq wt 331.30 mp 237.0 °C (510.2 °K)
k = 21.0096 exp (  5902.52//?7T
)
p= 1.24333.224 • lO^TA = 7610.3 exp ( — 6070.0//?D
17 = 900.654 — 4.87945
7
1+ 8.87944 • lO^T 2
5.41472 • 10 6T3
T A K P V
520 21.38 0.06941 1.0757 2.99
530 23.88 .07731 1.0724 2.65
540 26.58 .08577 1.0692 2.37
550 29.46 .09479 1.0660
Density: [ 190 , 2211 .
Conductance: [ 190 . 2211 .
Viscosity: [ 190 . 2211 .
Melting Point: [ 190 ]
.
100
Table 152. Tetrapropylammonium tetraphenylborate Table 154. Tetrabutylammonium iodide
Eq wt 505.57 mp 205.7 °C (478.9 °K)
p = 0.14613 + 3. 70736 • 10 3T 4.29706 • 10 6T 2
r) — 2348.89 — 12.944771+ 2.39385 • 10~ 2
:T2
1.48320 • lO 2 T3
T P V
490 0.9310 8.65
500 .9255 7.16
510 .9192 6.02
520 .9120 5.12
530 4.38
Density: [190 , 2211
Viscosity: [ 190 , 2211 .
Melting Point: [ 190 ]
.
Table 153. Tetrabutylammonium bromide
Eq wt 322.37 mp 1195 °C (392.7 °K)
k= 1926.41 exp (  10818A/RT)
p= 1.2877.039 • 10 4TA = 817140 exp ( 11041/tfT)
T A K P
400 0.7575 0.002362 1.0054
410 1.0631 .003293 0.9984
Density:[190 . 221] .
Conductance:[190 . 221] ,
Melting Point: [190].
Eq wt 369.37 mp 146.0 °C (419.2 °K)
k= — 6.48575 • 10 2 + 1.66797 • 10 4Tp= 1.446 8.388 10 4 TA = 136940 exp (9394.2/RT)
T A K P
420 1.755 0.005197 1.0937
430 2.336 .006865 1.0853
440 2.927 .008533 1.0769
Density: [190, 220, 221
1
.
Conductance: [ 190 , 220, 221 ]
.
Melting Point: [190].
Table 155. Tetrabutylammonium tetrafluoroborate
Eq wt 329.28 mp 162 °C (435 °K)
p= 1.19065.812.’. 104 T
p = 1099.50 — 6.25565 T+ 1.19468 • 10~ 2 T 2
7.64127 • 10« T 3
T P V
440 0.9349 9.00
450 .9291 7.37
460 .9232 6.07
470 .9174 5.05
480 .9116 4.27
490 .9058 3.67
500 .9000 3.22
510 .8942 2.86
520 .8884 2.55
530 .8826 2.25
540 .8768 1.91
Density: [ 190 , 221].
Viscosity: [ 190 , 221],
Melting Point: [190],
101
TABLE 156. Tetrabutylammonium hexafluorophosphate Table 158. Tetrahexylammonium tetrafluoroborate
Eq wt 387.43 mp 247 °C (520 °K)
k = 0.193219 + 4.43623 • 10~4 T
p = 1.3252 6.557 • 10~4 TA 4743.7 exp (5954.3ART)
i) = 3.173 • lO"3 exp (71591RT)
T A K P V
530 16.60 0.04190 0.9777 2.84
540 18.49 .04634 .9711 2.51
550 20.39 .05077 .9646 2.22
Density: [190, 221].
Conductance: [ 190 , 221 ]
.
Viscosity: [ 190 , 221 ]
.
Melting Point: [190],
Table 157. Tetrabutylammonium tetraphenylborate
Eq wt 561.68 mp 236.5 °C (509.7 °K)
k= 8.0270 exp (6587.0/RT)
p = 1.14354.945 • 10“4 TA 6841.1 exp ( 6893.0/RT)
rj 1.588 • 103 exp (8235/RT)
T A K P V
510 7.605 0.01207 0.8913
520 8.665 .01367 .8864 4.59
530 9.828 .01542 .8814 3.95
540 11.10 .01732 .8765 3.42
Density: [190, 221 1.
Conductance: [190, 221],
Viscosity: 1 190 . 2211 .
Melting Point: [190],
Eq wt 441.48 mp 91 °C (364 °K)
p= 1.12965.772 • 10~4 Trj 1.806 • 104 exp (9841/RT)
T P V
370 0.9161
380 .9103 82.61
390 .9045 59.14
400 .8987 43.06
410 .8930 31.83
420 .8872 23.88
430 .8814 18.15
440 .8757 13.97
450 .8699 10.88
460 .8641 8.56
470 .8583 6.81
480 .8526 5.47
490 .8468 4.43
500 .8410 3.62
Density: [190, 2211 .
Viscosity: 1 190 . 22 1] ,
Melting Point: [190].
Table 159. Tetranamylammonium thiocyanate
Eq wt 356.64 mp 50.5 °C (323.7 °K)
k 0.0621247 3.93243 • 10 4T+ 6.24733 • 107T 2
p= 1.07745.3662 • 104rA = 5. 7747 • 105 exp (9882.2/RT)
17= 116917 941.7747’+2.532767’2  2.27331 • 10 372
T A k 104 P V
330 0.1540 3.887 0.9003 253
340 .2558 6.420 .8950 151
350 .4090 10.20 .8896 91.1
360 .6145 15.24 .8842 60.6
370 .8731 21.51 .8789 45.4
380 1.1860 29.05 .8735 32.3
390 1.5540 37.83 .8681
Density: [ 172 ]
.
Conductance: [ 172 ].
Viscosity: [ 172 ],
Melting Point: [218].
102
TABLE 160. Lithium molybdate Table 161. Sodium molybdate
Eq wt 86.90 mp 705 °C (978 °K)
k = 4.531 + 7.740 • 103T 1.356 • lOT 2
T K
980 1.752
990 1.803
1000 1.853
1010 1.903
1020 1.953
1030 2.003
1040 2.052
1050 2.101
1060 2.150
1070 2.198
1080 2.247
1090 2.295
1100 2.342
1120 2.437
1140 2.530
1160 2.623
1180 2.714
1200 2.804
1220 2.893
Conductance: [ 117 ]
.
Melting Point: [130].
Eq wt 102.97 mp 687 °C (960 °K)
* = 3.1705 + 5.2419 • lO^T 0.8970 • 10<T 2
p = 3.407 0.629 • 10"3rA = 779.9 exp (5713/RT)
T A K P
1020 (46.3) 1.243 (2.765)
1030 (47.7) 1.277 (2.759)
1040 (49.0) 1.311 (2.753)
1050 (50.4) 1.345 (2.747)
1060 (51.8) 1.378 (2.740)
1070 (53.2) 1.411 (2.734)
1080 (54.5) 1.444 (2.728)
1090 (55.9) 1.477 (2.721)
1100 (57.3) 1.510 (2.715)
1110 (58.6) 1.543 (2.709)
1120 60.0 1575 2.703
1130 61.4 1.607 2.696
1140 62.8 1.640 2.690
1150 64.1 1.671 2.684
1160 65.5 1.703 2.677
1170 66.9 1.735 2.671
1180 68.2 1.767 2.665
1190 69.6 1.797 2.658
1200 71.0 1.828 2.652
1210 72.3 1.859 2.646
1220 73.7 1.890 2.640
1230 75.1 1.920 2.633
Density: [261 .
Conductance: [26, 761 .
Melting Point: [130],
103
TABLE 162. Potassium molybdate Table 163. Sodium tungstate
Eqwt 119.08 mp 926 °C (1199 °K) Eq wt 146.96 mp 698 °C (971 °K)
p = 2.8882. 83 • 104r1.28 • 10“T 2 k = 7.541 exp (3931/RT)
====^=^==== p= 4.629 0.797 • 10 3TA = 381.7 exp (4491/RT)
T A K P
1250 2.334
1300 2.304
1350 2.273 1050 44.4 1.14s 3.792
1400 2.241 1060 45.3 1.16s 3.784
1450 2.209 1070 46.2 1.18s 3.776
1500 2.176 1080 47.1 1.20s 3.768
1550 2.142 1090 48.0 1.23 3.760
1600 2.108 1100 48.9 1.25 3.752
1650 2.073 1110 49.8 1.27 3.744
1700 2.037 1120 50.7 1.29 3.736
1750 2.001 1130 51.6 1.31 3.728
1140 52.5 1.33 3.720
1150 53.4 1.35 3.712
Density: [25].' 1160 54.4 1.37 3.704
Melting Point: [130]. 1170 55.3 1.39 3.697
1180 56.2 1.41 3.689
1190 57.1 1.43 3.681
1200 58.0 1.45 3.673
1210 59.0 1.47 3.665
1220 59.9 1.49 3.657
1230 60.8 1.51 3.649
1240 61.7 1.53 3.641
TABLE 164. Potassium tungstate
Eq wt 163.07 mp 930 °C (1203 °K) Density: [26],
Conductance: [26]
.
p = 4.419— 1.233 • 103T+ 1.62 • 1QT 2Melting Point: [131],
T P
1250 3.131
t 1300 3.090
1350 3.050
1400 3.010
1450 2.972
1500 2.934
1550 2.897
1600 2.861
1650 2.826
1700 2.791
1750 2.757
Density: [25]
.
Melting Point: [130],
104
Table 165. Sodium thiocyanate Table 167. Sodium hydroxide
Eq wt 81.08 mp 310 °C (583 °K) Eq wt 40.01 mp 318 °C (591 °K)
k = 43.0 exp ( — 4740//? T)
t] = 526.399 — 2.49292 T+ 3.96856 • 10“3 T 2
2.11546 • 106 T3
T K V
590 0.754 2.56
600 .807 2.39
610 .861 2.25
620 .917 2.13
630 .974 2.02
640 1.035
650 1.096
Conductance:[1121 .
Viscosity: [ 1 12] .
Melting Point: [112],
Table 166. Potassium thiocyanate
Eq wt 97.18 mp 172 °C (455 °K)
k= 100 exp (— 58501RT)
p = 1.9581 0.800 103TA = 7874 exp ( 6082/RT)
rj= 1935.08 11.1776 T+ 2.16788 • 10" 2 T 2
 1.40826 • 105r3
T A K P V
450 8.8 0.144 1.5981 11.8
460 10.2 .166 1.5901 9.87
470 11.7 .190 1.5821 8.36
480 (13.4) .217 (1.5741) 7.20
490 (15.3) .246 (1.5661) 6.33
500 (17.3) .277 (1.5581) 5.65
510
520
(19.5) .311 (1.5501) 5.09
4.55
k = 3. 23 + 9.0 • 103T
p = 2.068 0.4784 • lO^T1
A = 668.2 exp (3120/RT)
7}= 164.771 — 0.61483371+ 7.80340 • 10 4 T 2
3.33334 • 10~ 7T3
T A K P V
600 (48.7) 2.17 (1.781)
610 (50.9) 2.26 (1.776)
620 53.1 2.35 1.771
630 55.3 2.44 1.767 3.79
640 57.5 2.53 1.762 3.52
650 59.7 2.62 1.757 3.28
660 61.9 2.71 1.752 3.07
670 64.1 2.80 1.747 2.87
680 66.4 2.89 1.743 2.70
690 68.6 2.98 1.738 2.55
700 70.9 3.07 1.733 2.42
710 73.2 3.16 1.728 2.31
720 75.4 3.25 1.724 2.20
730 77.7 3.34 1.719 2.11
740 2.03
750 1.96
760 1.90
770 1.84
780 1.78
790 1.72
800 1.66
810 1.59
820 1.52
Density: [37].
Conductance: [37].
Viscosity: [37]
.
Melting Point: [131].
Density:[110] .
Conductance: [112] ,
Viscosity:[112 ],
Melting Point: [131].
105
TABLE 168. Potassium hydroxide TABLE 169. Potassium dichromate
Eq wt 56.10 mp 360 °C (633 °K)
k =  1.38 + 5.80 • 103T
p = 2.013 0.4396 • 10"3rA = 520.2 exp (2467/RT)
r) = 52.7561  0. 166134T+ 1.80314 • 10~4r2
6.66494 10~ 8T3
T A K P V
640 1.732
650 1.727
660 1.723
670 81.8 2.51 1.718
680 83.9 2.56 1.714 2.21
690 86.o 2.62 1.710 2.08
700 88.2 2.68 1.705 1.96
710 90.3 2.74 1.701 1.84
720 92.5 2.80 1.696 1.74
730 94. 6 2.85 1.692 1.64
740 96.8 2.91 1.688 1.55
750 99.o 2.97 1.683 1.46
760 101.2 3.03 1.679 1.39
770 103.4 3.09 1.675 1.31
780 105.6 3.14 1.670 1.25
790 107.8 3.20 1.666 1.18
800 110.! 3.26 1.661 1.13
810 112.3 3.32 1.657 1.07
820 114.6 3.38 1.653 1.02
830 116.9 3.43 1.648 0.97
840 119.2 3.49 1.644 .93
850 121.5 3.55 1.639 .89
860 123.8 3.61 1.635 .85
870 126.! 3.67 1.631 .81
Eq wt 147.11 mp 398 °C (671 °K)
k = 73.0 exp (7800/PT)
p = 2.753 0.695. 103TA = 6052 exp (8141/RT)
tj = 79.56670.1106007 1.12662 • 10~ 5T2
+ 4.25741 • 10«7 3
T A K P V
690 16.o 0.24 7 2.273 11.87
700 17.4 •268 2.267 11.23
710 18.9 •290 2.260 10.60
720 20.4 •31s 2.253 9.99
730 22., .33 7 2.246 9.39
740 23.8 •363 2.239 8.81
750 25. 7 .38 a 2.232 8.24
760 27. 6 .41 7 2.225 7.69
770 29. 6 .446 2.218 7.16
780 31. 7 476 2.211 6.65
790 33.9 ,50 7 2.204
800 36., •54o 2.197
Density: [25, 110].
Conductance: [8, 110 ].
Viscosity: [8, 110].
Melting Point: [130].
Density: [37].
Conductance:[37] ,
Viscosity:[371 .
Melting Point: [132],
106
Table 170. Sodium metaphosphate Table 172. Lithium hydride
Eq wt 101.98 mp 625 °C (898 °K)
rj = 2.412 • 10 2 exp (19899/RT)
T i?
920 1290
930 1150
940 1020
950 913
960 818
970 735
980 661
990 597
1000 539
1010 488
1020 443
Viscosity: [200 ]
.
Melting Point: [130].
TABLE 171. Uranyl chloride
Eq wt 170.49 mp 588 °C (851 °K)
* =— 0.273 + 0.371 • 103r
T *
860 0.046
870 .050
880 .053
890 .057
900 .061
910 .065
920 .068
930 .072
940 .076
950 .079
960 .083
Eq wt 7.948 mp 688 °C (961 °K)
* = 37.47097.75006 • 10 2T+ 4.01 118 • 106T 2
T *
970 0.0366
980 .0438
990 .0590
1000 .0822
1010 .1134
1020 .1527
1030 .2000
Conductance: [ 165 ]
.
Melting Point: [211],
Table 173. Lithium chlorate
Eq wt 90.39 mp 127.8 °C (401.0 °K)
* = 0.95475 + 2.6390 10 3T
p = 2.3936 7.5702 • 10“ 4rA = 9394.7 exp (6072.1/RT)
17=13199.688.4573 T+ 0.198361 T2  1.48684 10_4r 3
T A * P V
410 5.52 0.1272 2.0832 29.14
420 6.69 .1536 2.0756 22.72
430 7.87 .1800 2.0681 18.49
440 9.05 .2064 2.0605 15.58
450 10.25 .2328 2.0529
Density: [164, 175 ].
Conductance: [164, 174].
Viscosity: 1 1751 .
Melting Point: [174].
Conductance: [64].
Melting Point: [64].
107
TABLE 174. Lithium perchlorate
Eq wt 106.40 mp 236 °C (509 °K)
p = 2.337 0.612 • 10 37
T P
530 2.013
540 2.007
550 2.000
560 1.994
570 1.988
580 1.982
590 1.976
600 1.970
610 1.964
620 1.958
630 1.951
640 1.945
650 1.939
Density:[ 177] ,
Melting Point: [130].
7. Cumulative Tables of Temperature Dependent Equations
The best temperature dependent equations for
specific conductance, density, equivalent conduct
ance and viscosity (tables 1—174) are summarizedin tables 175178 respectively. Tables 179182
contain sets of exponential and power series
equations for specific conductance and viscosity.
The precisions marked with asterisks (*) in table
179 are approximate; the values in these instances
may be 2 to 5 times larger than the table entries. Theuncertainties in brackets, being based on minimalinformation, are more qualitative than the un
bracketed values.
108
Table
175.
Specific
conductance
—
Best
equations
297268 068—9 109
Table
175.
Specific
conductance
—
Best
equations
—
Continued
110
Table
175.
Specific
conductance
—
Best
equations
—
Continued
111
Table
175.
Specific
conductance
—
Best
equations
—
Continued
112
Table
175.
Specific
conductance
—
Best
equations
—
Continued
113
Table 176. Density— Best equations
Salt
p — a — bT
Temperature range °K Reference
Uncertainty
estimate
(percent)a b • 103
LiF 2.3581 0.4902 11491320 [83] 0.5
NaF 2 655 .54 12831819 [25]
KF 2.6464 .6515 11541310 [83] .6
CsF 4.8985 1.2806 9851185 [83] .8
MgF2 3.235 0.524 16502100 [95]
CaF> 3 179 391 16402300 [951
SrF., 4 784 751 17502200 [951
RaF. 5 775 999 16002000 [951
1 aFq 5 793 682 17502450 [95]juai 3
CpF, 6 253 936 17002200 [951
ThF4 7.108 .7590 13931651 [167] (1)
uf4 7.784 .9920 13091614 [167] (1)
LiCl 1.8842 .4328 8941054 [79] 0.2
NaCl 2.1393 .5430 10761301 [79] .4
KC1 2.1359 .5831 10531212 [79] .5
RbCl 3.1210 .8832 9961196 [82] .4
CsCl 3.7692 1.065 9451179 [82] .1
Red., 2 276 1 10 706746 [361
MgCl 2 1.976 0.302 10211159 [113] .2
CaCl2 2.5261 .4225 10601223 [83] .9
SrCl 2 3.3896 .5781 11671310 [83] .7
BaCl 2 4.0152 .6813 12391354 [83] 5.0
yci3 3.007 .50 9981118 [36]
LaCl3 4.0895 .7774 11461246 [83] 0.6
CeCl 3 4.248 .920 11231223 [99]
MnCl 2 2.75701 .43766 9231123 [192]
CuCl 4.226 .76 709858 [36]
AgCl 5.505 .87 7591073 [166] 0.1
ZnCl2 2.7831 .448 593673 [98] .2
CdCl 2 4.078 .82 8401080 [54, 66] .3
HgCl 9.0928 4.0 799850 [36]
HgCl 2 5.9391 2.8624 550577 [103] .5
AlCls Quadratic equation* 480.1623.2 [149]
GaCl 3 2.7841 2.0826 360414 [148] .4
InCl 4.43 7 1.40 542638 [34]
InCl2 3.86a 1.60 541710 [34]
InCl3 3.944 2.10 870939 [34]
T1C1 6.893 1.80 708915 [36]
SnCl2 4.016 1.253 580753 [25] 1.3
SnCl4 3.0185 2.687 309.4411.2 [147] (0.8)
PbCl2 6.112 1.50 789983 [54] .3
BiCl3 5.073 2.30 523623 [32] .4
LiBr 3.0658 0.6520 8251012 [82]
NaBr 3.1748 .8169 10271218 [82] 1.0
KBr 2.9583 .8253 10141203 [82] 0.4
RbBr 3.7390 1.0718 9771180 [82] .4
CsBr 4.2449 1.2234 9101133 [82] .5
MgBr2 3.087 0.478 10401208 [113]
CaBr2 3.618 .500 10361064 [113]
114
Table 176. Density— Best equations — Continued
Salt
p = a — bT
Temperature range °K Reference
Uncertainty
estimate
(percent)a b 103
4.390 0.745 9501277 [1131
BaBr2 5.035 .924 11231173 [66]
LaBr3 5.0351 .096 10691185 [83]
NdBr3 4.9750 .7779 968 1133 [83]
AgBr 6.307 1.035 720 940 [22, 54] 0.08
ZnBr2 4.113 0.959 707 875 [113] 2.0
CdBr2 4.9831 1.08 853 993 [54]
HgBr2 6.7715 3.2331 511 592 [103] 0.1
InBr3 4.184 1.50 721 801 [34]
TIBr 7.4335 1.922 766 1023 [196]
PbBr2 6.789 1.65 778 873 [54] .8
BiBr3 5.958 2.6 525 715 [25]
Lil 3.7902 0.9176 748 940 [82]
Nal 3.6274 .9491 945 1185 [82] .4
KI 3.3594 .9557 955 1177 [79] .25
Rbl 3.9499 1.1435 928 1175 [82] .7
Csl 4.2410 1.1834 919 1126 [82] .4
Mgl 2 3.642 0.651 965 1161 [113]
Cal 2 4.233 .751 1059 1301 [113]
Srl2 4.803 .885 789 1299 [113]
Bal 2 5.222 .977 1043 1248 [113]
A1I3 4.383 2.50 473 513 [35]
Agl 6.415 1.01 870 1075 [22]
Znl2 4.856 1.360 729 861 [113]
Cdl 2 5.133 1.117 673 973 [66]
Hgl 2 6.9435 3.2351 532 627 [103] .1
Gal2 4.841 1.688 454 538 [105]
Inl 3 4.5448 1.50 503 633 [34]
Li2C0 3 2.2026 0.3729 1012 1115 [101] .2
Na2C0 3 2.4797 .4487 1138 1277 [101] .2
K2C03 2.4141 .4421 1181 1283 [101] .2
NaN0 2 2.226 .746 553  723 [66] 1.0
kno 2 2.167 .66 713  733 [173]
Ba(N0 2 )2 3.639 .70 573  613 [173]
LiN03 2.068 .546 545  714 [26]
NaN03 2.320 .715 583  643 [61, 66] 1.0
kno3 2.315 .729 620  880 [66] 0.2
RbN03 3.049 .972 592  766 [26]
CsN03 3.6206 1.1660s 688  764 [84] .15
AgN03 4.454 1.02 553  683 [25] .3
tino3 5.8041 1.8737 484.4 552.6 [191] .15
b 203 Quadratic equation* 723 1673 [201] .8
b 2o3 Quadratic equation* 1410 1890 [144] .8
SnS 5.111 0.683 1193 1324 [158]
PbS 7.260 .5400 1393 1473 [150]
Sb 2S3 4.387 .65 826 1091 [158]
Bi 2S3 7.237 .972 1016 1136 [158]
Li 2S04 2.464 .407 1133 1487 [25] (1)
Na2S0 4 2.628 .483 1173 1350 [25] (1)
115
Table 176. Density— Best equations— Continued
Salt
p = a — bT
Temperature range °K Reference
Uncertainty
estimate
(percent)a b 103
k2so 4 2.4697 0.4473 1348 1411 [178] 0.4
Rb 2S0 4 3.442 .665 1359 1818 [25] (1)
Cs 2S0 4 Quadratic equation* 1309 1803 [25] (1)
Ag2S04 5.843 1.089 953 1043 [226] (0.8)
Pr4NBF 4 1.2467 0.6415 525.6 547.3 [190, 221] (1)
Pr4NPF h 1.2433 .3224 513  545 [190, 221] (1)
Pr4NBPh4 Quadratic equation* 482  512 [190, 221] (1)
Bu 4NBr 1.287 0.7039 392  408 [190, 221] (1)
Bu 4NI 1.446 .8388 420  435 [190, 221] (1)
Bu4NBF4 1.1906 .5812 436  539 [190, 221] (1)
Bu4NPF6 1.3252 .6557 529  548 [190, 221] (1)
Bu 4NBPh4 1.1435 .4945 514.3 540.4 [190, 221] (1)
Hex4NBF4 1.1296 .5772 375  491 [190, 221] (1)
(nAmyl)4NSCN 1.0744 .53662 325.2 383.2 [172]
Na>Mo0 4 3.407 .629 116 1681 [261
K2Mo04 Quadratic equation* 1203 1795 [25]
Na>W0 4 4 629 O 797 1025 1774 [261
k2wo4 Quadratic equation* 1198 1794 [25]
K2Cr,0 7 2.753 0.695 693  808 [25]
KSCN 1.9581 .800 447  [HO]
NaOH 2.068 .4784 623  723 [37]
KOH 2.013 .4396 673  873 [37]
LiCIO;, 2.3936 .75702 406.3 426.6 [175]
FiC10 4 2.337 .612 534  644 [177]
*Quadratic Equations: p = a + bT+ cT 2
a b • 103 c • 106 Temperature range °K Reference
Uncertainty
estimate
(percent)
AlCU 5.711383 28.59744 0.2953960 480.1 623.2 [149]
b 2o3 2.03833 0.667971 .208005 723 1673 [201] 0.8
b 2o3 1.82216  .345772 .0871571 1410 1890 [144] .8
Cs 2S04 3.116 .586 .494 1309.21803.2 [25] (1)
Pr4NBPh4 0.14613 3.70736  4.29706 482  512 [190, 221] (1)
K2Mo04 2.888 0.283 0.128 1203.81795.5 [25]
k2wo 4 4.419 1.233 .162 1198.21793.5 [25]
116
TABLE 177. Equivalent conductance
A = A\e~E\IRT (ohm 1cm 2equiv 1)
Salt /4A(ohm 1cm2equip '1) fiscal moR 1
)s(ohm _1cm 2
equiv 1)
s%
LiF 320.71 2143.3 0.303 0.23
NaF 344.7 2964. .1187 .10
KF 480.27 3354.9 .188 .16
CsF 817.76 4068.2 .118 .97
LiCl 508.2 2015 .0847 .048
NaCl 544.6 2990 .0870 .057
KC1 548.0 3415.2 .109 .092
RbCl 754.1 4401 .192 .19
CsCl 1102 5110 .25 .26
BeCl2 5.3567 • 10 13 50479 .0169 21.6
MgCl2 263.7 4363 .105 0.28
CaCl2 675.3 5285 .0344 .046
SrCl2 689.6 5646 .0247 .036
BaCl2 772.5 6004 .0195 .025
YC13 959.2 8827 .276 1.8
LaCl3 469.4 5678 .277 0.63
CaCl3 460.7 6078.0 .188 .58
ThCl4 395.0 6764 .273 1.2
MnCl2 169.53 2694.3 .265 .59
CuCl 153.6 650.4 .968 .84
AgCl 268.22 1252.3 .279 0.21
ZnCl2 5.3419 • 10 7 24343 .040 18
(593672 °K)
ZnCl2 48591 15153 .062 3.3
(672825 °K)
ZnCl2 6096.5 11785 .080 0.94
(825970 °K)
CdCl2 224.4 2499 .0200 .035
HgCl 353.5 3469 .00732 .017
HgCl2 0.1775 5626.7 8.5 • 10 5 4.2
InCl 1208 3528 0.205 0.39
InCl2 288.4 3687 .389 2.37
InCl3 4.112 2181 .0580 0.426
T1C1 546.0 3421.0 .363 .43
SnCl2 361.8 2726.9 4.95 7.4
PbCl2 588.1 4093 0.301 0.53
BiCl3 32.36 981.3 1.58 9.6
LiBr 585.3 2117 0.32* 0.17
NaBr 622.7 3228 .179 .12
KBr 591.1 3747 .578 .53
RbBr 611.1 4171 .800 .91
CsBr 1169 5533 .317 .42
MgBr2 385.5 5404 .101 .29
CaBr2 506.7 4901 .053 .087
SrBr2 806.5 6183 .44 1.0
BaBr2 691.8 6153 .0390 0.068
LaBr3 2652 10296 .0874 .32
NdBr3 3973 11749 .101 .67
AgBr 210.2 1104 .108 1.0
117
Table 177. Equivalent conductance— Continued
A = A\e~E \lRT (ohm _1cm 2equiv_1)
Salt A \(ohm _1cm2equiv _1) £A(cal mol *) s(ohm_1cm 2
equiv1)
s%
ZnBr2 35684 14604 0.325 21.0
CdBr2 243.4 3226 .0263 0.06
HgBr2 0.31052 4065.3 8.6 • 104 7.0
InBr3 6.766 91.0 0.0259 .38
TIBr 425.8 3510.8 .0982 .16
PbBr 2 660.8 4559 .265 1.0
BiBr3 16.67 535.6 1.30 10
Lil 569.5 1809.9 0.0659 0.04
Nal 694.5 3221 .0127 .0085
KI 541.2 3442 .758 .68
Rbl 568.1 3999 .378 .45
Csl 1125 5450 .378 .48
Mgl2 751.1 6752 .081* .29
Cal 2 440.3 4617 .421 .69
Srl 2 610.1 5409 .57* 1.3
Bal2 831.2 6367 .25* 0.50
AII3 118670 11160 .121 7.2
Agl 239.9 1475 .122 0.10
Znl 2 17880 12636 .222 3.3
Cdl2 1109.0 6365 .448* 2.2
Hgl 2 0.07345 3114.3 .0313 3.3
Gal 2 771.8 5121 .453 7.7
Inl3 18.26 1779.9 .233 4.6
Li 2C03 754.5 4438 .140 0.15
Na2C03 550.2 4199 .035 .040
k2co3 544.6 4650 .0175 .021
NaN0 2 685.7 2949 .108 .15
kno 2 776.99 3267.2 .0617 .075
Ba(N0 2 )2 10217 8103.9 .0601 .80
LiN03 967.8 3589 .0515 .095
NaN03 705.6 3215 .0160 .028
KNO3 657.4 3577 .0832 .14
RbNOa 515.7 3496 .226 .57
CsN03 552.4 3688 .00503 .019
AgNOa 587.9 2898 .178 .45
TINOa 633.25 3348.3 .0843 .35
SnS 25730 13618 18.2 1.4
PbS 338.66  4867.0 12.3 0.61
Sb2S3 14940 12846 0.247 1.4
Bi 2S3 89320 55.18 10.6 0.012
Li 2S04 394.8 2932 0.482 .42
Na2S04 550.19 4507.0 .0077 .092
k2so 4 814.95 4721.6 .070 .05
Rb2S0 4 471.72 4956.6 .00709 .009
Cs 2S0 4 387.47 4528.7 .0067 .018
Ag2S04 199.04 3188.5 .0223 .032
Pr4NBF4 2973.9 4884.8 .0108 .035
Pr4NPF6 7610.3 6070.0 3.24 • 103 .013
Bu 4NBr 817140 11041 1.29 • 10 4 .017
118
TABLE 177. Equivalent conductance— Continued
A = A \e~E \IRT (ohm 1cm 2equiv_1)
Salt ^A(ohm _1cm2equiv_1) £\(cal mol1
) s(ohm~ 1cm 2
equiv 1)
s%
Bu4NI 136940 9394.2 0.047 2.0
Bu4NPF6 4743.7 5954.3 .041 0.22
Bu4NBPh4 6841.1 6893.0 1.62 • 103 .018
(rcAmyl)4NSCN 577470 9882.2 0.0532 13
Na2Mo0 4 779.9 5713 .142* 0.23
Na2W0 4 381.7 4491 .0352 .060
KSCN 7874 6082 .00708 .053
NaOH 668.2 3120 .0128 .020
KOH 520.2 2467 .490 .50
K2Cr207 6052 8141 .0144 .056
LiC103 9394.7 6072.1 .218 3.2
119
Table
178.
Viscosity
—
Best
equations
120
Table
178.
Viscosity—
Best
equations
—
Continued
121
TABLE
179.
Specific
conductanceexponential
equations
122
Table
179.
Specific
conductanceexponential
equations
—
Continued
123
Table
179.
Specific
conductanceexponential
equations
—
Continued
124
Table
179.
Specific
conductanceexponential
equations
—
Continued
125
Table
179.
Specific
conductanceexponential
equations
—
Continued
126
Table
180
.
Specific
conductance
—
Power
series
equations
—
Continued
297268 068—10 127
Table
180.
Specific
conductance
—
Power
series
equations
—
Continued
128
Table
180.
Specific
conductance
—
Power
series
equations
—
Continued
129
Table
180
.
Specific
conductance
—
Power
series
equations
—
Continued
130
Table 181. Viscosityexponential equations
Salt Viscosity (centipoise) Temperature
range °K
s Centipoise Reference
BeF2 tj = 1.756 • 10 7 exp (58466/RT) B46.9 1252.2 3.08 • 10« [225]
LiCl T) = 3.306 • 102 exp (7007/RT) 902.91082.9 0.0092
[121
]
NaCl rj — 1.860 • 102 exp (9308/RT) 1085.91243.2 .0109[121 ]
KC1 17 = 4.984 • 102 exp (6586/RT) 1056.51202.0 .0167[102
]
RbCl r) = 6.170 • 10~ 2 exp (6094/R7
1
) 1005.21148.2 .0064[121
]
CsCl r) = 6.036 • 10 2 exp (5687/RT) 928.01110.2 .0094
[121
]
CaCl2 17 = 1.088 • 10~ 2 exp (11997IRT) 1058.71242.6 .087 [109]
SrCl2 p = 4.401 • 104 exp (20655/RT) 1150.51258.6 .0706 [109]
BaCl2 17 = 1.643 • 10 3 exp (20029/RT) 1261.41313.9 .0651 [109]
LaCl3 17 = 2.061 • 10 2 exp (13049/RT) 1183 1276 [136]
TiCL, 7]= 4.952 • 10
 2 exp (1643/R71
) 293  333 .0095 [204]
CuCl 7] = 10.42 • 102 exp (5075/RT) 773.2 973.2 .0115 [47]
AgCl 7] = 30.98 • 10 2 exp (2915/RT) 723.2 973.2 .0059 [72]
ZnCl2 t) = 2.476 10 5 exp (24843/RT) 593.2 673.2 578.8 [98]
CdCl2 rj = 24.05 • 10 2 exp (3912/RT) 863.2 963.2 0.0075 [53]
HgCl2 7]6.585 • 10
 2 exp (3624/R71
) 554.0 579.3 .0195 [103]
AlCls 7} = 7.928 • 10 3 exp (3528/R7
1
)461.5 549.2 .00199 [149]
GaCl3 7]
— 1.804 • 102 exp (3193/RT) 355.9 519.7 .0138 [149]
SnCl4 17 = 3.187 • 10 2 exp (1928/RT) 273  423 .0059 [147]
PbCl2 17 = 5.619 • 10~ 2 exp (6762/RT) 773.2 973.2 .0091 [72]
BiCl3 17 = 37.87 10~ 2 exp (4693/RT) 533.2 613.2 .2205 [16]
LiBr 17 = 6.868 • 102 exp (5355/RT) 862.2 1046.2 .0180[102
]
NaBr7i = 11.09 • 10
 2 exp (5132/RT) 1053.71212.7 .0127[102]
KBr 7]= 9.083 • 102 exp (5161/RT) 1017.81181.2 .0139
[102
]
RbBr 7] = 11.58 • 10~ 2 exp (4863/R7
1
) 959.71139.5 .0076[102 ]
AgBr 7] = 38.06 • 102 exp (3088/R71
)713.2 873.2 .0105 [72]
ZnBro 673.2 [981
CdBr2 7) = 18.93 • 10 2 exp (4556/R7
7
)853.2 949.2 .0102 [53]
HgBr2 77 = 1.801 • 10 2 exp (5040/RD 528.2 548.2 .0078 [58]
AlBr3 77 = 3.491 • 10 2 exp (3123/RT) 373  523 .00152 [138]
PbBr2 77 = 16.51 • 10 2 exp (4855/RT) 698.21023.2 .1115 [142]
Lil 77=11.51 • 10 2 exp (4423/RT) 723.2 923.2 .0078 [47]
Nal 77 = 7.171 • 10 2 exp (5673/R7
7
) 946.41107.8 .00847[ 122 ]
KI 77 = 9.836 • 10 2 exp (5343/R7
1
) 975.11165.2 .00851 [122]
Rbl 77 = 8.514 • 10 2 exp (5165/R7
1
) 922.21126.4 .00418 [122
]
Csl 7}= 7.796 • 10 2 exp (5706/RT) 910.21126.9 .0168 [
122 ]
Agl 77=14.81 • 10 2 exp (5259/RT) 878.21100.2 .0831 [24]
Hgl 2 77 = 4.000 • 10 2 exp (4531/RT) 541.2 631.2 .0367 [103]
Li2C03 77 = 1.406 10 3 exp (16893/RT) 1046.21122.2 .1057 [107]
Na2C03 7}= 3.832 • 10
“5 exp (26260/RT) 1152.21245.2 .0112 [107]
k2co 3 77=1.161 • 105 exp (29487/RT) 1186.21257.2 .0207 [107]
LiN0 2 77 = 2.971 • 103 exp (8208/R7
1
) 502.7 527.2 .0816 [207]
NaN02 77 = 4.876 • 102 exp (4680/RT) 563  613 .192 [207]
kno 2 77 = 16.45 • 10 2 exp (3424/R7
1
) 686 .8 725.4 .00767 [125]
RbN02 7}= 8 . 754 10
 2 exp (4495/RT) 712  758 .0054 [207]
CsN02 7j= 0.1058 exp (4213/RT) 688  739 .0082 [207]
LiN03 77 = 5.663 • 10 2 exp (5103/RT) 533.2 702.2 .2283 [38]
NaN03 7j=10.40 10 2 exp (3886/R71
) 589.2 731.2 .0282, [38]
KNOa 77 = 8.384 10 2 exp (4301 /RT) 621.2 815.2 .0278 [38]
RbNOa 7}= 12.96 • 10
 2 exp (3976/R71
) 598  698 .0395 [139]
CsNOa 7}= 0.1284 exp (39U/RT) 698.2 776.2 .0074 [228]
131
Table 181. Viscosityexponential equations — Continued
Salt Viscosity (centipoise) Temperature
range °K
5 Centipoise Reference
AgN03 77= 11 .59  KG 2 exp (3620/RT) 530.0 593.4 0.0054 [69]
T1N03 77 = 8.430 • 10 2 exp (3657/RT) 492.5 553.7 .0141 [191]
B2O3 77 = 6.738 exp (18695/RT) J410 1893 162. [137]
Si02 77 = 9.004 • 104 exp (89236/RT) 2208 2595 65,800 [205]
Ge02 77 = 1.316 • 104 exp (74254//?D 1423 1773 7.610 • 105[140]
Ge0 2 77 = 1.967 • 103 exp (65143//?T) 1745 1991 8380. [137]
As 203 77 = 1.679 • 10 2 exp (22211/RT) 601  703 7680.
[202 ]
Pr4NBF4 77 = 6.663 • 103 exp (6037/RT) 522.8 546.7 0.00147 [190]
Pr4NPF6 tj = 5.752 • 103 exp (6461/RT) 517.5 541.9 .00358 [190]
Pr4NBPh4 tj = 9.287 • 104 exp (8897/RT) 483.5 529.2 .0398 [190]
Bu 4NBF4 77 = 0.2222 exp (7245/RT) 435.4 539.1 .129 [190]
Bu4NPF6 77 = 3.173  103 exp (7159/RT) 529.4 554.1 .00351 [190]
Bu4NBPh4 tj= 1.588 • 103 exp (8235//? 75 516.8 541.8 .00638 [190]
Hex4NBF4 77 = 1.806 • 104 exp (9841/RT) 376.0 502.8 2.90 [190]
(nAmyl)4NSCN 77 = 2.512 105 exp (10551/RT) 325.2 383.2 6.49 [172]
NaSCN 77 = 4.935 • 10~ 2 exp (4636/RT) 578.0 634.1 0.0223
[112
]
KSCN 7}= 8.580 • 10
3 exp (6454/RT) 448.8 523.8 .1792[112
]
NaOH 77 = 7.21110 2 exp (4937/RT) 623.2 823.2 .0881 [37]
KOH 7}= 2.295102 exp (6177/RT) 673.2 873.2 .0201 [37]
K2Cr2C>7 77 = 8.051 • 102 exp (6879/RT) 670.2 780.2 .1537 [3]
NaP0 3 77 = 2.412102 exp (19899/RT) 916 1029 63.3[200
]
LiC103 77 = 1.942 • 103 exp (7832/RT) 404.9 440.0 0.564 [175]
132
Table
182
.
Viscosity
power
series
equations
133
Table
182.
Viscosity
power
series
equations
—
Continued
134
8. References
[References which are marked marginally have data for molten salt mixtures; *, specific conductance; t, density and t, viscosity.]
[1] F. W. G. Kohlrausch, Wied. Ann. 17, 642 (1882).
[2] L. Poincare, Ann. Chim. Phys. 21, 289 (1890).
t[3] E. Brunner, Z. angew. Chem. 38, 350 (1904).
[4] K. Arndt, Z. Elektrochem. 12, 337 (1906).
t[5] H. M. Goodwin and R. D. Mailey, Phys. Rev. 23, 22
(1906); 25, 469 (1907); 26, 28 (1908).
t[6) K. Beck, Z. physik. Chem. 58, 425 (1907).
[7] R. Lorenz and H. T. Kalmus, ibid. 59, 17 (1907).
[8] idem, ibid. 59, 244 (1907).
*t[9] H. M. Goodwin and R. D. Mailey, Trans. Am. Electro
chem. Soc. 11, 211 (1907).
*[10] K. Arndt and A. Gessler, Z. Elektrochem. 14, 662
(1908).
*t[ll] idem, ibid. 14, 665 (1908).
[12] C. E. Fawsitt, J. Chem. Soc. 93, 1299 (1908).
[13] idem, Proc. Roy. Soc. A80, 290 (1908).
$[14] K. Arndt, Z. Apparatekunde 3, 549 (1908).
t[15] R. Lorenz, H. Frei and A. Jabs, Z. physik. Chem. 61,468 (1908).
$[16] A. H. W. Aten, ibid. 66, 641 (1909).
*$[17] K. Arndt and W. Lowenstein, Z. Elektrochem. 15, 789
(1909).
[18] E. Prideaux; J. Chem. Soc. 97, 2032 (1910).
*f[19] A. H. W. Aten, Z. physik. Chem. 73, 578 (1910).
[20] idem, ibid. 78, 1 (1912).
[21] C. Tubandt and E. Lorenz, ibid. 87, 513 (1914).
[22] R. Lorenz and A. Hochberg, Z. anorg. Chem. 94, 288
(1916).
[23] idem, ibid. 94, 305 (1916).
[24] idem, ibid. 94, 317 (1916).
[25] F. M. Jaeger, ibid. 101, 1 (1917).
[26] F. M. Jaeger and B. Kapma, ibid. 113, 27 (1920).
*t[27] A. Sandonnini, Gazz. Chim. Ital. 501, 289 (1920).
[28] A. Fleck and T. Wallace, Trans. Faraday Soc. 16,346 (1920).
[29] G. V. Hevesy, Kgl. Danske Videnskab. Selskab. Medd.Ill, 13 (1921).
[30] W. Biltz and W. Klemm, Z. anorg. Chem. 131, 22
(1923).
[31] K. Arndt and W. Kalass, Z. Elektrochem. 30, 12
(1924).
[32] A. Voigt and W. Biltz, Z. anorg. Chem. 133, 277
(1924).
[33] W. Biltz and W. Klemm, Z. physik. Chem. 110, 318
(1924).
[34] W. Klemm, Z. anorg. Chem. 152, 252 (1926).
[35] W. Biltz and W. Klemm, ibid, 152, 225, 267 (1926).
[36] W. Klemm, ibid. 152, 235, 295 (1926).
*$$[37] K. Arndt and G. Ploetz, Z. physik. Chem. 121, 439
(1926).
[38] R. S. Dantuma, Z. anorg. Chem. 175, 1 (1928).
[39] J. Bureau, Ann. Chim. 8, 5 (1937).
t[40] A. Wachter and J. H. Hildebrand, J. Am. Chem. Soc.
52, 4655 (1930).
[41] C. Tubandt, LandoltBornstein, Erg.Bd. II, p. 1042
(SpringerVerlag, Berlin, 1931).
*[42] E. Ryschkewitsch, Z. Elektrochem. 39, 531 (1933).
t[43] E. J. Salstron, J. Am. Chem. Soc. 55, 1029 (1933).
*t[44] S. Karpachev, A. Stromberg and V. N. Podchainova,Zhur. Obshchei Khim. 5, 1517 (1935).
[45] S. Karpachev, Zhur. Fiz. Khim. 6, 1079 (1935).
*[46] K. P. Batashev, Legkie Metal. 5, 48 (1936).
[47] S. Karpachev and A. Stromberg, Zhur. Fiz. Khim. 11,852 (1938).
[48] K. E. Schwarz, Z. Elektrochem. 45 , 740 (1939).
*t[49] V. P. Barzakovskii, Bull. Acad. Sci. URSS, Classe
Sci. Chim. 825 (1940).
*[50] E. Lee and E. P. Pearson, Trans. Electrochem. Soc.
88, 171 (1945).
*[51] H. Bloom and E. Heymann, Proc. Roy. Soc. (London)A188, 392 (1947).
*[52] H. R. Bronstein and M. A. Bredig, J. Am. Chem. Soc.
80, 2077 (1959).
t[53] H. Bloom, B. S. Harrap and E. Heymann, Proc. Roy.Soc. (London) A194, 237 (1948).
t[54] N. K. Boardman, F. H. Dorman and E. Heymann, J.
Phys. Chem. 53, 375 (1949).
*t[55] H. Grothe, Z. Elektrochem. 53, 362 (1949).
t[56] S. P. Pavlenko, Izvest. Sektora Fiz.Khim. Anal., Inst,
Obshch, Neorg. Khim. Akad. Nauk SSSR 17, 220(1949).
$[57] K. Ogawa, Nippon Kinzoku Gakkaishi (J. Japan Inst.
Metals) 14B, No. 2, 49 (1950).
*1$[58] G. Jander and K. Broderson, Z. anorg. Chem. 264,57(1951).
[59] J. W. Menary, A. R. Ubbelohde and I. Woodward,Proc. Roy. Soc. (London) A203, 158 (1951).
*t[60] R. C. Spooner and F. E. W. Wetmore, Can. J. Chem. 29,777(1951).
*t[61] J. Byrne, H. Fleming and F. E. W. Wetmore, ibid. 30,922 (1952).
[62] J. D. Edwards, C. S. Taylor, A. S. Russel and L. F.
Maranville, J. Electrochem. Soc. 99, 527 (1952).
*t[63] P. W. Huber, E. V. Potter and H. W. St. Clair, U.S.Bur. Mines, Rept. of Investigations 4858 (1952).
[64] L. Ochs and F. Strassmann, Z. Naturforsch 7b, 637(1952).
[65] W. J. Davis, S. E. Rogers and A. R. Ubbelohde, Proc.
Roy. Soc. (London) A2 2 0, 14 (1953).
*t[66] H. Bloom, I. W. Knaggs, J. J. Molloy, and D. Welch,Trans, Faraday Soc. 49, 1458 (1953).
*t[67] J. D. Edwards, C. S. Taylor, L. A. Cosgrove, andA. S. Russell, J. Electrochem. Soc. 100, 508 (1953).
[68] A. E. van Arkel, E. A. Flood, and N. A. H. Bright,
Can. J. Chem. 31, 1009 (1953).
[69] F. A. Pugsley and F. E. W. Wetmore, ibid. 32, 839
(1954).
t[70] J. S. Peake and M. R. Bothwell, J. Am. Chem. Soc. 76,2653(1954).
*$$[71] I. P. Vereschetina and N. P. Luzhnaya, Izvest. Sektora
Fiz.Khim. Anal., Inst. Obshch. Neorg. Khim., Akad.,
Nauk, SSSR. 25, 188 (1954).
*4[72] B. S. Harrap and E. Heymann, Trans. Faraday Soc.
51,259(1955).
[73] D. Argyriades, Dissertation, Aachen (1955).
[74] J. W. Johnson, P. A. Agron and M. A. Bredig, J. Am.Chem. Soc. 77, 2734 (1955).
[75] C. Kroger and P. Weisgerber, Z. physik. Chem. (Frank
furt) 5, 3 (1955).
*$[76] K. B. Morris, M. I. Cook, C. Z. Sykes, and M. C.
Templeman, J. Am. Chem. Soc. 77, 851 (1955).
*[77] P. I. Protsenko, Izvest. Sektora Fiz.Khim. Anal.,
Inst. Obshchei Neorg. Khim., Akad Nauk SSSR. 26,173(1955).
*$$[78] V. D. Polyakov, ibid. 26, 191 (1955).
*$[79] E. R. van Artsdalen and I. S. Yaffe, J. Phys. Chem. 59,118(1955).
[80] E. Vogel, H. Schinke and F. Sauerwald, Z. anorg.
allgem. Chem. 284, 131 (1956).
[81] H. Schinke and F. Sauerwald, ibid. 287, 313 (1956).
[82] I. S. Yaffe and E. R. van Artsdalen, J. Phys. Chem. 60,1125(1956).
[83] idem; Chemistry Division Semiannual Progress Report,
Oak Ridge National Laboratory, ORNL—2159, p. 77
(1956).
[84] D. F. Smith and E. R. van Artsdalen, ibid., ORNL—2159, p. 80 (1956).
[85] H. Winterhager and L. Werner; Forschungsber.
Wirtsch. Verkehrsministeriums NordrheinWestfalen,
No. 341 (1956).
*[86] idem., ibid. No. 438 (1957).
*t[87] F. R. Duke and R. A. Fleming, J. Electrochem. Soc.
104,251 (1957).
*t[88] E. W. Yim and M. Feinleib, ibid. 104, 622, 662 (1957).
[89] R. B. Ellis, J. E. Smith and E. B. Baker, J. Phys. Chem.62,766(1958).
135
*tt[90] N. N. Greenwood and I. J. Worrall, J. Chem. Soc. 1680
(1958).
t[91] R. B. Ellis and J. E. Smith, Prog. Rep. U.S.A.E.C.,
Contract No. AT(40—1)—2073, March 1958; ibid.
December 1958.
*t[92] Y. Doucet and M. Bizouard, Compt. rend. 248, 1328
(1959).
*t[93] idem. Bull. soc. chim. France 1570 (1959).
[94] J. O’M. Bockris’, E. H. Crook, H. Bloom and N. E.
Richards, Proc. Roy. Soc. (London) A255, 558 (1960).
[95] A. D. Kirshenbaum, J. A. Cahill, and C. S. Stokes,
J. Inorg. Nucl. Chem. 15, 297 (1960).
[96] J. O’M. Bockris, A. Pilla and J. L. Barton, J. Phys.
Chem. 64 , 507 (1960).
*tt[97] M. F. Lantratov and O. F. Moiseeva, Zhur. Fiz. Khim.
34,367(1960).
[98] J. D. Mackenzie and W. K. Murphy, J. Chem. Phys. 33,366(1960).
*t[99] G. W. Mellors and S. Senderoff, J. Phys. Chem. 64,294(1960).
*[100] Y. Doucet and M. Bizouard, Compt. rend. 250, 73
(1960).
t[101] G. J. Janz and M. R. Lorenz, J. Electrochem. Soc. 108,1052 (1961).
[102] I. G. Murgulescu and S. Zuca, Z. physik. Chem. 218,379(1961).
[103] G. J. Janz and J. D. E. McIntyre, J. Electrochem. Soc.
109,842(1962).*[104] L. F. Grantham and S. J. Yosim, J. Chem. Phys. 38,
1671 (1963).
*t[105] E. F. Riebling and C. E. Erickson, J. Phys. Chem. 67,307 (1963).
*[106] A. S. Dworkin, R. A. Sallach, H. R. Bronstein, M. A.
Bredig and J. D. Corbett, ibid, 67, 1145 (1963).
4[107] G. J. Janz and F. Saegusa, J. Electrochem. Soc. 110,452(1963).
[108] W. Karl and A. Klemm, Z. Naturforsch. 19a, 1619
(1964).
[109] G. J. Janz and R. D. Reeves, Trans. Faraday Soc. 61,2305(1965).
[110] J. P. Frame, E. Rhodes and A. R. Ubbelohde, Trans.
Faraday Soc. 55, 2039 (1959).
[111] S. Karpachev, Zhur. Obshch. Khim. 5, 625 (1935).
[112] D. W. Plester, S. E. Rogers and A. R. Ubbelohde, Proc.
Roy. Soc. A2 3 5 , 469 (1956).
[113] J. O’M. Bockris, A. Pilla, and J. L. Barton, Rev. Chim.Acad. Rep. Populaire Roumaine 7, No. 1, 59 (1962).
*[114] L. F. Grantham, J. Chem. Phys. 43, 1415 (1965).
[115] A. Kvist and A. Lunden, Z. Naturforsch. 20a, 235
(1965).
*[116] L. A. King and F. R. Duke, J. Electrochem. Soc. Ill,712(1964).
[117] A. Kvist and A. Lunden, Z. Naturforsch 20a, 102 (1965).
*[118] A. S. Dworkin, H. R. Bronstein, and M. A. Bredig,
Discussions Faraday Soc. 32, 188 (1961).
*[119] H. R. Bronstein, A. S. Dworkin and M. A. Bredig,
J. Phys. Chem. 66, 44 (1962).
*[120] A. S. Dworkin, H. R. Bronstein, and M. A. Bredig,
J. Phys. Chem. 66, 1201 (1962).
[121] I. G. Murgulescu and S. Zuca, Z. physik. Chem. 222,300 (1963).
$[122] I. G. Murgulescu and S. Zuca, Revue Roumaine deChimie. 10, 123 (1965).
[123] E. H. Crook, Ph. D. Thesis, University of Pennsylvania,Philadelphia, Pa. (1958).
*[124] F. R. Duke and L. Bissell, J. Electrochem. Soc. Ill,717 (1964).
[125a] E. R. Buckle and P. E. Tsaoussoglou, unpublished work(1966).
[125b] E. R. Buckle and P. E. Tsaoussoglou, J. Chem. Soc.
667 (1964); Trans Faraday Soc. 60, 2144 (1964).
[125c] A. R. Ubbelohde, Imperial College, London (private
communication, 1966).
[126] A. D. Kirshenbaum, J. A. Cahill, P. J. Gonigal, andA. V. Grosse, J. Inorg. Nucl. Chem. 24, 1287 (1962).
[127] J. W. Johnson, W. J. Silva, and D. Cubicciotti, Tech.Report No. 38 (1965) Stanford Research Inst., MenloPark, California.
4[128] G. V. Voroliev, S. F. Pal’guev, and S. V. Karpachev,Trudy No. 6 (1965); Inst. Electrochem. Urals. Acad.Sci., Eng. Trans 1. Electrochem. Solid and Liq.
Electrolytes 3, 33 (1966). Consultants Bureau, NewYork (1966).
[129] I. G. Murgulescu, and S. Zuca, private communication,June 1966; S. Zuca and L. Ionescu, Revue Roumainede Chimie, to be published.
[130] Selected Values of Chemical Thermodynamic Prop
erties, NBS Circular 500, United States GovernmentPrinting Office, Washington, D.C. (1952).
*1$[131] Edward W. Washburn, Ed., International Critical
Tables of Numerical Data Physics, Chemistry andTechnology (McGrawHill Book Company, Inc.,
New York, N.Y., 1926).
[132] K. K. Kelly, Contributions to the Data on Theoretical
Metallurgy, Bureau of Mines Bulletin 393, United
States Government Printing Office, Washington,D.C. (1936).
[133] Samuel J. Schneider, Compilation of the melting points
of the metal oxides, NBS Mono. 68, United States
Government Printing Office, Washington, D.C. (1963).
*1$[134] M. Blander, Ed., Molten Salt Chemistry (Interscience
Publishers, New York, 1964).
*t[135] F. R. Duke and R. A. Fleming, J. Electrochem. Soc.
105,412(1958).
$[136] M. V. Smirnov, V. A. Khokhlov and V. P. Stepanov,
Russ. J. Phys. Chem. 40 , 671 (1966).
[137] E. F. Riebling, Corning Glass Works, Corning, NewYork (private communication 1966).
[138] K. H. Grothe and P. Kleinschmit, Institut fur Anor
ganische Chemie der Technischen HochschuleHannover (private communications, 1966).
$[139] I. G. Murgulescu and S. Zuca, Electrochimica Acta 11,1383 (1966).
t[140] C. R. Kurkjian and R. W. Douglas, Phys. and Chem.Glasses 1, 19 (1960).
$[141] E. F. Riebling, J. Chem. Phys. 39, 1889 (1963).
t[142] I. G. Murgulescu and S. Zuca, Revue Roumaine deChimie 10, 129 (1965).
[143] J. D. Mackenzie, J. Chem. Phys. 32, 1150 (1960).
1$[144] E. F. Riebling, J. Amer. Ceram. Soc. 49, 19 (1966).
[145] J. D. Mackenzie, Trans. Faraday Soc. 52, 1564 (1956).
[146] J. D. Mackenzie, J. Chem. Phys. 29 , 605 (1958).
[147] P. Pugachevich, L. Nisel’son, T. Sokolova, and N.
Anurov, Russ. J. Inorg. Chem. 8, 404 (1963).
[148] N. N. Greenwood and K. Wade, J. Inorg. and Nucl.
Chem. 3, 349 (1957).
[149] L. A. Nisel’son and T. D. Sokolova, Russ. J. Inorg.
Chem. 10, 827 (1965).
t[150] M. C. Bell and S. N. Flengas, J. Electrochem. Soc. 113,27(1966).
*[151] M. C. Bell and S. N. Flengas, J. Electrochem. Soc. 113,31 (1966).
*[152] M. Bourgon, G. Derge and G. M. Pound, AIME Trans.,
Journal of Metals 1454 (Nov. 1957).
*[153] D. Argyriades, G. Derge, and G. M. Pound, AIMETrans. 2 1 5 , 909 (1959).
*[154] A. A. Velikanov, Ph. D. Thesis, Kiev State University,
Kiev, U.S.S.R. (1962).
*[155] A. A. Velikanov, Transactions of the AllState Conference on the Physical Chemistry of Fused Salts
and Slags, Moscow (Nov. 22—25, 1960).
*[156] A. A. Velikanov, Ukrain. Khim. XXVI, 319 (1960).
[157] Yu. K. Delimarskii and A. A. Velikanov, Akad. Nauk.SSSR. Zhurnal Neorg. Khimii. Ill, 1075 (1958).
[158] A. A. Velikanov, Visnif Kievskogo Universitetu No. 3,
1960 Seriya Fizikh, Khimii, vip. 1, Khimiya. 123 (1960).
*[159] H. Inoye, J. W. Tomlinson and J. Chipman, Trans.
Faraday Soc. 49, 796 (1953).
[160] H. H. Baumbach and C. Wagner, Z. Physik. Chem.B22, 199 (1933).
*[161] A. Kvist, Z. Naturforsch. 21a, 1221 (1966); 21a, 1601
(1966).
[162] A. Kvist and A. Lunden; Z. Naturforch. 21a, 1509
(1966).
*t[163] E. F. Riebling and S. D. Gabelnick, J. Electrochem.
Soc. 112, 822 (1965).
136
*££[164] D. F. Williams, Ph. D. Thesis, University of Manitoba,
Canada (1963).
[165] K. Moers, Z. anorg. Chem. 113, 179 (1920).
*t[166] M. C. Bell and S. N. Flengas, J. Electrochem. Soc.
111,569,575(1964).[167] A. D. Kirshenbaum and J. A. Cahill, J. Inorg. Nucl.
Chem. 19, 65 (1961).
*[168] G. M. Pound, G. Derge, and G. Osuch, Trans. AIME203,481(1955).
*[169] L. Yang, G. M. Pound, and G. Derge, Trans. AIME204, 783 (1956).
[170] F. H. Spedding and A. H. Daane, Met. Rev. 5, 297
(1960).
*[171] A. S. Dworkin, H. R. Bronstein, and M. A. Bredig, J.
Phys. Chem. 67, 2715 (1963).
[172] L. C. Kenausis, E. C. Evers, and C. A. Kraus, Proc.
Nat. Acad. Sc. 49, 141 (1963).
t[ 1 73] P. I. Protsenko and A. Ya. Malakhova, Russ. J. Inorg.
Chem. 6, 850 (1961).
*[174] A. N. Campbell, E. M. Kartzmark, and D. F. Williams,
Can. J. Chem. 40, 890 (1962).
t£[175] A. N. Campbell and D. F. Williams, Can. J. Chem.42, 1779 (1964).
[176] L. J. B. Husband, J. Sci. Inst. 35, 300 (1958).
t[177] G. F. Petersen, W. M. Ewing, and G. P. Smith, J. Chem.and Eng. Data 6, 540 (1961).
t[l 78] R. W. Neithamer and J. S. Peake, J. Chem. and Eng.
Data 6, 197 (1961).
*[179] P. I. Protsenko and R. P. Shisholina, Ukr. Khim. Zh.
31, 1048 (1965).
t[180] G. P. Smith and G. F. Petersen, J. Chem. and Eng.
Data 6, 493 (1961).
*t[181] M. Bizouard, Ann. Physique 6, 851 (1961).
[182] H. R. Bronstein, A. S. Dworkin, and M. A. Bredig,
Chemistry Division Annual Progress Report, OakRidge National Laboratory, ORNL2983 (1960).
*[183] M. F. Lantratov and O. F. Moiseeva, Zhur. Prikl. Khim.34, 1169(1961).
t[184] V. D. Polyakov and S. I. Berul, Izvest. Sektora Fiz.
Khim. Anal. Akad. Nauk SSSR. 26, 164 (1955).
*[185] P. I. Protsenko and O. N. Shokina, Russ. J. Inorg.
Chem. 5, 208 (1960).
*[186] Yu. K. Delimarskii, I. N. Sheiko, and V. G. Feshchenko,Zhur. Fiz. Khim. 29, 1499 (1955).
*[187] M. F. Lantratov and O. F. Moiseeva, Zhur. Prikl. Khim.36, 2201 (1963).
*[188] I. N. Belaev, Izvest Sektora Fiz.Khim. Anal. Akad.Nauk SSSR 23, 176 (1953).
[189] L. F. Grantham and S. J. Yosim, J. Chem. Phys. 45,1192 (1966).
[190] J. E. Lind, Jr., H. A. A. AbdelRehim, and S. W.Rudich, J. Phys. Chem. 70, 3610 (1966).
[191] G. J. Janz and A. Timidei, Trans. Faraday Soc. (in
publication, 1968).
*££[192] I. G. Murgulescu and S. Zuca, Rev. Chim. Acad. Rep.Populaire Roumaine 2, 227 (1959).
[193] C. A. Angell, J. Electrochem. Soc. 112, 956 (1965).
*[194] H. C. Cowen and H. J. Axon, Trans. Faraday Soc. 52,242 (1956).
*[195] E. R. Buckle and P. E. Tsaoussoglou, Trans. FaradaySoc. 60, 2144 (1964).
t[196] E. R. Buckle, P. E. Tsaoussoglou, and A. R. Ubbelohde,Trans. Faraday Soc. 60, 684 (1964).
[197] V. P. Mashovetz and Z. F. Lundina, Ukrain. Akad.Nauk. Inst., Proc. First All Union Conf. on AqueousSolutions, 191 (1935).
*[198] H. R. Bronstein and M. A. Bredig, Chemistry Division
Semiannual Progress Report, Oak Ridge National
Laboratory, ORNL2782, 59 (1959).
*[199] B. F. Markov and V. D. Prisyazhnyii, Ukrain. Khim,Zhur. 28, 268 (1962).
£[200] K. Arndt; Z. Elektrochem. 13, 578 (1907).
[201] A. Napolitano, P. Macedo, and E. Hawkins, J. Amer.Ceram. Soc. 48, 613 (1965).
[202] I. Karutz and I. Stranski, Z. Anorg. Chem. 292 , 330
(1957).
*££[203] E. J. Gorenbein, Zhur. Obshchei Khim. 17, 871 (1947).
££[204] A. P. Toropov, J. Gen. Chem. (U.S.S.R.) 26, 3635 (1956).
£[205] J. F. Bacon, A. A. Hasapis and J. W. Wholley, Jr.,
Phys. and Chem. of Glasses 1, 90 (1960).
£[206] J. O’M. Bockris, J. D. Mackenzie and J. A. Kitchener,
Trans. Faraday Soc. 51, 1734 (1955).
[207] P. I. Protsenko, A. V. Protsenko and O. N. Razumouskaya, Russ. J. Inorg. Chem. 10, 405 (1965).
£[208] P. I. Protsenko and O. N. Shokina, Russ. J. Inorg.
Chem. 9, 82 (1964).
£[209] P. C. Li, A. C. Ghose, and G. J. Su, J. Amer. Ceram.Soc. 47, 478 (1964).
[210] V. T. Slavyanskii, Dokl. Akad. Nauk. SSSR 58, 1077
(1947) (Translation available as AECtr—3785).[211] C. E. Messier, E. B. Damon, P. C. Maybury, J. Mellor,
and R. A. Seales, J. Phys. Chem. 62 , 220 (1958).
[212] S. N. Flengas, University of Toronto, Toronto, Canada(private communication 1967).
[213] T. F. Young, Argonne National Laboratory, Argonne,Illinois (private communication 1966).
*t[214] S. I. Sklyarenko and I. E. Krauze, Zhur. Fiz. Khim. 13,1315(1939).
*[215] A. G. Bergman and I. M. Chagin, Izvest. Akad. Nauk.S.S.S.R., Ser. Khim. 5, 727, 738 (1940).
t[216] I. I. Bokhovkin, J. Gen. Chem. (U.S.S.R.) 19, 805
(1949).
[217] S. Brillant, Compt. Rend. Ser. C. 262 , 447 (1966).
[218] L. C. Kenausis, E. C. Evers and C. A. Kraus, Proc.
Nat. Acad. Sci. 48, 121 (1962).
[219] B. R. Sundheim and A. Berlin, J. Phys. Chem. 68,1266 (1964).
[220] P. Walden and E. J. Birr, Z. Physik. Chem. 160, 57
(1932).
[221] J. E. Lind, Cornell University, Ithaca, New York(private communication 1966).
£[222] E. F. Riebling, J. Am. Ceram. Soc. 47, 478 (1964).
[223] E. A. Ukshe, Russian Chemical Reviews 34, 141 (1965).
*£[224] B. de Nooijer and J. A. A. Ketelaar, unpublished work(1967); B. de Nooijer, Ph. D. Thesis. Amsterdam(1965).
[225] C. T. Moynihan and S. Cantor, Oak Ridge National
Laboratory, Oak Ridge, Tennessee (private communication, 1967).
[226] A. Kvist, Z. Naturforsch. 22a, 208, 467 (1967).
[227] C. E. Johnson, private communication to G. J. Janz
(1968).
[228] P. I. Protsenko and O. N. Razumovskaya, Zh. Prikl.
Khim. 38, 2355 (1965).
9. Additional Data Sources
[1] L. S. Charnoff, An Annotated Bibliography of Molten Salts;
Univ. Microfilms Inc., Ann Arbor, Mich. (1958).
[2] G. J. Janz, Bibliography on Molten Salts, Rensselaer Poly
technic Inst. Tech. Bull. Series, Troy, N.Y. (1961).
[3] C. J. Smithells, Metals Reference Book (Butterworths Sci.
Public. (London), 1955).
[4] Toshio Ishino et al. Ed., Physicochemical constants of
fused salts, Electrochem. Soc. Japan, Osaka (1964).
[5] G. Petit, La Cryometrie A Haute Temperature et ses Applications, Masson et Cie, Editeurs (Paris) 1965.
[6] T. Fprland, K. Grojtheim, K. Motzfeld, and S. Urnes, Eds.,
Selected Topics in High Temperature Chemistry, Univesitetsforloget (Oslo), 1966; Scandinavian Univ. Books(Boston).
[7] G. J. Janz, Molten Salt Handbook (Academic Press Inc.,
Publ., N.Y., 1967).
137
[8] Electrochemistry of Molten and Solid Electrolytes, Engl.
Transl., Trudy No. 1, Vol. 1 (1961); Trudy No. 4, Vol. 2(1964) and Trudy No. 6, Vol. 3., Consultants Bureau,N.Y. (19611966).
[9] A. G. Morachevskii, Review of electrochemistry of moltensalts, J. Appl. Chem. U.S.S.R. (Engl. Transl.) 33 , 1422
(1960); 34 , 1339 (1961); 35 , 1337 (1962); 36 , 1325 (1963).
[10] LandoltBornstein, Vol. 2, Pt. Ill (SpringerVerlag, Berlin,
1956).
[11] International Critical Tables, (McGrawHill Book Co.,
New York, N.Y., 1933).
[12] J. Lunsden, Thermodynamics of Molten Salt Mixtures(Academic Press (London and N.Y.) 1966).
[13] M. R. Lorenz and G. J. Janz, Molten Carbonates, Bibliogra
phy, U.S. Dept. Commerce, O.T.S. Rpt. P.B. 151991,
Washington (1958).
[14] G. J. Janz, R. D. Reeves, and A. T. Ward, Molten Salt Data:
Electrical Conductance, Density, and Viscosity; Rensselaer Polytechnic Institute Technical Bulletin Series
(1964), Troy, N.Y.
[15] M. Blander, Ed., Molten Salt Chemistry (Interscience
Publishers, New York, 1964).
[16] B. R. Sundheim, Ed., Fused Salts (McGrawHill Book Co.,
New York, N.Y., 1964).
[17] Yu. K. Delimarskii and B. F. Markov, Electrochemistry of
Fused Salts, translated by A. Peiperel and R. E. Wood,Eds. (Sigma Press, Washington, D.C., 1961).
[18] H. Bloom and J. O’M. Bockris, Eds., Advances in Electrochemistry, Vol. II (Butterworth Publ., N.Y., 1959).
[19] A. D. Graves, D. J. Inman, and G. J. Hills, in P. Delahay andC. Tobias (ed.) Advances in Electrochemistry and Electrochemical Engineering, Vol. 4 (InterscienceWiley,N.Y., 1965).
[20] J. D. Corbett and F. R. Duke, in H. B. Jonassen and A.Weissberger, Eds. Technique of Inorganic Chemistry,Vol. 1 (Interscience Publishers, 1963).
[21] J. O’M. Bockris, J. L. White, J. D. Mackenzie, Eds., PhysicoChemical Measurements of High Temperatures (Academic Press Inc., New York, 1959).
[22] R. A. Bailey and G. J. Janz, in J. Lagowski, ed., NonAqueousChemistry (Academic Press, Inc., N.Y., 1965).
[23] J. D. Corbett in A. F. Scott, Ed., Survey of Progress in
Chemistry. Vol. 2 (Academic Press, Inc., N.Y., 1965).
[24] G. J. Janz and S. C. Wait, in H. A. Symanski (ed.,) RamanSpectroscopy (Plenum Press, N.Y., 1966).
[25] R. D. Reeves and G. J. Janz, in P. Delahay and C. Tobias(eds.) Advances in Electrochemistry and ElectrochemicalEngineering, Vol. 5 (InterscienceWiley, N.Y., 1966).
[26] D. Inman and N. S. Wrench, Corrosion In Fused Salts,
Brit. Corros. J. 1, 246 (1966).
[27] Soviet Research on Corrosion of Special Alloys, 19501960U.S. Dept. Commerce, O.T.S. Report 6131480, Washington (1961).
[28] V. S. Bagotskii and Yu. B. Vasilev, Fuel Cells; Eng. Transl.,
Consultants Bur. N.Y. (1966).
10. Compound Index
Page
AgBr 16, 70, 110, 115, 117, 120, 123, 128, 131, 133
AgCl 10, 56, 109, 114, 117, 120, 122, 127, 131, 133
AgF 4, 47, 109, 122, 126
Agl 21, 81, 111, 115, 118, 121, 124, 128, 131, 133
AgNO :! 28, 90, 112, 115, 118, 121, 125, 129, 132, 134
Ag,S 31, 96, 112, 125, 130
Ag>S0 4 33, 100, 112, 116, 118, 125, 130
AlBr:s 18, 72, 120, 131, 133
AlCl:i 11, 58, 114, 116, 120, 131, 133
All, 21, 79, 111, 115, 118, 124, 128
(n  AmylLNSCN... 34, 102, 113, 116, 119, 121, 125, 130, 132, 134
As 20, 30,94,121,132,134
B.O, 29, 92, 115, 116, 121, 132, 134
BaBr, 16, 68. 110. 115, 117, 123, 128
BaCl, 7, 51, 109, 114, 117, 120, 122, 127, 131, 133
BaF, 4, 45, 114
BaI» 21, 79, 111, 115, 118, 124, 128
Ba(NO.)> 25, 87, 111, 115. 118, 124, 129
BeCl, 6, 50, 109, 114, 117, 122, 126
BeF, 3, 44, 120, 131, 133
BiBr:i 18, 75, 110, 115, 118, 123, 128
BiCL 13, 63, 110, 114, 118, 120, 123, 127, 131, 133
BiL 23, 85, 111, 124, 129
Bi>03 30, 94, 112, 125, 129
Bi,Ss 31, 98, 112, 115, 118, 125, 130Bu 4NBF4 34, 101, 116, 118, 121, 132, 134
Bu 4NBPh 4 34, 102, 113, 116, 119, 121, 125, 130, 132, 134
Bu 4NBr 33, 101, 112, 116, 118, 125, 130
Bu 4NI 33, 101, 112, 116, 119, 125, 130
Bu 4NPFk 34, 102, 112, 116, 119, 121, 125, 130, 132, 134
CaBr2 15, 67, 110, 114, 117, 123. 128
CaCl, 7, 50, 109, 114, 117, 120, 122, 127, 131, 133CaF.» 4 44 114
Cal,~. 20, 78, 111, 115, 118,’ 124, 128
CdBr 17, 71, 110, 115, 118, 120, 123, 128, 131, 133
CdCL 11, 57, 110, 114, 117, 120, 123, 127, 131, 133
Cdl 2 22, 82, 111. 115, 118, 124, 128
CeCL 8, 53, 109, 114, 122, 127
CeF :) 4, 45, 114
Page
CeL 21, 80, 111, 124, 128
CoS 30, 95, 112, 125, 129
CrO :i 29, 91, 112. 125. 129
CsBr 15, 66, 110, 114, 117. 123, 128
CsCl 6, 49, 109. 114, 117, 120, 122, 126, 131. 133
CsF 3, 43, 109, 114, 117, 122, 126
Csl 20, 77, 111, 115, 118. 120, 124, 128, 131, 133
CsN02 25, 87, 111, 121, 124, 129. 131, 134
CsNO:, 28, 90, 112, 115, 118, 121, 125, 129. 131, 134
Cs,S0 4 32, 100. 112, 116, 118, 125, 130
CuBr 16. 69, 110, 123, 128
CuCl 9, 56, 109, 114, 117, 120, 122, 127. 131. 133
CuF2 4, 46, 109, 122, 126
Cu 2S 31, 96, 112, 125, 129
DyCL 9, 54, 109, 122, 127
ErCl.i 9, 54, 109, 122, 127
FeO 29, 92, 112, 125, 129
FeS 30, 95, 112, 129
GaCL 12, 59, 114, 120, 131, 133Gal, 22, 83, 111. 115, 118, 124. 129GdBr.) 16, 69, 110, 123, 128GdCL 9 r 54, 109, 122. 127Ge0 2 30, 93, 112, 121, 125, 132, 134GeS 31. 96, 112, 125, 130
HeX4NBF4 34,102.116,121,132,134HgBr2 17, 71, 110, 115, 118. 120, 123, 128, 131, 133HgCl 11, 58, 110. 114, 117, 123. 127HgCl, 11, 58, 110, 114, 117, 120. 123. 127. 131, 133HgL 22, 82, 111, 115, 118. 121, 124, 129, 131, 133HoCL 9, 54, 109, 122, 127
InBr.) 18. 72, 110, 115, 118, 123, 128InCl 12, 59, 110, 114, 117. 123, 127InCl2 12, 60, 110, 114, 117, 123, 127In Cl.) 12, 60, 110, 114, 117. 123, 127
Inl; , 22, 83, 111, 115, 118, 124, 129
138
Page
KBr 14, 65, 110, 114, 117, 120, 123, 127, 131, 133
KC1 5, 48, 109, 114, 117, 120, 122, 126, 131, 133
K,CO j 23, 86, 111, 115, 118, 121, 124, 129, 131, 133
K,Cr,0 7 36, 106, 113, 116, 119, 121, 126, 130, 132, 134
KF 3, 43, 109, 114, 117, 122, 126
KI 19, 76, 111, 115, 118, 120, 124, 128, 131, 133
K,Mo0 4 35, 104, 116
KNO> 24, 87, 111, 115, 118, 121, 124, 129, 131, 133
KNO, 26, 89, 111, 115, 118, 121, 124, 129, 131, 134
KOH 36, 106, 113, 116, 119, 121, 126, 130, 132, 134
KSCN 35, 105, 113, 116, 119. 121, 126, 132, 134
K,S0 4 32, 99, 112, 116, 118, 125, 130
K 2W0 4 35, 104, 116
LaBr, 16, 68, 110, 115, 117, 123, 128
LaCli 8, 52, 109, 114, 117, 120, 122, 127, 131
LaF, 4, 45, 114
Lai, 21, 80, 111, 124, 128
LiBr 14, 64, 110, 114, 117, 120, 123, 127, 131, 133
LiCl 4, 47, 109, 114, 117, 120, 122, 126, 131, 133
LiClO's 37, 107, 113, 116, 119, 121, 126, 130, 132, 134
LiClOi 37, 108, 116
LLCOi 23, 85, 111, 115, 118, 121, 124, 129, 131, 134
LiF 2, 42, 109, 114, 117, 122, 126
LiH 36, 107, 113, 126, 130
Lil 19, 75, 111, 115, 118, 120, 124, 128, 131, 133
Li,Mo0 4 35,103,113,125,130LiNO, . 24, 86, 111, 121, 124, 129, 131, 134
LiNOs 25, 88, 111, 118, 121, 124, 129, 131, 134
Li2S0 4 32, 99, 112, 115, 118, 125, 130
MgBr. 15, 66, 110, 114, 117, 123, 128
MgCl, 6, 50, 109, 114, 117, 122, 126
MgF> 4, 44, 114
Mgl, 20, 78, 111, 115, 118, 124, 128
MnCl, 9, 55, 109, 114, 117, 122, 127
MnF> 4, 46, 109, 122, 126
MoO:i 29, 91, 112, 125, 129
NaBr 14, 64, 110, 114, 117, 120, 123, 127, 131, 133NaCl 4, 48, 109, 114, 117, 120, 122, 126, 131, 133
NaiCO.i 23, 85, 111, 115, 118, 121, 124, 129, 131, 134NaF 3, 42, 109, 114, 117, 122, 126Nal 19, 76, 111, 115, 118, 120, 124, 128, 131, 133Na2Mo0 4 35, 103, 113, 116, 119, 125, 130NaNO 24, 86, 111, 115, 118, 121, 124, 129, 131, 134NaNO :i 25, 88. Ill, 115, 118, 121, 124, 129, 131, 134NaOH 36, 105, 113, 116, 119, 121, 126, 130, 132, 134
NaP03 36,107,121,132,134NaSCN 35, 105, 113, 121, 126, 130, 132, 134Na2S0 4 32, 99, 112, 115, 118, 125, 130Na 2W0 4 35, 104, 113,116, 119, 126, 130NdBr
:s 16, 69, 110, 115, 117, 123, 128NdCl
: , 9, 53, 109, 122, 127Ndl3 21, 80, 111, 124, 128
NiS 31, 95, 112, 129
Page
PbBr, 18, 74, 110, 115, 118, 120, 123, 128, 131, 133
PbCl 13, 62, 110, 115, 118, 120, 123, 127, 131, 133
PbF, 4, 47, 109, 122, 126
Pbl, : 23, 84, 111, 124, 129
PbO 30, 94, 112, 125, 129
PbS 31, 97, 112, 115, 118, 125, 130
PrBr, 16,68,110,123,128PrCL 8, 53, 109, 122, 127
Prlj . 21, 80, 111, 124, 128
Pr4NBF4 33, 100, 112, 116, 118, 121, 125, 130, 132, 134
Pr4NBPh 4 33, 101, 116, 121, 132, 134
Pr4NPFH 33, 100, 112, 116, 118, 121, 125, 130, 132, 134
RbBr 15, 65, 110, 114, 117, 120, 123, 128, 131, 133
RbCl 6, 49, 109, 114, 117, 120, 122, 126, 131, 133
Rbl 20, 77, 111, 115, 118, 120, 124, 128, 131, 133
RbNO) 25, 87, 111, 121. 124, 129, 131. 133
RbNOs 27, 89, 112, 115, 118, 121, 124, 129, 131, 134
Rb,S0 4 32, 99, 112, 116, 118, 125, 130
Sb>Of 30, 94, 112, 125, 129
Sb)S t 31, 98, 112, 115, 118, 125, 130
ScCli 8, 51, 109, 122, 127
SiO, 29, 93, 121, 132, 134
SnCL 12, 61, 110, 114, 117, 123, 127
SnCl 4 13,62,114,120,131,133SnS 31, 97, 112, 115, 125. 130
SrBr2 15, 67, 110, 115, 117, 123, 128
SrCL 7, 51, 109, 114, 117, 120, 122, 127, 131, 133SrF., 4 45 114
Srl 2 . 20, 79, 111, 115, H8, 124, 128
TeCl2 13,63,110,123,127TeCL 13,63,110,123,127Te0 2 30, 95, 112, 125, 129
ThCl 4 9, 55, 109, 117, 122, 127
ThF4 4, 46, 114TiCl4 9, 55, 117, 120, 131, 133
TIBr 18, 73, 110, 115, 118, 123, 128T1C1 12,61,110,114,117,123,127Til 23, 84, 111, 124, 129
TINO3 28, 91, 112, 115, 118, 121, 125, 129, 132, 134
UC14 9, 55, 109, 122, 127
UF4 4, 46, 114
U0 2C1> 36,107,113,126,130U 203 29, 91, 112, 125, 129
YCl :t 8, 52, 109, 117, 122, 127
ZnBr2. 17, 70, 110, 115, 118, 120, 123, 128, 131, 133
ZnCl) 10, 57, 109, 110, 114, 117, 120, 122, 123, 127, 131, 133ZnF> 4, 47, 109, 122, 126
Znl 2 21, 81, 111, 118, 124, 128
139
National Standard Reference Data Series
National Bureau of Standards
National Standard Reference Data System, Plan of Operation, NSRDSNBS 1 —15 cents*
Thermal Properties of Aqueous Uniunivalent Electrolytes, NSRDSNBS 2 — 45 cents*
Selected Tables of Atomic Spectra, Atomic Energy Levels and Multiplet Tables — Si II,
Si ill, Si iv, NSRDSNBS 3, Section 1 — 35 cents*
Selected Tables of Atomic Spectra, Atomic Energy Levels and Multiplet Tables —Si I, NSRDSNBS 3, Section 2— 20 cents*
Atomic Transition Probabilities, Volume I, Hydrogen Through Neon, NSRDSNBS 4 —$2.50*
The Band Spectrum of Carbon Monoxide, NSRDSNBS 5 — 70 cents*
Tables of Molecular Vibrational Frequencies. Part 1, NSRDSNBS 6 — 40 cents*
High Temperature Properties and Decomposition of Inorganic Salts. Part 1. Sulfates,
NSRDSNBS 7 — 35 cents*
Thermal Conductivity of Selected Materials. NSRDSNBS 8— $1.00*
Tables of Biomolecular Gas Reactions. NSRDSNBS 9 — $2.00*
Selected Values of Electric Dipole Moments for Molecules in the Gas Phase. NSRDSNBS 10 — 40 cents*
Tables of Molecular Vibrational Frequencies, Part 2, NSRDSNBS 11 — 30 cents*
Tables for the Rigid Asymmetric Rotor: Transformation Coefficient for Symmetric to
Asymmetric Bases and Expectation Values of P^ and P^. NSRDSNBS 12 — 60
cents*
Hydrogenation of Ethylene on Metallic Catalysts. NSRDSNBS 13— $1.00*
XRay Wavelengths and XRay Atomic Energy Levels, NSRDSNBS 14— 40 cents*
*Send orders with remittance to: Superintendent of Documents, U.S. Government Printing Office,
Washington, D.C. 20402. Remittances from foreign countries should include an additional onefourth of the
purchase price for postage.
NATIONAL BUREAU OF STANDARDS
The National Bureau of Standards 1 was established by an act of Congress March 3,
1901. Today, in addition to serving as the Nation’s central measurement laboratory,
the Bureau is a principal focal point in the Federal Government for assuring maxi
mum application of the physical and engineering sciences to the advancement of tech
nology in industry and commerce. To this end the Bureau conducts research and
provides central national services in three broad program areas and provides cen
tral national services in a fourth. These are: (1) basic measurements and standards,
(2) materials measurements and standards, (3) technological measurements and
standards, and (4) transfer of technology.
The Bureau comprises the Institute for Basic Standards, the Institute for Materials
Research, the Institute for Applied Technology, and the Center for Radiation Research.
THE INSTITUTE FOR BASIC STANDARDS provides the central basis within the
United States of a complete and consistent system of physical measurement, coor
dinates that system with the measurement systems of other nations, and furnishes
essential services leading to accurate and uniform physical measurements throughout
the Nation’s scientific community, industry, and commerce. The Institute consists
of an Office of Standard Reference Data and a group of divisions organized by the
following areas of science and engineering
:
Applied Mathematics—Electricity—Metrology—Mechanics—Heat—Atomic Phys
ics—Cryogenics 2—Radio Physics 2—Radio Engineering2—Astrophysics 2—Time
and Frequency. 2
THE INSTITUTE FOR MATERIALS RESEARCH conducts materials research lead
ing to methods, standards of measurement, and data needed by industry, commerce,educational institutions, and government. The Institute also provides advisory andresearch services to other government agencies. The Institute consists of an Office of
Standard Reference Materials and a group of divisions organized by the following
areas of materials research:
Analytical Chemistry—Polymers—Metallurgy— Inorganic Materials— Physical
Chemistry.
THE INSTITUTE FOR APPLIED TECHNOLOGY provides for the creation of appro
priate opportunities for the use and application of technology within the Federal Gov
ernment and within the civilian sector of American industry. The primary functions
of the Institute may be broadly classified as programs relating to technological meas
urements and standards and techniques for the transfer of technology. The Institute
consists of a Clearinghouse for Scientific and Technical Information,3 a Center for
Computer Sciences and Technology, and a group of technical divisions and offices
organized by the following fields of technology:
Building Research—Electronic Instrumentation— Technical Analysis— Product
Evaluation—Invention and Innovation— Weights and Measures— Engineering
Standards—Vehicle Systems Research.
THE CENTER FOR RADIATION RESEARCH engages in research, measurement,and application of radiation to the solution of Bureau mission problems and the
problems of other agencies and institutions. The Center for Radiation Research con
sists of the following divisions:
Reactor Radiation—Linac Radiation—Applied Radiation—Nuclear Radiation.
1 Headquarters and Laboratories at Gaithersburg, Maryland, unless otherwise noted; mailing address Washington, D. C. 20234.2 Located at Boulder, Colorado 80302.3 Located at 5285 Port Royal Road, Springfield, Virginia 22151.
U S. GOVERNMENT PRINTING OFFICE : 1968 OL— 297268
4
